#------------------------------------------------------------------------------
#$Date: 2016-03-26 03:56:29 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180203 $
#$URL: svn://www.crystallography.net/cod/cif/7/10/97/7109707.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7109707
loop_
_publ_author_name
'Ze-Min Zhang'
'Lu-Yi Pan'
'Wei-Quan Lin'
'Ji-Dong Leng'
'Fu-Sheng Guo'
'Yan-Cong Chen'
'Jun-Liang Liu'
'Ming-Liang Tong'
_publ_section_title
;
 Wheel-shaped nanoscale 3d-4f {CoII16LnIII24} clusters (Ln = Dy and
 Gd)
;
_journal_name_full               Chem.Commun.
_journal_page_first              8081
_journal_paper_doi               10.1039/c3cc45075a
_journal_volume                  49
_journal_year                    2013
_chemical_formula_sum            'C228 H460 Co16 Gd26 N66 O302'
_chemical_formula_weight         13990.00
_chemical_name_systematic
;
?
;
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 123.109(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   29.3969(9)
_cell_length_b                   35.5750(6)
_cell_length_c                   24.9218(6)
_cell_measurement_reflns_used    13258
_cell_measurement_temperature    150(2)
_cell_measurement_theta_max      59.9357
_cell_measurement_theta_min      3.0081
_cell_volume                     21831.3(12)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.20
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.20
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.20
;
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      150(2)
_diffrn_detector_area_resol_mean 16.0855
_diffrn_measured_fraction_theta_full 0.988
_diffrn_measured_fraction_theta_max 0.988
_diffrn_measurement_device_type  'Xcalibur, Sapphire3, Gemini ultra'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  mirror
_diffrn_radiation_source         'Enhance Ultra (Cu) X-ray Source'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54178
_diffrn_reflns_av_R_equivalents  0.0705
_diffrn_reflns_av_sigmaI/netI    0.0792
_diffrn_reflns_limit_h_max       33
_diffrn_reflns_limit_h_min       -32
_diffrn_reflns_limit_k_max       39
_diffrn_reflns_limit_k_min       -39
_diffrn_reflns_limit_l_max       27
_diffrn_reflns_limit_l_min       -27
_diffrn_reflns_number            46551
_diffrn_reflns_theta_full        60.00
_diffrn_reflns_theta_max         60.00
_diffrn_reflns_theta_min         3.01
_exptl_absorpt_coefficient_mu    30.749
_exptl_absorpt_correction_T_max  0.0838
_exptl_absorpt_correction_T_min  0.0406
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.20
Empirical absorption correction using spherical harmonics,
implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            pink
_exptl_crystal_density_diffrn    2.128
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'irregular block'
_exptl_crystal_F_000             13604
_exptl_crystal_size_max          0.29
_exptl_crystal_size_mid          0.18
_exptl_crystal_size_min          0.16
_platon_squeeze_details
;
SQUEEZE removed 10 disordered hydroxyl ions, 54 disordered water molecules
and 20 disordered methanol molecules per formula unit. This value is
calculated based upon elemental analysis data.
;
_refine_diff_density_max         2.286
_refine_diff_density_min         -4.959
_refine_diff_density_rms         0.244
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.016
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1237
_refine_ls_number_reflns         16298
_refine_ls_number_restraints     1293
_refine_ls_restrained_S_all      1.009
_refine_ls_R_factor_all          0.0962
_refine_ls_R_factor_gt           0.0775
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1565P)²+200.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2199
_refine_ls_wR_factor_ref         0.2384
_reflns_number_gt                11886
_reflns_number_total             16298
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c3cc45075a.txt
_cod_data_source_block           cogd
_cod_original_sg_symbol_H-M      C2/m
_cod_database_code               7109707
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_group
Co1 Co 0.52386(6) 0.90781(4) 0.84640(7) 0.0396(4) Uani 1 1 d . .
Co2 Co 0.45377(5) 0.77482(4) 0.64663(6) 0.0323(4) Uani 1 1 d . .
Co3 Co 0.75273(6) 0.90729(4) 0.88639(7) 0.0385(4) Uani 1 1 d . .
Co4 Co 0.67486(5) 0.77993(4) 0.67315(6) 0.0295(4) Uani 1 1 d . .
Gd1 Gd 0.57740(4) 1.0000 0.91240(4) 0.0429(2) Uani 1 2 d SD .
Gd2 Gd 0.74507(4) 1.0000 0.94107(4) 0.0466(3) Uani 1 2 d S .
Gd3 Gd 0.62112(2) 0.943709(16) 0.81858(3) 0.03481(15) Uani 1 1 d . .
Gd4 Gd 0.52321(2) 0.860395(15) 0.72123(2) 0.03021(14) Uani 1 1 d . .
Gd5 Gd 0.65489(2) 0.862110(15) 0.74057(2) 0.03059(15) Uani 1 1 d . .
Gd6 Gd 0.537793(19) 0.805871(15) 0.59569(2) 0.02696(13) Uani 1 1 d . .
Gd7 Gd 0.58357(2) 0.743143(16) 0.51103(2) 0.03212(15) Uani 1 1 d . .
Gd8 Gd 0.61844(5) 1.0000 0.51793(6) 0.0733(4) Uani 1 2 d S .
N1 N 0.4396(3) 0.8993(2) 0.8168(4) 0.043(2) Uani 1 1 d . .
N2 N 0.5436(4) 0.8772(3) 0.9282(4) 0.060(3) Uani 1 1 d . .
N3 N 0.4777(3) 0.7260(2) 0.7091(4) 0.037(2) Uani 1 1 d . .
N4 N 0.3833(3) 0.7810(2) 0.6517(3) 0.032(2) Uani 1 1 d . .
N5 N 0.2445(3) 0.7916(2) 0.3064(4) 0.038(2) Uani 1 1 d . .
N6 N 0.8263(3) 0.8994(3) 0.8889(4) 0.049(3) Uani 1 1 d . .
N7 N 0.7896(4) 0.8743(3) 0.9726(4) 0.051(3) Uani 1 1 d . .
N8 N 0.7050(3) 0.7307(2) 0.7338(4) 0.038(2) Uani 1 1 d . .
N9 N 0.4110(4) 0.8878(3) 0.6501(5) 0.065(3) Uani 1 1 d . .
N10 N 0.5393(7) 0.8964(5) 0.6081(8) 0.0445(17) Uani 0.515(7) 1 d P 1
O27 O 0.5214(6) 0.8694(5) 0.5570(7) 0.0445(17) Uani 0.515(7) 1 d PU 1
O28 O 0.5433(6) 0.9400(4) 0.6063(7) 0.0445(17) Uani 0.515(7) 1 d PU 1
O1W O 0.5798(6) 0.9588(4) 0.7125(7) 0.039(3) Uani 0.515(7) 1 d PU 1
H1WA H 0.5980 0.9504 0.6979 0.046 Uiso 0.515(7) 1 d PR 1
H1WB H 0.5475 0.9504 0.6894 0.046 Uiso 0.515(7) 1 d PR 1
N10' N 0.5645(7) 0.9325(6) 0.6672(9) 0.0497(17) Uani 0.485(7) 1 d PU 2
O1W' O 0.5247(7) 0.8714(5) 0.5679(7) 0.034(3) Uani 0.485(7) 1 d PU 2
H1WC H 0.5044 0.8822 0.5777 0.040 Uiso 0.485(7) 1 d PR 2
H1WD H 0.5547 0.8832 0.5860 0.040 Uiso 0.485(7) 1 d PR 2
O28' O 0.5302(7) 0.9315(5) 0.5914(8) 0.0497(17) Uani 0.485(7) 1 d PU 2
O27' O 0.5810(8) 0.9670(5) 0.7083(9) 0.0497(17) Uani 0.485(7) 1 d PU 2
N11 N 0.7252(4) 0.8919(3) 0.7018(5) 0.063(3) Uani 1 1 d . .
N12 N 0.5000 0.7017(4) 0.5000 0.0578(14) Uani 1 2 d S .
N14 N 0.6660(5) 0.7962(4) 0.9477(6) 0.083(4) Uani 1 1 d . .
N15 N 0.5876(4) 0.6691(3) 0.7096(6) 0.070(3) Uani 1 1 d . .
N16 N 0.9131(3) 0.7501(3) 0.8799(5) 0.1338(18) Uani 0.515(7) 1 d PDU 1
O45 O 0.8606(4) 0.7301(6) 0.8521(12) 0.1338(18) Uani 0.515(7) 1 d PDU 1
N16' N 0.9044(3) 0.7458(3) 0.8748(5) 0.1338(18) Uani 0.485(7) 1 d PDU 2
O45' O 0.9533(5) 0.7688(6) 0.8958(14) 0.138(3) Uani 0.485(7) 1 d PDU 2
N17 N 0.7428(3) 1.0000 0.7496(9) 0.139(9) Uani 1 2 d SDU .
N18 N 0.4271(11) 1.0000 0.6949(14) 0.141(9) Uani 1 2 d SU .
O1 O 0.4960(3) 0.9618(2) 0.8514(3) 0.0435(17) Uani 1 1 d U .
O2 O 0.5325(3) 0.85235(19) 0.8245(3) 0.0369(15) Uani 1 1 d U .
O3 O 0.5042(2) 0.79627(18) 0.7391(3) 0.0348(14) Uani 1 1 d U .
O4 O 0.3857(2) 0.7738(2) 0.5488(3) 0.0371(16) Uani 1 1 d U .
O5 O 0.3316(2) 0.7759(2) 0.4170(3) 0.0368(17) Uani 1 1 d U .
O6 O 0.7864(3) 0.9617(2) 0.8984(3) 0.0489(18) Uani 1 1 d U .
O7 O 0.7247(3) 0.85309(19) 0.8531(3) 0.0392(17) Uani 1 1 d U .
O8 O 0.6954(3) 0.79872(19) 0.7640(3) 0.0382(16) Uani 1 1 d U .
O9 O 0.5972(3) 0.9363(2) 0.8965(3) 0.0447(16) Uani 1 1 d U .
H9B H 0.6095 0.9150 0.9138 0.054 Uiso 1 1 d R .
O10 O 0.5728(4) 1.0000 0.8151(4) 0.0393(18) Uani 1 2 d SU .
H10B H 0.5402 1.0000 0.7829 0.047 Uiso 1 2 d SR .
O11 O 0.5259(2) 0.91981(19) 0.7662(3) 0.0364(13) Uani 1 1 d U .
H11B H 0.5017 0.9352 0.7402 0.044 Uiso 1 1 d R .
O12 O 0.4724(2) 0.82698(19) 0.6227(3) 0.0344(13) Uani 1 1 d U .
H12 H 0.4450 0.8388 0.5929 0.041 Uiso 1 1 d R .
O13 O 0.4887(2) 0.75272(18) 0.6024(3) 0.0319(14) Uani 1 1 d U .
H13 H 0.5081 0.7334 0.6209 0.038 Uiso 1 1 d R .
O14 O 0.6680(4) 1.0000 0.9443(5) 0.051(2) Uani 1 2 d SU .
H14B H 0.6817 0.9784 0.9590 0.061 Uiso 0.50 1 d PR .
O15 O 0.6728(4) 1.0000 0.8319(4) 0.0403(19) Uani 1 2 d SU .
H15 H 0.6843 1.0000 0.8072 0.048 Uiso 1 2 d SR .
O16 O 0.7100(3) 0.9357(2) 0.9171(3) 0.0426(17) Uani 1 1 d U .
H16 H 0.7068 0.9150 0.9317 0.051 Uiso 1 1 d R .
O17 O 0.6877(3) 0.9206(2) 0.7939(3) 0.0406(14) Uani 1 1 d U .
H17B H 0.6954 0.9363 0.7744 0.049 Uiso 1 1 d R .
O18 O 0.6155(3) 0.87601(19) 0.8022(3) 0.0383(15) Uani 1 1 d U .
H18B H 0.6287 0.8633 0.8365 0.046 Uiso 1 1 d R .
O19 O 0.5814(2) 0.81817(19) 0.7079(3) 0.0377(15) Uani 1 1 d U .
H19B H 0.5999 0.8175 0.7486 0.045 Uiso 1 1 d R .
O20 O 0.6315(2) 0.83001(18) 0.6435(3) 0.0350(14) Uani 1 1 d U .
H20B H 0.6361 0.8430 0.6182 0.042 Uiso 1 1 d R .
O21 O 0.6000(2) 0.75429(18) 0.6175(3) 0.0314(14) Uani 1 1 d U .
H21B H 0.5957 0.7351 0.6345 0.038 Uiso 1 1 d R .
O22 O 0.5491(2) 0.80272(18) 0.5065(3) 0.0320(14) Uani 1 1 d U .
H22B H 0.5766 0.8166 0.5301 0.038 Uiso 1 1 d R .
O23 O 0.4281(3) 0.8638(2) 0.6938(3) 0.0449(16) Uani 1 1 d U .
O24 O 0.4442(3) 0.9016(2) 0.6369(3) 0.0485(18) Uani 1 1 d U .
O25 O 0.3619(4) 0.8990(4) 0.6193(6) 0.101(4) Uani 1 1 d U .
O26 O 0.5674(3) 0.8933(2) 0.6762(3) 0.0398(14) Uani 1 1 d U .
O29 O 0.6761(3) 0.9048(2) 0.6733(3) 0.0517(18) Uani 1 1 d U .
O30 O 0.7412(3) 0.8693(2) 0.7455(3) 0.0466(17) Uani 1 1 d U .
O31 O 0.7550(4) 0.9011(4) 0.6811(5) 0.096(3) Uani 1 1 d U .
O32 O 0.5000 0.7343(3) 0.5000 0.0578(14) Uani 1 2 d SU .
O33 O 0.5421(3) 0.6844(2) 0.5056(4) 0.0578(14) Uani 1 1 d U .
N13 N 0.6489(3) 0.6822(2) 0.5085(4) 0.090(3) Uani 0.515(7) 1 d PDU 1
O34 O 0.6525(5) 0.6921(4) 0.5609(5) 0.062(3) Uani 0.515(7) 1 d PDU 1
O35 O 0.6222(5) 0.6989(4) 0.4644(5) 0.058(2) Uani 0.515(7) 1 d PDU 1
O36 O 0.6714(6) 0.6520(3) 0.5171(7) 0.079(4) Uani 0.515(7) 1 d PDU 1
N13' N 0.6489(3) 0.6822(2) 0.5085(4) 0.090(3) Uani 0.485(7) 1 d PDU 2
O34' O 0.6658(6) 0.7021(4) 0.5515(5) 0.066(3) Uani 0.485(7) 1 d PDU 2
O35' O 0.6011(4) 0.6881(5) 0.4608(6) 0.058(3) Uani 0.485(7) 1 d PDU 2
O36' O 0.6758(4) 0.6660(5) 0.4910(7) 0.070(3) Uani 0.485(7) 1 d PDU 2
O37 O 0.6784(5) 0.7964(4) 1.0030(6) 0.111(4) Uani 1 1 d U .
O38 O 0.6587(5) 0.7654(3) 0.9193(5) 0.096(4) Uani 1 1 d U .
O39 O 0.6576(4) 0.8272(3) 0.9187(5) 0.081(3) Uani 1 1 d U .
O40 O 0.5684(3) 0.6925(3) 0.6656(4) 0.067(2) Uani 1 1 d U .
O41 O 0.6121(4) 0.6795(3) 0.7672(4) 0.074(3) Uani 1 1 d U .
O42 O 0.5835(5) 0.6338(4) 0.6974(6) 0.106(4) Uani 1 1 d U .
O43 O 0.9260(4) 0.7281(3) 0.8533(5) 0.1338(18) Uani 1 1 d DU .
O44 O 0.8899(4) 0.7665(4) 0.9014(5) 0.1338(18) Uani 1 1 d DU .
O46 O 0.6970(4) 1.0000 0.7388(6) 0.083(4) Uani 1 2 d SDU .
O47 O 0.7672(4) 0.9706(3) 0.7565(7) 0.131(5) Uani 1 1 d DU .
O48 O 0.4706(5) 1.0000 0.6988(6) 0.076(4) Uani 1 2 d SU .
O49 O 0.4041(6) 1.0324(4) 0.6957(8) 0.144(6) Uani 1 1 d U .
C1 C 0.4132(5) 0.8665(4) 0.8040(6) 0.060(3) Uani 1 1 d U .
H1 H 0.4303 0.8445 0.8017 0.072 Uiso 1 1 calc R .
C2 C 0.3627(5) 0.8631(4) 0.7941(7) 0.071(4) Uani 1 1 d U .
H2 H 0.3456 0.8394 0.7881 0.085 Uiso 1 1 calc R .
C3 C 0.3379(6) 0.8969(4) 0.7936(8) 0.087(5) Uani 1 1 d . .
H3 H 0.3021 0.8964 0.7845 0.105 Uiso 1 1 calc R .
C4 C 0.3633(5) 0.9297(4) 0.8053(7) 0.074(5) Uani 1 1 d . .
H4 H 0.3465 0.9523 0.8062 0.088 Uiso 1 1 calc R .
C5 C 0.4124(4) 0.9301(3) 0.8158(5) 0.051(3) Uani 1 1 d . .
C6 C 0.4455(4) 0.9673(4) 0.8302(5) 0.051(3) Uani 1 1 d . .
C7 C 0.4222(6) 1.0000 0.8234(10) 0.064(6) Uani 1 2 d S .
H7 H 0.3859 1.0000 0.8128 0.077 Uiso 1 2 calc SR .
C8 C 0.5548(6) 0.8932(4) 0.9847(6) 0.072(4) Uani 1 1 d . .
H8 H 0.5521 0.9197 0.9869 0.087 Uiso 1 1 calc R .
C9 C 0.5696(7) 0.8723(5) 1.0367(8) 0.096(5) Uani 1 1 d U .
H9 H 0.5770 0.8837 1.0752 0.115 Uiso 1 1 calc R .
C10 C 0.5735(8) 0.8346(5) 1.0329(9) 0.100(5) Uani 1 1 d U .
H10 H 0.5866 0.8198 1.0703 0.120 Uiso 1 1 calc R .
C11 C 0.5590(6) 0.8169(5) 0.9756(7) 0.082(4) Uani 1 1 d U .
H11 H 0.5582 0.7903 0.9720 0.098 Uiso 1 1 calc R .
C12 C 0.5460(5) 0.8401(4) 0.9242(5) 0.054(3) Uani 1 1 d . .
C13 C 0.5372(4) 0.8263(3) 0.8636(4) 0.041(3) Uani 1 1 d . .
C14 C 0.5307(5) 0.7880(3) 0.8462(5) 0.048(3) Uani 1 1 d . .
H14 H 0.5380 0.7698 0.8778 0.058 Uiso 1 1 calc R .
C15 C 0.5146(4) 0.7759(3) 0.7867(5) 0.039(3) Uani 1 1 d . .
C16 C 0.5044(4) 0.7343(3) 0.7702(5) 0.042(3) Uani 1 1 d . .
C17 C 0.5237(5) 0.7062(3) 0.8190(6) 0.055(3) Uani 1 1 d . .
H17 H 0.5423 0.7129 0.8630 0.066 Uiso 1 1 calc R .
C18 C 0.5142(5) 0.6693(4) 0.7999(6) 0.062(4) Uani 1 1 d . .
H18 H 0.5272 0.6497 0.8307 0.074 Uiso 1 1 calc R .
C19 C 0.4856(4) 0.6610(4) 0.7354(7) 0.062(3) Uani 1 1 d . .
H19 H 0.4775 0.6356 0.7215 0.074 Uiso 1 1 calc R .
C20 C 0.4687(4) 0.6896(3) 0.6908(5) 0.040(3) Uani 1 1 d . .
H20 H 0.4504 0.6835 0.6466 0.048 Uiso 1 1 calc R .
C21 C 0.3815(4) 0.7798(3) 0.7032(5) 0.041(3) Uani 1 1 d . .
H21 H 0.4141 0.7740 0.7428 0.049 Uiso 1 1 calc R .
C22 C 0.3368(4) 0.7862(4) 0.7035(5) 0.054(3) Uani 1 1 d . .
H22 H 0.3382 0.7844 0.7424 0.064 Uiso 1 1 calc R .
C23 C 0.2890(5) 0.7954(5) 0.6477(6) 0.067(4) Uani 1 1 d . .
H23 H 0.2574 0.8010 0.6475 0.081 Uiso 1 1 calc R .
C24 C 0.2881(4) 0.7961(4) 0.5916(6) 0.062(4) Uani 1 1 d . .
H24 H 0.2559 0.8022 0.5517 0.074 Uiso 1 1 calc R .
C25 C 0.3369(4) 0.7875(3) 0.5960(5) 0.042(3) Uani 1 1 d . .
C26 C 0.3387(4) 0.7844(3) 0.5364(5) 0.043(3) Uani 1 1 d . .
C27 C 0.2949(4) 0.7917(4) 0.4784(5) 0.053(4) Uani 1 1 d . .
H27 H 0.2627 0.7997 0.4754 0.064 Uiso 1 1 calc R .
C28 C 0.2939(4) 0.7883(3) 0.4219(5) 0.038(3) Uani 1 1 d . .
C29 C 0.2423(4) 0.7980(3) 0.3584(5) 0.040(3) Uani 1 1 d . .
C30 C 0.1950(5) 0.8116(4) 0.3518(6) 0.061(4) Uani 1 1 d . .
H30 H 0.1950 0.8176 0.3890 0.074 Uiso 1 1 calc R .
C31 C 0.1483(5) 0.8166(4) 0.2924(6) 0.061(4) Uani 1 1 d . .
H31 H 0.1154 0.8251 0.2870 0.074 Uiso 1 1 calc R .
C32 C 0.1524(5) 0.8083(4) 0.2414(6) 0.060(4) Uani 1 1 d . .
H32 H 0.1213 0.8109 0.1992 0.072 Uiso 1 1 calc R .
C33 C 0.2007(4) 0.7962(3) 0.2498(5) 0.040(3) Uani 1 1 d . .
H33 H 0.2018 0.7910 0.2131 0.048 Uiso 1 1 calc R .
C34 C 0.8489(5) 0.8641(4) 0.8907(6) 0.060(4) Uani 1 1 d . .
H34 H 0.8297 0.8418 0.8870 0.072 Uiso 1 1 calc R .
C35 C 0.8965(5) 0.8620(4) 0.8973(8) 0.079(2) Uani 1 1 d . .
H35 H 0.9116 0.8379 0.8999 0.095 Uiso 1 1 calc R .
C36 C 0.9250(5) 0.8934(4) 0.9004(8) 0.079(2) Uani 1 1 d . .
H36 H 0.9586 0.8918 0.9035 0.095 Uiso 1 1 calc R .
C37 C 0.9012(5) 0.9283(4) 0.8987(8) 0.079(2) Uani 1 1 d . .
H37 H 0.9199 0.9510 0.9029 0.095 Uiso 1 1 calc R .
C38 C 0.8522(5) 0.9296(4) 0.8913(8) 0.079(2) Uani 1 1 d . .
C39 C 0.8264(5) 0.9656(4) 0.8939(5) 0.054(3) Uani 1 1 d . .
C40 C 0.8494(7) 1.0000 0.8932(10) 0.064(6) Uani 1 2 d S .
H40 H 0.8813 1.0000 0.8921 0.076 Uiso 1 2 calc SR .
C41 C 0.8166(5) 0.8860(4) 1.0352(6) 0.058(4) Uani 1 1 d . .
H41 H 0.8227 0.9122 1.0437 0.070 Uiso 1 1 calc R .
C42 C 0.8342(6) 0.8630(4) 1.0838(5) 0.067(5) Uani 1 1 d . .
H42 H 0.8551 0.8724 1.1263 0.080 Uiso 1 1 calc R .
C43 C 0.8226(6) 0.8249(4) 1.0732(6) 0.069(5) Uani 1 1 d . .
H43 H 0.8336 0.8085 1.1083 0.083 Uiso 1 1 calc R .
C44 C 0.7950(5) 0.8110(3) 1.0118(5) 0.060(4) Uani 1 1 d . .
H44 H 0.7868 0.7850 1.0035 0.072 Uiso 1 1 calc R .
C45 C 0.7794(4) 0.8365(3) 0.9619(5) 0.047(3) Uani 1 1 d . .
C46 C 0.7471(4) 0.8255(3) 0.8934(5) 0.046(3) Uani 1 1 d . .
C47 C 0.7456(4) 0.7885(3) 0.8737(5) 0.042(3) Uani 1 1 d . .
H47 H 0.7631 0.7700 0.9063 0.051 Uiso 1 1 calc R .
C48 C 0.7209(3) 0.7764(3) 0.8112(4) 0.029(2) Uani 1 1 d . .
C49 C 0.7251(4) 0.7373(3) 0.7954(4) 0.034(3) Uani 1 1 d . .
C50 C 0.7480(4) 0.7084(3) 0.8403(5) 0.049(3) Uani 1 1 d . .
H50 H 0.7646 0.7138 0.8846 0.058 Uiso 1 1 calc R .
C51 C 0.7466(5) 0.6725(3) 0.8211(6) 0.054(4) Uani 1 1 d . .
H51 H 0.7611 0.6525 0.8512 0.065 Uiso 1 1 calc R .
C52 C 0.7232(4) 0.6657(3) 0.7559(6) 0.051(3) Uani 1 1 d . .
H52 H 0.7210 0.6409 0.7406 0.061 Uiso 1 1 calc R .
C53 C 0.7038(4) 0.6955(3) 0.7146(5) 0.038(3) Uani 1 1 d . .
H53 H 0.6888 0.6909 0.6704 0.045 Uiso 1 1 calc R .
O2W O 0.6885(6) 0.9608(4) 0.5929(7) 0.137(5) Uani 1 1 d U .
H2WA H 0.7173 0.9643 0.6296 0.165 Uiso 1 1 d R .
H2WB H 0.6858 0.9375 0.5842 0.165 Uiso 1 1 d R .
O3W O 0.6384(6) 0.9587(4) 0.4584(7) 0.129(5) Uani 1 1 d U .
H3WB H 0.6057 0.9567 0.4481 0.154 Uiso 1 1 d R .
H3WA H 0.6453 0.9427 0.4385 0.154 Uiso 1 1 d R .
O4W O 0.6093(7) 1.0000 0.6067(8) 0.105(4) Uani 1 2 d SU .
H4WA H 0.5880 0.9829 0.6043 0.126 Uiso 0.50 1 d PR .
H4WB H 0.6364 1.0000 0.6450 0.126 Uiso 1 2 d SR .
O5W O 0.5695(5) 0.9438(4) 0.5101(6) 0.107(4) Uani 1 1 d U .
H5WA H 0.5976 0.9345 0.5430 0.128 Uiso 1 1 d R .
H5WB H 0.5442 0.9487 0.5159 0.128 Uiso 1 1 d R .
O6W O 0.5337(7) 1.0000 0.4186(9) 0.132(7) Uani 1 2 d SU .
H6W H 0.5285 1.0194 0.3959 0.158 Uiso 1 1 d R .
O7W O 0.6157(3) 0.7574(3) 0.7886(4) 0.068(2) Uani 1 1 d U .
H7WA H 0.6288 0.7605 0.8283 0.082 Uiso 1 1 d R .
H7WB H 0.6143 0.7340 0.7812 0.082 Uiso 1 1 d R .
O8W O 1.0000 0.7851(2) 1.0000 0.164(5) Uani 1 2 d SU .
H8WA H 1.0151 0.7734 1.0354 0.197 Uiso 0.50 1 d PR .
H8WB H 0.9692 0.7751 0.9742 0.197 Uiso 0.50 1 d PR .
O9W O 0.5338 0.9875(2) 0.9796 0.066(3) Uani 0.50 1 d PRU .
O10W O 0.6568 0.9875(2) 1.0156 0.072(3) Uani 0.50 1 d PRDU .
O11W O 0.7542 1.0129(2) 1.0398 0.073(3) Uani 0.50 1 d PRU .
O12W O 0.8438 0.9875(2) 1.0334 0.072(3) Uani 0.50 1 d PRU .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0181 0.0091 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0311 0.0180 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0492 0.0322 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co -2.3653 3.6143 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Gd Gd -8.8380 11.9157 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O9 Co1 O11 84.9(3) . .
O9 Co1 N2 91.4(3) . .
O11 Co1 N2 154.9(4) . .
O9 Co1 O2 112.5(3) . .
O11 Co1 O2 82.7(3) . .
N2 Co1 O2 75.9(4) . .
O9 Co1 O1 80.2(3) . .
O11 Co1 O1 94.9(3) . .
N2 Co1 O1 109.0(4) . .
O2 Co1 O1 166.7(3) . .
O9 Co1 N1 152.3(3) . .
O11 Co1 N1 109.1(3) . .
N2 Co1 N1 85.2(4) . .
O2 Co1 N1 93.3(3) . .
O1 Co1 N1 75.0(3) . .
O9 Co1 Gd3 41.7(2) . .
O11 Co1 Gd3 44.25(17) . .
N2 Co1 Gd3 123.8(3) . .
O2 Co1 Gd3 93.7(2) . .
O1 Co1 Gd3 93.7(2) . .
N1 Co1 Gd3 151.0(2) . .
O9 Co1 Gd4 105.5(2) . .
O11 Co1 Gd4 40.37(19) . .
N2 Co1 Gd4 118.4(3) . .
O2 Co1 Gd4 42.78(19) . .
O1 Co1 Gd4 131.9(2) . .
N1 Co1 Gd4 100.2(2) . .
Gd3 Co1 Gd4 67.29(4) . .
O13 Co2 O3 118.4(3) . .
O13 Co2 O12 84.3(3) . .
O3 Co2 O12 81.6(3) . .
O13 Co2 O4 79.2(3) . .
O3 Co2 O4 156.7(3) . .
O12 Co2 O4 85.4(3) . .
O13 Co2 N4 149.2(3) . .
O3 Co2 N4 91.4(3) . .
O12 Co2 N4 109.4(3) . .
O4 Co2 N4 74.8(3) . .
O13 Co2 N3 91.0(3) . .
O3 Co2 N3 75.2(3) . .
O12 Co2 N3 150.6(3) . .
O4 Co2 N3 122.3(3) . .
N4 Co2 N3 89.2(3) . .
O13 Co2 Gd6 42.46(19) . .
O3 Co2 Gd6 93.9(2) . .
O12 Co2 Gd6 43.97(19) . .
O4 Co2 Gd6 89.9(2) . .
N4 Co2 Gd6 151.2(2) . .
N3 Co2 Gd6 119.5(2) . .
O16 Co3 O7 114.5(3) . .
O16 Co3 O17 85.6(3) . .
O7 Co3 O17 81.1(3) . .
O16 Co3 O6 80.3(3) . .
O7 Co3 O6 162.6(3) . .
O17 Co3 O6 91.4(3) . .
O16 Co3 N6 149.7(3) . .
O7 Co3 N6 93.6(3) . .
O17 Co3 N6 111.2(3) . .
O6 Co3 N6 74.4(3) . .
O16 Co3 N7 88.5(4) . .
O7 Co3 N7 76.5(3) . .
O17 Co3 N7 152.0(3) . .
O6 Co3 N7 114.6(3) . .
N6 Co3 N7 87.0(4) . .
O16 Co3 Gd3 42.50(17) . .
O7 Co3 Gd3 93.32(19) . .
O17 Co3 Gd3 44.3(2) . .
O6 Co3 Gd3 92.1(2) . .
N6 Co3 Gd3 152.7(3) . .
N7 Co3 Gd3 120.2(3) . .
O21 Co4 O20 85.3(2) . .
O21 Co4 O8 115.9(3) . .
O20 Co4 O8 82.5(3) . .
O21 Co4 O5 79.3(3) . 2_656
O20 Co4 O5 89.9(3) . 2_656
O8 Co4 O5 162.2(3) . 2_656
O21 Co4 N8 89.5(3) . .
O20 Co4 N8 151.7(3) . .
O8 Co4 N8 74.8(3) . .
O5 Co4 N8 116.4(3) 2_656 .
O21 Co4 N5 150.1(3) . 2_656
O20 Co4 N5 107.3(3) . 2_656
O8 Co4 N5 92.9(3) . 2_656
O5 Co4 N5 73.9(3) 2_656 2_656
N8 Co4 N5 90.8(3) . 2_656
O21 Co4 Gd6 42.65(18) . .
O20 Co4 Gd6 44.10(18) . .
O8 Co4 Gd6 94.41(19) . .
O5 Co4 Gd6 91.30(17) 2_656 .
N8 Co4 Gd6 120.4(2) . .
N5 Co4 Gd6 148.8(2) 2_656 .
O14 Gd1 O10 76.3(4) . .
O14 Gd1 O10W 50.9(3) . 6_575
O10 Gd1 O10W 125.6(2) . 6_575
O14 Gd1 O10W 50.9(3) . .
O10 Gd1 O10W 125.6(2) . .
O10W Gd1 O10W 21.5(4) 6_575 .
O14 Gd1 O9 73.98(19) . .
O10 Gd1 O9 73.49(19) . .
O10W Gd1 O9 99.8(2) 6_575 .
O10W Gd1 O9 79.7(2) . .
O14 Gd1 O9 73.98(19) . 6_575
O10 Gd1 O9 73.49(19) . 6_575
O10W Gd1 O9 79.7(2) 6_575 6_575
O10W Gd1 O9 99.8(2) . 6_575
O9 Gd1 O9 138.3(4) . 6_575
O14 Gd1 O1 140.0(2) . .
O10 Gd1 O1 82.7(3) . .
O10W Gd1 O1 145.8(2) 6_575 .
O10W Gd1 O1 128.2(2) . .
O9 Gd1 O1 67.5(2) . .
O9 Gd1 O1 131.4(2) 6_575 .
O14 Gd1 O1 140.0(2) . 6_575
O10 Gd1 O1 82.7(3) . 6_575
O10W Gd1 O1 128.2(2) 6_575 6_575
O10W Gd1 O1 145.8(2) . 6_575
O9 Gd1 O1 131.4(2) . 6_575
O9 Gd1 O1 67.5(2) 6_575 6_575
O1 Gd1 O1 68.0(3) . 6_575
O14 Gd1 O9W 130.1(3) . 6_575
O10 Gd1 O9W 151.4(2) . 6_575
O10W Gd1 O9W 79.20(6) 6_575 6_575
O10W Gd1 O9W 82.84(8) . 6_575
O9 Gd1 O9W 120.2(3) . 6_575
O9 Gd1 O9W 100.9(3) 6_575 6_575
O1 Gd1 O9W 80.7(2) . 6_575
O1 Gd1 O9W 69.5(2) 6_575 6_575
O14 Gd1 O9W 130.1(3) . .
O10 Gd1 O9W 151.4(2) . .
O10W Gd1 O9W 82.84(8) 6_575 .
O10W Gd1 O9W 79.20(6) . .
O9 Gd1 O9W 100.9(3) . .
O9 Gd1 O9W 120.2(3) 6_575 .
O1 Gd1 O9W 69.5(2) . .
O1 Gd1 O9W 80.7(2) 6_575 .
O9W Gd1 O9W 19.4(3) 6_575 .
O14 Gd1 Gd3 60.1(2) . .
O10 Gd1 Gd3 38.17(12) . .
O10W Gd1 Gd3 107.56(10) 6_575 .
O10W Gd1 Gd3 96.02(10) . .
O9 Gd1 Gd3 38.2(2) . .
O9 Gd1 Gd3 101.6(2) 6_575 .
O1 Gd1 Gd3 82.44(19) . .
O1 Gd1 Gd3 117.26(18) 6_575 .
O9W Gd1 Gd3 157.41(16) 6_575 .
O9W Gd1 Gd3 138.21(16) . .
O14 Gd1 Gd3 60.1(2) . 6_575
O10 Gd1 Gd3 38.17(12) . 6_575
O10W Gd1 Gd3 96.02(10) 6_575 6_575
O10W Gd1 Gd3 107.56(10) . 6_575
O9 Gd1 Gd3 101.6(2) . 6_575
O9 Gd1 Gd3 38.2(2) 6_575 6_575
O1 Gd1 Gd3 117.26(18) . 6_575
O1 Gd1 Gd3 82.44(19) 6_575 6_575
O9W Gd1 Gd3 138.21(16) 6_575 6_575
O9W Gd1 Gd3 157.41(16) . 6_575
Gd3 Gd1 Gd3 63.67(3) . 6_575
O14 Gd2 O15 76.0(4) . .
O14 Gd2 O11W 61.3(3) . 6_575
O15 Gd2 O11W 135.6(3) . 6_575
O14 Gd2 O11W 61.3(3) . .
O15 Gd2 O11W 135.6(3) . .
O11W Gd2 O11W 22.3(4) 6_575 .
O14 Gd2 O6 138.7(2) . .
O15 Gd2 O6 81.2(3) . .
O11W Gd2 O6 123.2(2) 6_575 .
O11W Gd2 O6 139.9(2) . .
O14 Gd2 O6 138.7(2) . 6_575
O15 Gd2 O6 81.2(3) . 6_575
O11W Gd2 O6 139.9(2) 6_575 6_575
O11W Gd2 O6 123.2(2) . 6_575
O6 Gd2 O6 68.4(4) . 6_575
O14 Gd2 O16 73.6(2) . .
O15 Gd2 O16 74.03(16) . .
O11W Gd2 O16 82.3(3) 6_575 .
O11W Gd2 O16 103.2(3) . .
O6 Gd2 O16 67.2(3) . .
O6 Gd2 O16 131.6(3) 6_575 .
O14 Gd2 O16 73.6(2) . 6_575
O15 Gd2 O16 74.03(16) . 6_575
O11W Gd2 O16 103.2(3) 6_575 6_575
O11W Gd2 O16 82.3(2) . 6_575
O6 Gd2 O16 131.6(3) . 6_575
O6 Gd2 O16 67.2(3) 6_575 6_575
O16 Gd2 O16 138.6(3) . 6_575
O14 Gd2 O12W 128.1(3) . 6_575
O15 Gd2 O12W 153.4(3) . 6_575
O11W Gd2 O12W 70.9 6_575 6_575
O11W Gd2 O12W 66.8 . 6_575
O6 Gd2 O12W 84.16(19) . 6_575
O6 Gd2 O12W 72.77(18) 6_575 6_575
O16 Gd2 O12W 120.0(2) . 6_575
O16 Gd2 O12W 100.1(2) 6_575 6_575
O14 Gd2 O12W 128.1(3) . .
O15 Gd2 O12W 153.4(3) . .
O11W Gd2 O12W 66.8 6_575 .
O11W Gd2 O12W 70.9 . .
O6 Gd2 O12W 72.77(18) . .
O6 Gd2 O12W 84.16(19) 6_575 .
O16 Gd2 O12W 100.1(2) . .
O16 Gd2 O12W 120.0(2) 6_575 .
O12W Gd2 O12W 19.9(3) 6_575 .
O14 Gd2 Gd3 60.0(2) . .
O15 Gd2 Gd3 37.99(15) . .
O11W Gd2 Gd3 104.29(11) 6_575 .
O11W Gd2 Gd3 116.79(10) . .
O6 Gd2 Gd3 80.91(17) . .
O6 Gd2 Gd3 115.72(17) 6_575 .
O16 Gd2 Gd3 38.71(14) . .
O16 Gd2 Gd3 101.82(15) 6_575 .
O12W Gd2 Gd3 158.03(17) 6_575 .
O12W Gd2 Gd3 138.16(17) . .
O14 Gd2 Gd3 60.0(2) . 6_575
O15 Gd2 Gd3 37.99(15) . 6_575
O11W Gd2 Gd3 116.79(10) 6_575 6_575
O11W Gd2 Gd3 104.29(11) . 6_575
O6 Gd2 Gd3 115.72(16) . 6_575
O6 Gd2 Gd3 80.91(17) 6_575 6_575
O16 Gd2 Gd3 101.82(15) . 6_575
O16 Gd2 Gd3 38.71(15) 6_575 6_575
O12W Gd2 Gd3 138.16(17) 6_575 6_575
O12W Gd2 Gd3 158.03(17) . 6_575
Gd3 Gd2 Gd3 63.57(2) . 6_575
O14 Gd2 H14B 21.4 . .
O15 Gd2 H14B 84.7 . .
O11W Gd2 H14B 51.0 6_575 .
O11W Gd2 H14B 60.1 . .
O6 Gd2 H14B 123.9 . .
O6 Gd2 H14B 159.5 6_575 .
O16 Gd2 H14B 56.7 . .
O16 Gd2 H14B 94.7 6_575 .
O12W Gd2 H14B 121.9 6_575 .
O12W Gd2 H14B 114.3 . .
Gd3 Gd2 H14B 56.7 . .
Gd3 Gd2 H14B 78.8 6_575 .
O1W Gd3 O9 138.6(5) . .
O1W Gd3 O15 82.1(4) . .
O9 Gd3 O15 114.6(3) . .
O1W Gd3 O10 80.5(5) . .
O9 Gd3 O10 72.4(3) . .
O15 Gd3 O10 68.5(3) . .
O1W Gd3 O18 95.4(4) . .
O9 Gd3 O18 90.2(3) . .
O15 Gd3 O18 145.2(3) . .
O10 Gd3 O18 145.6(3) . .
O1W Gd3 O16 142.4(5) . .
O9 Gd3 O16 78.4(3) . .
O15 Gd3 O16 73.2(3) . .
O10 Gd3 O16 114.6(3) . .
O18 Gd3 O16 89.5(2) . .
O1W Gd3 O27' 6.4(6) . .
O9 Gd3 O27' 139.5(6) . .
O15 Gd3 O27' 76.0(5) . .
O10 Gd3 O27' 76.7(6) . .
O18 Gd3 O27' 101.4(5) . .
O16 Gd3 O27' 139.4(6) . .
O1W Gd3 O17 77.6(5) . .
O9 Gd3 O17 140.9(2) . .
O15 Gd3 O17 77.8(3) . .
O10 Gd3 O17 141.9(3) . .
O18 Gd3 O17 67.8(2) . .
O16 Gd3 O17 69.9(2) . .
O27' Gd3 O17 78.3(6) . .
O1W Gd3 O11 74.9(4) . .
O9 Gd3 O11 69.4(2) . .
O15 Gd3 O11 142.2(2) . .
O10 Gd3 O11 78.2(2) . .
O18 Gd3 O11 67.8(2) . .
O16 Gd3 O11 139.9(2) . .
O27' Gd3 O11 79.3(5) . .
O17 Gd3 O11 124.3(2) . .
O1W Gd3 Co3 113.1(4) . .
O9 Gd3 Co3 107.50(16) . .
O15 Gd3 Co3 78.24(19) . .
O10 Gd3 Co3 142.14(19) . .
O18 Gd3 Co3 70.88(16) . .
O16 Gd3 Co3 34.85(19) . .
O27' Gd3 Co3 112.9(6) . .
O17 Gd3 Co3 35.91(14) . .
O11 Gd3 Co3 138.48(16) . .
O1W Gd3 Co1 109.6(4) . .
O9 Gd3 Co1 34.82(16) . .
O15 Gd3 Co1 141.8(2) . .
O10 Gd3 Co1 77.6(2) . .
O18 Gd3 Co1 71.72(19) . .
O16 Gd3 Co1 107.3(2) . .
O27' Gd3 Co1 113.3(5) . .
O17 Gd3 Co1 139.41(17) . .
O11 Gd3 Co1 35.40(16) . .
Co3 Gd3 Co1 124.69(4) . .
O1W Gd3 Gd1 116.3(4) . .
O9 Gd3 Gd1 38.44(17) . .
O15 Gd3 Gd1 82.9(3) . .
O10 Gd3 Gd1 36.8(2) . .
O18 Gd3 Gd1 127.62(19) . .
O16 Gd3 Gd1 88.74(19) . .
O27' Gd3 Gd1 113.1(5) . .
O17 Gd3 Gd1 154.51(15) . .
O11 Gd3 Gd1 80.94(16) . .
Co3 Gd3 Gd1 123.52(3) . .
Co1 Gd3 Gd1 59.11(3) . .
O11 Gd4 O12 140.5(2) . .
O11 Gd4 O18 70.5(2) . .
O12 Gd4 O18 140.1(2) . .
O11 Gd4 O19 140.3(2) . .
O12 Gd4 O19 69.1(2) . .
O18 Gd4 O19 72.6(2) . .
O11 Gd4 O26 84.3(2) . .
O12 Gd4 O26 87.5(2) . .
O18 Gd4 O26 68.5(2) . .
O19 Gd4 O26 69.0(2) . .
O11 Gd4 O3 134.2(2) . .
O12 Gd4 O3 69.2(2) . .
O18 Gd4 O3 109.2(2) . .
O19 Gd4 O3 72.3(2) . .
O26 Gd4 O3 139.9(2) . .
O11 Gd4 O2 69.7(2) . .
O12 Gd4 O2 132.2(2) . .
O18 Gd4 O2 73.6(2) . .
O19 Gd4 O2 112.8(2) . .
O26 Gd4 O2 139.4(2) . .
O3 Gd4 O2 66.8(2) . .
O11 Gd4 O23 80.2(2) . .
O12 Gd4 O23 76.3(2) . .
O18 Gd4 O23 143.4(3) . .
O19 Gd4 O23 139.5(2) . .
O26 Gd4 O23 130.7(2) . .
O3 Gd4 O23 76.3(2) . .
O2 Gd4 O23 76.0(2) . .
O11 Gd4 O24 70.2(2) . .
O12 Gd4 O24 70.4(2) . .
O18 Gd4 O24 131.0(2) . .
O19 Gd4 O24 128.9(2) . .
O26 Gd4 O24 79.7(2) . .
O3 Gd4 O24 119.1(2) . .
O2 Gd4 O24 117.2(3) . .
O23 Gd4 O24 51.1(3) . .
O11 Gd4 N9 74.1(3) . .
O12 Gd4 N9 71.1(3) . .
O18 Gd4 N9 144.4(3) . .
O19 Gd4 N9 140.0(3) . .
O26 Gd4 N9 105.6(3) . .
O3 Gd4 N9 97.3(3) . .
O2 Gd4 N9 96.7(3) . .
O23 Gd4 N9 25.1(3) . .
O24 Gd4 N9 26.0(3) . .
O11 Gd4 Co1 34.57(17) . .
O12 Gd4 Co1 147.73(17) . .
O18 Gd4 Co1 71.87(19) . .
O19 Gd4 Co1 138.55(15) . .
O26 Gd4 Co1 115.53(17) . .
O3 Gd4 Co1 100.13(17) . .
O2 Gd4 Co1 35.52(16) . .
O23 Gd4 Co1 71.53(17) . .
O24 Gd4 Co1 90.94(18) . .
N9 Gd4 Co1 80.6(2) . .
O11 Gd4 Gd5 99.42(16) . .
O12 Gd4 Gd5 99.72(17) . .
O18 Gd4 Gd5 41.50(19) . .
O19 Gd4 Gd5 41.42(16) . .
O26 Gd4 Gd5 41.68(15) . .
O3 Gd4 Gd5 108.92(16) . .
O2 Gd4 Gd5 111.33(15) . .
O23 Gd4 Gd5 172.12(18) . .
O24 Gd4 Gd5 121.3(2) . .
N9 Gd4 Gd5 147.2(3) . .
Co1 Gd4 Gd5 112.53(3) . .
O11 Gd4 H19B 128.7 . .
O12 Gd4 H19B 86.6 . .
O18 Gd4 H19B 58.2 . .
O19 Gd4 H19B 19.9 . .
O26 Gd4 H19B 77.8 . .
O3 Gd4 H19B 69.0 . .
O2 Gd4 H19B 94.4 . .
O23 Gd4 H19B 144.8 . .
O24 Gd4 H19B 148.3 . .
N9 Gd4 H19B 157.2 . .
Co1 Gd4 H19B 118.9 . .
Gd5 Gd4 H19B 40.0 . .
O17 Gd5 O20 141.6(2) . .
O17 Gd5 O19 140.4(3) . .
O20 Gd5 O19 69.1(2) . .
O17 Gd5 O7 68.9(2) . .
O20 Gd5 O7 134.0(2) . .
O19 Gd5 O7 109.8(2) . .
O17 Gd5 O18 69.9(2) . .
O20 Gd5 O18 139.3(2) . .
O19 Gd5 O18 72.4(2) . .
O7 Gd5 O18 72.0(2) . .
O17 Gd5 O26 86.0(2) . .
O20 Gd5 O26 86.3(2) . .
O19 Gd5 O26 69.2(2) . .
O7 Gd5 O26 138.2(3) . .
O18 Gd5 O26 68.0(2) . .
O17 Gd5 O8 132.3(2) . .
O20 Gd5 O8 68.9(2) . .
O19 Gd5 O8 73.5(2) . .
O7 Gd5 O8 67.1(2) . .
O18 Gd5 O8 111.9(2) . .
O26 Gd5 O8 140.6(2) . .
O17 Gd5 O30 77.9(3) . .
O20 Gd5 O30 79.7(2) . .
O19 Gd5 O30 141.5(3) . .
O7 Gd5 O30 76.1(3) . .
O18 Gd5 O30 140.8(2) . .
O26 Gd5 O30 132.0(3) . .
O8 Gd5 O30 74.5(3) . .
O17 Gd5 O29 71.2(3) . .
O20 Gd5 O29 70.4(2) . .
O19 Gd5 O29 130.6(2) . .
O7 Gd5 O29 118.5(2) . .
O18 Gd5 O29 131.3(2) . .
O26 Gd5 O29 81.2(2) . .
O8 Gd5 O29 115.8(3) . .
O30 Gd5 O29 50.9(2) . .
O17 Gd5 N11 73.9(3) . .
O20 Gd5 N11 72.8(3) . .
O19 Gd5 N11 141.9(3) . .
O7 Gd5 N11 97.2(3) . .
O18 Gd5 N11 143.7(3) . .
O26 Gd5 N11 107.6(3) . .
O8 Gd5 N11 94.1(3) . .
O30 Gd5 N11 24.5(3) . .
O29 Gd5 N11 26.4(3) . .
O17 Gd5 Gd4 99.64(19) . .
O20 Gd5 Gd4 99.20(16) . .
O19 Gd5 Gd4 41.66(17) . .
O7 Gd5 Gd4 108.6(2) . .
O18 Gd5 Gd4 40.92(14) . .
O26 Gd5 Gd4 41.70(18) . .
O8 Gd5 Gd4 111.00(17) . .
O30 Gd5 Gd4 173.67(17) . .
O29 Gd5 Gd4 122.85(17) . .
N11 Gd5 Gd4 149.2(2) . .
O17 Gd5 Gd3 37.51(19) . .
O20 Gd5 Gd3 147.10(15) . .
O19 Gd5 Gd3 102.95(18) . .
O7 Gd5 Gd3 78.94(18) . .
O18 Gd5 Gd3 36.47(16) . .
O26 Gd5 Gd3 61.66(17) . .
O8 Gd5 Gd3 141.44(17) . .
O30 Gd5 Gd3 115.39(18) . .
O29 Gd5 Gd3 95.90(19) . .
N11 Gd5 Gd3 108.3(2) . .
Gd4 Gd5 Gd3 62.409(15) . .
O17 Gd5 H19B 129.3 . .
O20 Gd5 H19B 86.2 . .
O19 Gd5 H19B 20.5 . .
O7 Gd5 H19B 90.0 . .
O18 Gd5 H19B 59.7 . .
O26 Gd5 H19B 80.5 . .
O8 Gd5 H19B 68.2 . .
O30 Gd5 H19B 142.7 . .
O29 Gd5 H19B 151.1 . .
N11 Gd5 H19B 156.6 . .
Gd4 Gd5 H19B 42.9 . .
Gd3 Gd5 H19B 94.9 . .
O19 Gd6 O27 99.1(4) . .
O19 Gd6 O1W' 93.4(4) . .
O27 Gd6 O1W' 5.8(7) . .
O19 Gd6 O22 145.6(2) . .
O27 Gd6 O22 76.9(5) . .
O1W' Gd6 O22 82.0(5) . .
O19 Gd6 O22 144.7(2) . 2_656
O27 Gd6 O22 75.9(4) . 2_656
O1W' Gd6 O22 80.3(4) . 2_656
O22 Gd6 O22 68.3(3) . 2_656
O19 Gd6 O21 91.1(2) . .
O27 Gd6 O21 139.6(5) . .
O1W' Gd6 O21 141.1(5) . .
O22 Gd6 O21 73.0(2) . .
O22 Gd6 O21 115.5(2) 2_656 .
O19 Gd6 O13 91.2(2) . .
O27 Gd6 O13 139.5(5) . .
O1W' Gd6 O13 139.9(5) . .
O22 Gd6 O13 114.2(2) . .
O22 Gd6 O13 73.4(2) 2_656 .
O21 Gd6 O13 78.5(2) . .
O19 Gd6 O12 68.1(2) . .
O27 Gd6 O12 78.9(5) . .
O1W' Gd6 O12 76.0(5) . .
O22 Gd6 O12 141.23(19) . .
O22 Gd6 O12 76.8(2) 2_656 .
O21 Gd6 O12 140.2(2) . .
O13 Gd6 O12 68.9(2) . .
O19 Gd6 O20 68.3(2) . .
O27 Gd6 O20 78.1(4) . .
O1W' Gd6 O20 76.3(4) . .
O22 Gd6 O20 77.5(2) . .
O22 Gd6 O20 140.7(2) 2_656 .
O21 Gd6 O20 69.6(2) . .
O13 Gd6 O20 141.1(2) . .
O12 Gd6 O20 126.0(2) . .
O19 Gd6 Co4 71.62(17) . .
O27 Gd6 Co4 112.8(4) . .
O1W' Gd6 Co4 111.6(4) . .
O22 Gd6 Co4 78.51(13) . .
O22 Gd6 Co4 142.90(17) 2_656 .
O21 Gd6 Co4 35.10(14) . .
O13 Gd6 Co4 107.63(14) . .
O12 Gd6 Co4 139.39(13) . .
O20 Gd6 Co4 35.62(15) . .
O19 Gd6 Co2 70.67(18) . .
O27 Gd6 Co2 114.5(5) . .
O1W' Gd6 Co2 112.0(5) . .
O22 Gd6 Co2 142.40(14) . .
O22 Gd6 Co2 79.63(17) 2_656 .
O21 Gd6 Co2 105.85(17) . .
O13 Gd6 Co2 34.19(16) . .
O12 Gd6 Co2 36.27(16) . .
O20 Gd6 Co2 138.57(16) . .
Co4 Gd6 Co2 122.74(4) . .
O19 Gd6 Gd7 129.17(16) . .
O27 Gd6 Gd7 112.7(5) . .
O1W' Gd6 Gd7 117.5(5) . .
O22 Gd6 Gd7 36.21(15) . .
O22 Gd6 Gd7 83.07(16) 2_656 .
O21 Gd6 Gd7 39.44(15) . .
O13 Gd6 Gd7 89.15(16) . .
O12 Gd6 Gd7 153.55(14) . .
O20 Gd6 Gd7 80.36(17) . .
Co4 Gd6 Gd7 60.06(3) . .
Co2 Gd6 Gd7 123.34(3) . .
O19 Gd6 H22B 126.6 . .
O27 Gd6 H22B 69.8 . .
O1W' Gd6 H22B 73.8 . .
O22 Gd6 H22B 19.9 . .
O22 Gd6 H22B 85.1 2_656 .
O21 Gd6 H22B 72.7 . .
O13 Gd6 H22B 131.8 . .
O12 Gd6 H22B 146.9 . .
O20 Gd6 H22B 58.3 . .
Co4 Gd6 H22B 66.4 . .
Co2 Gd6 H22B 162.3 . .
Gd7 Gd6 H22B 44.9 . .
O22 Gd7 O32 73.5(3) . .
O22 Gd7 O33 126.9(3) . .
O32 Gd7 O33 53.4(4) . .
O22 Gd7 O4 81.8(2) . 2_656
O32 Gd7 O4 136.0(2) . 2_656
O33 Gd7 O4 136.0(3) . 2_656
O22 Gd7 O5 81.0(2) . 2_656
O32 Gd7 O5 137.7(2) . 2_656
O33 Gd7 O5 138.4(2) . 2_656
O4 Gd7 O5 69.9(2) 2_656 2_656
O22 Gd7 O21 74.3(2) . .
O32 Gd7 O21 73.91(15) . .
O33 Gd7 O21 89.8(3) . .
O4 Gd7 O21 133.1(2) 2_656 .
O5 Gd7 O21 66.9(2) 2_656 .
O22 Gd7 O13 74.8(2) . 2_656
O32 Gd7 O13 72.04(17) . 2_656
O33 Gd7 O13 87.8(2) . 2_656
O4 Gd7 O13 66.6(2) 2_656 2_656
O5 Gd7 O13 132.5(2) 2_656 2_656
O21 Gd7 O13 139.1(2) . 2_656
O22 Gd7 O34 154.6(3) . .
O32 Gd7 O34 118.5(4) . .
O33 Gd7 O34 68.9(4) . .
O4 Gd7 O34 99.3(4) 2_656 .
O5 Gd7 O34 75.7(4) 2_656 .
O21 Gd7 O34 87.3(3) . .
O13 Gd7 O34 129.1(3) 2_656 .
O22 Gd7 O34' 147.8(3) . .
O32 Gd7 O34' 133.4(5) . .
O33 Gd7 O34' 82.2(4) . .
O4 Gd7 O34' 84.6(4) 2_656 .
O5 Gd7 O34' 66.9(3) 2_656 .
O21 Gd7 O34' 94.7(3) . .
O13 Gd7 O34' 125.3(3) 2_656 .
O34 Gd7 O34' 15.1(5) . .
O22 Gd7 O35' 152.1(4) . .
O32 Gd7 O35' 108.9(4) . .
O33 Gd7 O35' 61.9(4) . .
O4 Gd7 O35' 78.1(4) 2_656 .
O5 Gd7 O35' 109.4(3) 2_656 .
O21 Gd7 O35' 133.5(4) . .
O13 Gd7 O35' 79.6(3) 2_656 .
O34 Gd7 O35' 49.5(3) . .
O34' Gd7 O35' 48.5(3) . .
O22 Gd7 O35 145.9(3) . .
O32 Gd7 O35 124.1(4) . .
O33 Gd7 O35 76.9(4) . .
O4 Gd7 O35 65.5(3) 2_656 .
O5 Gd7 O35 95.7(3) 2_656 .
O21 Gd7 O35 135.6(3) . .
O13 Gd7 O35 83.3(3) 2_656 .
O34 Gd7 O35 48.4(3) . .
O34' Gd7 O35 42.1(3) . .
O35' Gd7 O35 15.5(4) . .
O22 Gd7 N12 98.2(3) . .
O32 Gd7 N12 24.7(4) . .
O33 Gd7 N12 28.7(3) . .
O4 Gd7 N12 143.65(14) 2_656 .
O5 Gd7 N12 146.30(17) 2_656 .
O21 Gd7 N12 80.34(17) . .
O13 Gd7 N12 78.22(18) 2_656 .
O34 Gd7 N12 95.6(4) . .
O34' Gd7 N12 109.9(5) . .
O35' Gd7 N12 87.1(4) . .
O35 Gd7 N12 102.6(4) . .
O2W Gd8 O2W 73.2(7) 6_575 .
O2W Gd8 O6W 143.2(4) 6_575 .
O2W Gd8 O6W 143.2(4) . .
O2W Gd8 O4W 75.7(6) 6_575 .
O2W Gd8 O4W 75.7(6) . .
O6W Gd8 O4W 112.7(7) . .
O2W Gd8 O3W 117.2(6) 6_575 .
O2W Gd8 O3W 73.8(5) . .
O6W Gd8 O3W 79.9(6) . .
O4W Gd8 O3W 140.8(4) . .
O2W Gd8 O3W 73.8(5) 6_575 6_575
O2W Gd8 O3W 117.2(6) . 6_575
O6W Gd8 O3W 79.9(6) . 6_575
O4W Gd8 O3W 140.8(4) . 6_575
O3W Gd8 O3W 76.3(8) . 6_575
O2W Gd8 O5W 78.2(5) 6_575 6_575
O2W Gd8 O5W 141.8(5) . 6_575
O6W Gd8 O5W 71.0(4) . 6_575
O4W Gd8 O5W 73.0(4) . 6_575
O3W Gd8 O5W 143.4(5) . 6_575
O3W Gd8 O5W 77.1(5) 6_575 6_575
O2W Gd8 O5W 141.8(5) 6_575 .
O2W Gd8 O5W 78.2(5) . .
O6W Gd8 O5W 71.0(4) . .
O4W Gd8 O5W 73.0(4) . .
O3W Gd8 O5W 77.1(5) . .
O3W Gd8 O5W 143.4(5) 6_575 .
O5W Gd8 O5W 112.3(7) 6_575 .
O2W Gd8 H3WB 138.2 6_575 .
O2W Gd8 H3WB 84.8 . .
O6W Gd8 H3WB 62.9 . .
O4W Gd8 H3WB 133.0 . .
O3W Gd8 H3WB 20.9 . .
O3W Gd8 H3WB 86.1 6_575 .
O5W Gd8 H3WB 133.0 6_575 .
O5W Gd8 H3WB 61.2 . .
O2W Gd8 H5WA 124.6 6_575 .
O2W Gd8 H5WA 59.2 . .
O6W Gd8 H5WA 90.0 . .
O4W Gd8 H5WA 67.0 . .
O3W Gd8 H5WA 76.4 . .
O3W Gd8 H5WA 152.2 6_575 .
O5W Gd8 H5WA 124.1 6_575 .
O5W Gd8 H5WA 19.3 . .
H3WB Gd8 H5WA 66.3 . .
C1 N1 C5 116.2(10) . .
C1 N1 Co1 127.1(8) . .
C5 N1 Co1 116.5(7) . .
C12 N2 C8 119.5(10) . .
C12 N2 Co1 116.2(8) . .
C8 N2 Co1 124.3(8) . .
C16 N3 C20 119.3(9) . .
C16 N3 Co2 114.0(7) . .
C20 N3 Co2 126.7(7) . .
C21 N4 C25 117.3(9) . .
C21 N4 Co2 127.4(6) . .
C25 N4 Co2 115.3(7) . .
C33 N5 C29 118.8(9) . .
C33 N5 Co4 125.8(8) . 2_656
C29 N5 Co4 115.1(6) . 2_656
C38 N6 C34 118.7(12) . .
C38 N6 Co3 116.6(9) . .
C34 N6 Co3 124.7(9) . .
C45 N7 C41 116.6(10) . .
C45 N7 Co3 113.8(6) . .
C41 N7 Co3 129.2(9) . .
C49 N8 C53 119.1(9) . .
C49 N8 Co4 114.8(7) . .
C53 N8 Co4 126.2(7) . .
O23 N9 O25 121.4(13) . .
O23 N9 O24 118.9(9) . .
O25 N9 O24 119.7(12) . .
O23 N9 Gd4 57.6(5) . .
O25 N9 Gd4 178.7(11) . .
O24 N9 Gd4 61.4(5) . .
O26 N10 O27 133.6(14) . .
O26 N10 O28 96.2(12) . .
O27 N10 O28 129.4(15) . .
O26 N10 H1WC 122.7 . .
O27 N10 H1WC 43.9 . .
O28 N10 H1WC 122.4 . .
O26 N10 H1WD 118.3 . .
O27 N10 H1WD 42.3 . .
O28 N10 H1WD 112.8 . .
H1WC N10 H1WD 86.1 . .
N10 O27 Gd6 112.1(11) . .
N10 O27 H1WC 44.7 . .
Gd6 O27 H1WC 105.6 . .
N10 O27 H1WD 43.8 . .
Gd6 O27 H1WD 106.1 . .
H1WC O27 H1WD 88.5 . .
Gd3 O1W H1WA 110.5 . .
Gd3 O1W H1WB 113.0 . .
H1WA O1W H1WB 108.7 . .
O26 N10' O27' 137.2(16) . .
O26 N10' O28' 96.4(13) . .
O27' N10' O28' 126.3(16) . .
O26 N10' H1WA 121.6 . .
O27' N10' H1WA 36.3 . .
O28' N10' H1WA 127.2 . .
O26 N10' H1WB 119.3 . .
O27' N10' H1WB 42.7 . .
O28' N10' H1WB 115.9 . .
H1WA N10' H1WB 78.1 . .
Gd6 O1W' H1WC 112.3 . .
Gd6 O1W' H1WD 111.6 . .
H1WC O1W' H1WD 108.5 . .
N10' O27' Gd3 105.4(12) . .
N10' O27' H1WA 44.8 . .
Gd3 O27' H1WA 95.7 . .
N10' O27' H1WB 48.6 . .
Gd3 O27' H1WB 94.2 . .
H1WA O27' H1WB 92.2 . .
O30 N11 O31 121.0(11) . .
O30 N11 O29 119.5(10) . .
O31 N11 O29 119.4(11) . .
O30 N11 Gd5 57.5(6) . .
O31 N11 Gd5 172.9(9) . .
O29 N11 Gd5 62.1(6) . .
O32 N12 O33 117.8(7) . 2_656
O32 N12 O33 117.8(7) . .
O33 N12 O33 124.4(14) 2_656 .
O32 N12 Gd7 57.6(3) . 2_656
O33 N12 Gd7 60.2(5) 2_656 2_656
O33 N12 Gd7 175.3(9) . 2_656
O32 N12 Gd7 57.6(3) . .
O33 N12 Gd7 175.3(9) 2_656 .
O33 N12 Gd7 60.2(5) . .
Gd7 N12 Gd7 115.1(5) 2_656 .
O37 N14 O38 119.9(15) . .
O37 N14 O39 118.8(15) . .
O38 N14 O39 121.2(13) . .
O40 N15 O41 120.7(11) . .
O40 N15 O42 120.6(12) . .
O41 N15 O42 118.6(12) . .
O43 N16 O44 164.7(11) . .
O43 N16 O45 89.5(13) . .
O44 N16 O45 75.3(13) . .
N16 O45 O44 45.2(6) . .
O43 N16' O44 170.2(11) . .
O43 N16' O45' 78.6(14) . .
O44 N16' O45' 91.9(15) . .
N16' O45' O43 43.7(6) . .
O46 N17 O47 121.5(8) . .
O46 N17 O47 121.5(8) . 6_575
O47 N17 O47 117.0(15) . 6_575
O48 N18 O49 120.7(14) . 6_575
O48 N18 O49 120.7(14) . .
O49 N18 O49 118(3) 6_575 .
C6 O1 Co1 120.5(7) . .
C6 O1 Gd1 133.8(7) . .
Co1 O1 Gd1 105.3(3) . .
C13 O2 Co1 117.2(7) . .
C13 O2 Gd4 140.9(7) . .
Co1 O2 Gd4 101.7(3) . .
C15 O3 Co2 118.9(6) . .
C15 O3 Gd4 137.4(6) . .
Co2 O3 Gd4 103.6(3) . .
C26 O4 Co2 118.5(6) . .
C26 O4 Gd7 134.6(6) . 2_656
Co2 O4 Gd7 106.3(3) . 2_656
C28 O5 Co4 119.7(6) . 2_656
C28 O5 Gd7 134.4(6) . 2_656
Co4 O5 Gd7 105.8(3) 2_656 2_656
C39 O6 Co3 118.5(8) . .
C39 O6 Gd2 134.4(7) . .
Co3 O6 Gd2 105.6(4) . .
C46 O7 Co3 118.0(6) . .
C46 O7 Gd5 138.2(6) . .
Co3 O7 Gd5 103.8(3) . .
C48 O8 Co4 118.4(6) . .
C48 O8 Gd5 139.0(7) . .
Co4 O8 Gd5 102.6(2) . .
Co1 O9 Gd3 103.5(3) . .
Co1 O9 Gd1 107.0(3) . .
Gd3 O9 Gd1 103.3(3) . .
Co1 O9 H9B 83.3 . .
Gd3 O9 H9B 105.9 . .
Gd1 O9 H9B 145.7 . .
Gd1 O10 Gd3 105.1(2) . 6_575
Gd1 O10 Gd3 105.1(2) . .
Gd3 O10 Gd3 111.0(4) 6_575 .
Gd1 O10 H10B 111.9 . .
Gd3 O10 H10B 111.7 6_575 .
Gd3 O10 H10B 111.7 . .
Co1 O11 Gd4 105.1(3) . .
Co1 O11 Gd3 100.3(2) . .
Gd4 O11 Gd3 106.8(3) . .
Co1 O11 H11B 114.3 . .
Gd4 O11 H11B 114.6 . .
Gd3 O11 H11B 114.4 . .
Co2 O12 Gd4 105.2(3) . .
Co2 O12 Gd6 99.8(3) . .
Gd4 O12 Gd6 106.8(2) . .
Co2 O12 H12 114.5 . .
Gd4 O12 H12 114.6 . .
Gd6 O12 H12 114.5 . .
Co2 O13 Gd6 103.3(3) . .
Co2 O13 Gd7 107.6(2) . 2_656
Gd6 O13 Gd7 101.5(2) . 2_656
Co2 O13 H13 114.2 . .
Gd6 O13 H13 114.5 . .
Gd7 O13 H13 114.4 2_656 .
Gd2 O14 Gd1 161.7(5) . .
Gd2 O14 H14B 77.0 . .
Gd1 O14 H14B 109.2 . .
Gd2 O15 Gd3 105.1(3) . .
Gd2 O15 Gd3 105.1(3) . 6_575
Gd3 O15 Gd3 111.4(4) . 6_575
Gd2 O15 H15 111.7 . .
Gd3 O15 H15 111.6 . .
Gd3 O15 H15 111.6 6_575 .
Co3 O16 Gd3 102.7(3) . .
Co3 O16 Gd2 106.8(3) . .
Gd3 O16 Gd2 102.4(2) . .
Co3 O16 H16 88.0 . .
Gd3 O16 H16 102.9 . .
Gd2 O16 H16 146.9 . .
Co3 O17 Gd5 105.5(3) . .
Co3 O17 Gd3 99.8(3) . .
Gd5 O17 Gd3 107.1(3) . .
Co3 O17 H17B 114.2 . .
Gd5 O17 H17B 114.4 . .
Gd3 O17 H17B 114.5 . .
Gd4 O18 Gd5 97.6(2) . .
Gd4 O18 Gd3 108.2(2) . .
Gd5 O18 Gd3 107.2(3) . .
Gd4 O18 H18B 114.2 . .
Gd5 O18 H18B 114.3 . .
Gd3 O18 H18B 114.0 . .
Gd6 O19 Gd5 108.7(3) . .
Gd6 O19 Gd4 107.7(2) . .
Gd5 O19 Gd4 96.9(2) . .
Gd6 O19 H19B 166.8 . .
Gd5 O19 H19B 75.2 . .
Gd4 O19 H19B 83.9 . .
Co4 O20 Gd5 105.5(2) . .
Co4 O20 Gd6 100.3(3) . .
Gd5 O20 Gd6 106.2(3) . .
Co4 O20 H20B 114.5 . .
Gd5 O20 H20B 114.5 . .
Gd6 O20 H20B 114.6 . .
Co4 O21 Gd6 102.3(3) . .
Co4 O21 Gd7 107.8(3) . .
Gd6 O21 Gd7 101.6(2) . .
Co4 O21 H21B 114.5 . .
Gd6 O21 H21B 114.7 . .
Gd7 O21 H21B 114.6 . .
Gd7 O22 Gd6 105.8(2) . .
Gd7 O22 Gd6 105.9(2) . 2_656
Gd6 O22 Gd6 111.5(2) . 2_656
Gd7 O22 H22B 105.7 . .
Gd6 O22 H22B 83.9 . .
Gd6 O22 H22B 139.1 2_656 .
N9 O23 Gd4 97.4(7) . .
N9 O24 Gd4 92.6(6) . .
N10' O26 N10 77.8(11) . .
N10' O26 Gd5 120.5(8) . .
N10 O26 Gd5 122.5(9) . .
N10' O26 Gd4 123.2(11) . .
N10 O26 Gd4 118.5(8) . .
Gd5 O26 Gd4 96.6(2) . .
N11 O29 Gd5 91.5(7) . .
N11 O30 Gd5 98.0(6) . .
N12 O32 Gd7 97.7(3) . 2_656
N12 O32 Gd7 97.7(3) . .
Gd7 O32 Gd7 164.5(6) 2_656 .
N12 O33 Gd7 91.0(7) . .
O35 N13 O36 131.9(12) . .
O35 N13 O34 118.3(11) . .
O36 N13 O34 109.0(11) . .
O35 N13 Gd7 60.4(8) . .
O36 N13 Gd7 162.3(11) . .
O34 N13 Gd7 58.0(6) . .
N13 O34 Gd7 95.7(7) . .
N13 O35 Gd7 97.4(9) . .
N16' O43 N16 12.5(6) . .
N16' O43 O45' 57.8(10) . .
N16 O43 O45' 45.3(9) . .
N16' O44 N16 12.4(6) . .
N16' O44 O45 47.1(8) . .
N16 O44 O45 59.5(9) . .
N1 C1 C2 123.4(13) . .
N1 C1 H1 118.3 . .
C2 C1 H1 118.3 . .
C1 C2 C3 115.5(13) . .
C1 C2 H2 122.3 . .
C3 C2 H2 122.3 . .
C4 C3 C2 121.8(15) . .
C4 C3 H3 119.1 . .
C2 C3 H3 119.1 . .
C5 C4 C3 118.3(15) . .
C5 C4 H4 120.8 . .
C3 C4 H4 120.8 . .
C4 C5 N1 124.6(12) . .
C4 C5 C6 122.1(12) . .
N1 C5 C6 113.2(10) . .
O1 C6 C7 126.0(12) . .
O1 C6 C5 113.6(10) . .
C7 C6 C5 120.3(11) . .
C6 C7 C6 124.8(17) . 6_575
C6 C7 H7 117.6 . .
C6 C7 H7 117.6 6_575 .
C9 C8 N2 121.9(13) . .
C9 C8 H8 119.1 . .
N2 C8 H8 119.1 . .
C8 C9 C10 118.3(17) . .
C8 C9 H9 120.8 . .
C10 C9 H9 120.8 . .
C9 C10 C11 121.9(18) . .
C9 C10 H10 119.1 . .
C11 C10 H10 119.1 . .
C12 C11 C10 116.8(16) . .
C12 C11 H11 121.6 . .
C10 C11 H11 121.6 . .
N2 C12 C11 121.3(13) . .
N2 C12 C13 115.0(10) . .
C11 C12 C13 123.6(12) . .
O2 C13 C14 121.3(10) . .
O2 C13 C12 114.7(10) . .
C14 C13 C12 123.8(10) . .
C15 C14 C13 123.4(10) . .
C15 C14 H14 118.3 . .
C13 C14 H14 118.3 . .
O3 C15 C14 126.7(10) . .
O3 C15 C16 112.9(9) . .
C14 C15 C16 120.3(9) . .
N3 C16 C17 122.7(10) . .
N3 C16 C15 115.9(9) . .
C17 C16 C15 121.3(9) . .
C18 C17 C16 117.4(11) . .
C18 C17 H17 121.3 . .
C16 C17 H17 121.3 . .
C17 C18 C19 119.3(12) . .
C17 C18 H18 120.4 . .
C19 C18 H18 120.4 . .
C18 C19 C20 120.1(11) . .
C18 C19 H19 120.0 . .
C20 C19 H19 120.0 . .
N3 C20 C19 121.2(10) . .
N3 C20 H20 119.4 . .
C19 C20 H20 119.4 . .
N4 C21 C22 124.3(9) . .
N4 C21 H21 117.8 . .
C22 C21 H21 117.8 . .
C21 C22 C23 120.0(12) . .
C21 C22 H22 120.0 . .
C23 C22 H22 120.0 . .
C22 C23 C24 118.3(13) . .
C22 C23 H23 120.9 . .
C24 C23 H23 120.9 . .
C23 C24 C25 117.3(10) . .
C23 C24 H24 121.3 . .
C25 C24 H24 121.3 . .
N4 C25 C24 122.5(10) . .
N4 C25 C26 116.4(10) . .
C24 C25 C26 121.1(9) . .
O4 C26 C27 126.0(11) . .
O4 C26 C25 112.9(8) . .
C27 C26 C25 121.1(10) . .
C26 C27 C28 123.4(11) . .
C26 C27 H27 118.3 . .
C28 C27 H27 118.3 . .
O5 C28 C27 126.3(9) . .
O5 C28 C29 114.4(9) . .
C27 C28 C29 119.2(9) . .
N5 C29 C30 120.8(9) . .
N5 C29 C28 114.6(9) . .
C30 C29 C28 124.6(11) . .
C31 C30 C29 121.0(13) . .
C31 C30 H30 119.5 . .
C29 C30 H30 119.5 . .
C32 C31 C30 115.5(12) . .
C32 C31 H31 122.3 . .
C30 C31 H31 122.3 . .
C31 C32 C33 121.9(10) . .
C31 C32 H32 119.1 . .
C33 C32 H32 119.1 . .
N5 C33 C32 121.9(11) . .
N5 C33 H33 119.1 . .
C32 C33 H33 119.1 . .
C35 C34 N6 120.4(13) . .
C35 C34 H34 119.8 . .
N6 C34 H34 119.8 . .
C34 C35 C36 122.2(13) . .
C34 C35 H35 118.9 . .
C36 C35 H35 118.9 . .
C35 C36 C37 115.9(14) . .
C35 C36 H36 122.0 . .
C37 C36 H36 122.0 . .
C38 C37 C36 120.6(14) . .
C38 C37 H37 119.7 . .
C36 C37 H37 119.7 . .
N6 C38 C37 122.1(13) . .
N6 C38 C39 114.2(13) . .
C37 C38 C39 123.2(13) . .
O6 C39 C40 125.6(13) . .
O6 C39 C38 115.5(12) . .
C40 C39 C38 118.9(14) . .
C39 C40 C39 121.4(19) 6_575 .
C39 C40 H40 119.3 6_575 .
C39 C40 H40 119.3 . .
C42 C41 N7 123.4(12) . .
C42 C41 H41 118.3 . .
N7 C41 H41 118.3 . .
C41 C42 C43 120.2(11) . .
C41 C42 H42 119.9 . .
C43 C42 H42 119.9 . .
C44 C43 C42 119.9(12) . .
C44 C43 H43 120.1 . .
C42 C43 H43 120.1 . .
C43 C44 C45 117.7(12) . .
C43 C44 H44 121.2 . .
C45 C44 H44 121.2 . .
N7 C45 C44 122.1(10) . .
N7 C45 C46 114.7(10) . .
C44 C45 C46 123.0(10) . .
O7 C46 C47 122.4(10) . .
O7 C46 C45 115.1(9) . .
C47 C46 C45 122.1(9) . .
C48 C47 C46 125.9(9) . .
C48 C47 H47 117.0 . .
C46 C47 H47 117.0 . .
O8 C48 C47 122.1(9) . .
O8 C48 C49 115.9(8) . .
C47 C48 C49 121.9(8) . .
N8 C49 C50 120.9(10) . .
N8 C49 C48 115.2(8) . .
C50 C49 C48 123.9(9) . .
C51 C50 C49 120.1(11) . .
C51 C50 H50 120.0 . .
C49 C50 H50 120.0 . .
C50 C51 C52 118.4(11) . .
C50 C51 H51 120.8 . .
C52 C51 H51 120.8 . .
C53 C52 C51 118.7(10) . .
C53 C52 H52 120.7 . .
C51 C52 H52 120.7 . .
N8 C53 C52 122.7(10) . .
N8 C53 H53 118.6 . .
C52 C53 H53 118.6 . .
Gd8 O2W H2WA 134.1 . .
Gd8 O2W H2WB 117.3 . .
H2WA O2W H2WB 108.5 . .
Gd8 O3W H3WB 67.7 . .
Gd8 O3W H3WA 175.9 . .
H3WB O3W H3WA 110.9 . .
Gd8 O4W H4WA 112.9 . .
Gd8 O4W H4WB 122.3 . .
H4WA O4W H4WB 106.5 . .
Gd8 O5W H5WA 91.3 . .
Gd8 O5W H5WB 110.8 . .
H5WA O5W H5WB 113.1 . .
Gd8 O6W H6W 113.6 . .
H7WA O7W H7WB 108.3 . .
H8WA O8W H8WB 108.5 . .
O9W O9W Gd1 80.30(16) 6_575 .
O10W O10W Gd1 79.25(18) 6_575 .
O11W O11W Gd2 78.84(18) 6_575 .
O12W O12W Gd2 80.03(17) 6_575 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Co1 O9 2.072(7) .
Co1 O11 2.078(7) .
Co1 N2 2.094(10) .
Co1 O2 2.099(7) .
Co1 O1 2.118(7) .
Co1 N1 2.184(9) .
Co1 Gd3 3.5288(19) .
Co1 Gd4 3.5372(18) .
Co2 O13 2.030(7) .
Co2 O3 2.088(6) .
Co2 O12 2.110(7) .
Co2 O4 2.150(6) .
Co2 N4 2.155(9) .
Co2 N3 2.176(8) .
Co2 Gd6 3.5154(17) .
Co3 O16 2.059(8) .
Co3 O7 2.083(7) .
Co3 O17 2.092(6) .
Co3 O6 2.121(8) .
Co3 N6 2.146(11) .
Co3 N7 2.151(9) .
Co3 Gd3 3.5157(17) .
Co4 O21 2.065(6) .
Co4 O20 2.078(7) .
Co4 O8 2.107(7) .
Co4 O5 2.153(7) 2_656
Co4 N8 2.161(8) .
Co4 N5 2.175(8) 2_656
Co4 Gd6 3.5096(14) .
Gd1 O14 2.328(12) .
Gd1 O10 2.354(10) .
Gd1 O10W 2.3878(17) 6_575
Gd1 O10W 2.3878(16) .
Gd1 O9 2.425(7) .
Gd1 O9 2.425(7) 6_575
Gd1 O1 2.431(7) .
Gd1 O1 2.431(7) 6_575
Gd1 O9W 2.6446(17) 6_575
Gd1 O9W 2.6446(17) .
Gd1 Gd3 3.7963(11) .
Gd1 Gd3 3.7963(11) 6_575
Gd2 O14 2.310(13) .
Gd2 O15 2.367(9) .
Gd2 O11W 2.3694(18) 6_575
Gd2 O11W 2.3694(18) .
Gd2 O6 2.422(9) .
Gd2 O6 2.422(9) 6_575
Gd2 O16 2.445(7) .
Gd2 O16 2.445(7) 6_575
Gd2 O12W 2.5736(16) 6_575
Gd2 O12W 2.5736(16) .
Gd2 Gd3 3.8020(9) .
Gd2 Gd3 3.8020(8) 6_575
Gd2 H14B 2.2747 .
Gd3 O1W 2.291(14) .
Gd3 O9 2.415(8) .
Gd3 O15 2.423(6) .
Gd3 O10 2.429(6) .
Gd3 O18 2.433(7) .
Gd3 O16 2.434(6) .
Gd3 O27' 2.47(2) .
Gd3 O17 2.492(8) .
Gd3 O11 2.503(6) .
Gd4 O11 2.373(7) .
Gd4 O12 2.380(6) .
Gd4 O18 2.399(6) .
Gd4 O19 2.431(7) .
Gd4 O26 2.431(8) .
Gd4 O3 2.447(7) .
Gd4 O2 2.453(7) .
Gd4 O23 2.493(8) .
Gd4 O24 2.575(7) .
Gd4 N9 2.930(10) .
Gd4 Gd5 3.6305(8) .
Gd4 H19B 2.4889 .
Gd5 O17 2.370(7) .
Gd5 O20 2.410(7) .
Gd5 O19 2.419(7) .
Gd5 O7 2.427(6) .
Gd5 O18 2.427(8) .
Gd5 O26 2.430(6) .
Gd5 O8 2.467(7) .
Gd5 O30 2.485(8) .
Gd5 O29 2.580(9) .
Gd5 N11 2.917(11) .
Gd5 H19B 2.3511 .
Gd6 O19 2.397(7) .
Gd6 O27 2.399(17) .
Gd6 O1W' 2.404(17) .
Gd6 O22 2.424(7) .
Gd6 O22 2.432(5) 2_656
Gd6 O21 2.433(6) .
Gd6 O13 2.439(7) .
Gd6 O12 2.477(7) .
Gd6 O20 2.482(6) .
Gd6 Gd7 3.7874(8) .
Gd6 H22B 2.4820 .
Gd7 O22 2.325(7) .
Gd7 O32 2.3393(18) .
Gd7 O33 2.385(8) .
Gd7 O4 2.388(7) 2_656
Gd7 O5 2.429(6) 2_656
Gd7 O21 2.456(7) .
Gd7 O13 2.462(5) 2_656
Gd7 O34 2.489(13) .
Gd7 O34' 2.516(14) .
Gd7 O35' 2.524(15) .
Gd7 O35 2.560(15) .
Gd7 N12 2.747(8) .
Gd8 O2W 2.340(13) 6_575
Gd8 O2W 2.340(13) .
Gd8 O6W 2.366(16) .
Gd8 O4W 2.37(2) .
Gd8 O3W 2.377(17) .
Gd8 O3W 2.377(17) 6_575
Gd8 O5W 2.408(12) 6_575
Gd8 O5W 2.408(12) .
Gd8 H3WB 2.1988 .
Gd8 H5WA 2.5721 .
N1 C1 1.342(16) .
N1 C5 1.347(15) .
N2 C12 1.329(17) .
N2 C8 1.381(16) .
N3 C16 1.310(13) .
N3 C20 1.351(13) .
N4 C21 1.313(14) .
N4 C25 1.332(11) .
N5 C33 1.300(11) .
N5 C29 1.353(15) .
N5 Co4 2.175(8) 2_656
N6 C38 1.302(18) .
N6 C34 1.408(16) .
N7 C45 1.371(15) .
N7 C41 1.372(15) .
N8 C49 1.331(13) .
N8 C53 1.336(13) .
N9 O23 1.251(14) .
N9 O25 1.274(14) .
N9 O24 1.286(15) .
N10 O26 1.429(18) .
N10 O27 1.45(2) .
N10 O28 1.56(2) .
N10 H1WC 1.0175 .
N10 H1WD 1.0042 .
O27 H1WC 1.0031 .
O27 H1WD 0.9756 .
O1W H1WA 0.8500 .
O1W H1WB 0.8501 .
N10' O26 1.41(2) .
N10' O27' 1.50(3) .
N10' O28' 1.58(2) .
N10' H1WA 1.0676 .
N10' H1WB 1.1231 .
O1W' H1WC 0.8503 .
O1W' H1WD 0.8505 .
O27' H1WA 0.8977 .
O27' H1WB 1.0159 .
N11 O30 1.222(13) .
N11 O31 1.279(17) .
N11 O29 1.297(12) .
N12 O32 1.159(18) .
N12 O33 1.321(11) 2_656
N12 O33 1.321(11) .
N12 Gd7 2.747(8) 2_656
N14 O37 1.217(18) .
N14 O38 1.255(18) .
N14 O39 1.270(17) .
N15 O40 1.240(14) .
N15 O41 1.262(15) .
N15 O42 1.280(16) .
N16 O43 1.213(8) .
N16 O44 1.219(8) .
N16 O45 1.481(14) .
O45 O44 1.66(2) .
N16' O43 1.208(8) .
N16' O44 1.211(8) .
N16' O45' 1.479(15) .
O45' O43 1.71(3) .
N17 O46 1.220(9) .
N17 O47 1.228(8) .
N17 O47 1.228(8) 6_575
N18 O48 1.23(3) .
N18 O49 1.34(2) 6_575
N18 O49 1.34(2) .
O1 C6 1.290(13) .
O2 C13 1.296(13) .
O3 C15 1.277(12) .
O4 C26 1.296(13) .
O4 Gd7 2.388(7) 2_656
O5 C28 1.260(13) .
O5 Co4 2.153(7) 2_656
O5 Gd7 2.429(6) 2_656
O6 C39 1.250(16) .
O7 C46 1.299(12) .
O8 C48 1.270(11) .
O9 H9B 0.8500 .
O10 Gd3 2.429(6) 6_575
O10 H10B 0.8500 .
O11 H11B 0.8500 .
O12 H12 0.8502 .
O13 Gd7 2.462(5) 2_656
O13 H13 0.8498 .
O14 H14B 0.8499 .
O15 Gd3 2.423(6) 6_575
O15 H15 0.8505 .
O16 H16 0.8504 .
O17 H17B 0.8496 .
O18 H18B 0.8508 .
O19 H19B 0.8500 .
O20 H20B 0.8503 .
O21 H21B 0.8492 .
O22 Gd6 2.432(5) 2_656
O22 H22B 0.8500 .
O32 Gd7 2.3393(17) 2_656
N13 O35 1.111(11) .
N13 O36 1.217(12) .
N13 O34 1.299(12) .
C1 C2 1.37(2) .
C1 H1 0.9500 .
C2 C3 1.40(2) .
C2 H2 0.9500 .
C3 C4 1.33(2) .
C3 H3 0.9500 .
C4 C5 1.321(19) .
C4 H4 0.9500 .
C5 C6 1.562(17) .
C6 C7 1.315(15) .
C7 C6 1.315(15) 6_575
C7 H7 0.9500 .
C8 C9 1.34(2) .
C8 H8 0.9500 .
C9 C10 1.35(3) .
C9 H9 0.9500 .
C10 C11 1.40(2) .
C10 H10 0.9500 .
C11 C12 1.39(2) .
C11 H11 0.9500 .
C12 C13 1.471(17) .
C13 C14 1.409(16) .
C14 C15 1.358(16) .
C14 H14 0.9500 .
C15 C16 1.522(15) .
C16 C17 1.430(16) .
C17 C18 1.373(18) .
C17 H17 0.9500 .
C18 C19 1.379(18) .
C18 H18 0.9500 .
C19 C20 1.381(17) .
C19 H19 0.9500 .
C20 H20 0.9500 .
C21 C22 1.338(17) .
C21 H21 0.9500 .
C22 C23 1.371(16) .
C22 H22 0.9500 .
C23 C24 1.384(19) .
C23 H23 0.9500 .
C24 C25 1.410(17) .
C24 H24 0.9500 .
C25 C26 1.519(16) .
C26 C27 1.334(13) .
C27 C28 1.400(16) .
C27 H27 0.9500 .
C28 C29 1.516(12) .
C29 C30 1.395(17) .
C30 C31 1.373(15) .
C30 H30 0.9500 .
C31 C32 1.37(2) .
C31 H31 0.9500 .
C32 C33 1.386(17) .
C32 H32 0.9500 .
C33 H33 0.9500 .
C34 C35 1.32(2) .
C34 H34 0.9500 .
C35 C36 1.37(2) .
C35 H35 0.9500 .
C36 C37 1.41(2) .
C36 H36 0.9500 .
C37 C38 1.35(2) .
C37 H37 0.9500 .
C38 C39 1.507(19) .
C39 C40 1.402(17) .
C40 C39 1.402(17) 6_575
C40 H40 0.9500 .
C41 C42 1.312(18) .
C41 H41 0.9500 .
C42 C43 1.385(19) .
C42 H42 0.9500 .
C43 C44 1.373(17) .
C43 H43 0.9500 .
C44 C45 1.397(16) .
C44 H44 0.9500 .
C45 C46 1.484(15) .
C46 C47 1.394(16) .
C47 C48 1.381(14) .
C47 H47 0.9500 .
C48 C49 1.470(14) .
C49 C50 1.393(15) .
C50 C51 1.356(17) .
C50 H50 0.9500 .
C51 C52 1.397(18) .
C51 H51 0.9500 .
C52 C53 1.365(16) .
C52 H52 0.9500 .
C53 H53 0.9500 .
O2W H2WA 0.8501 .
O2W H2WB 0.8496 .
O3W H3WB 0.8499 .
O3W H3WA 0.8504 .
O4W H4WA 0.8505 .
O4W H4WB 0.8462 .
O5W H5WA 0.8497 .
O5W H5WB 0.8502 .
O6W H6W 0.8501 .
O7W H7WA 0.8500 .
O7W H7WB 0.8502 .
O8W H8WA 0.8500 .
O8W H8WB 0.8500 .
O9W O9W 0.891(15) 6_575
O10W O10W 0.891(15) 6_575
O11W O11W 0.917(15) 6_575
O12W O12W 0.891(15) 6_575
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O16 Co3 Gd3 O1W 153.5(5) . .
O7 Co3 Gd3 O1W -83.1(4) . .
O17 Co3 Gd3 O1W -9.4(5) . .
O6 Co3 Gd3 O1W 80.4(4) . .
N6 Co3 Gd3 O1W 21.3(7) . .
N7 Co3 Gd3 O1W -159.4(5) . .
O16 Co3 Gd3 O9 -34.8(4) . .
O7 Co3 Gd3 O9 88.6(3) . .
O17 Co3 Gd3 O9 162.3(3) . .
O6 Co3 Gd3 O9 -107.9(3) . .
N6 Co3 Gd3 O9 -167.0(6) . .
N7 Co3 Gd3 O9 12.3(3) . .
O16 Co3 Gd3 O15 77.5(4) . .
O7 Co3 Gd3 O15 -159.1(3) . .
O17 Co3 Gd3 O15 -85.4(4) . .
O6 Co3 Gd3 O15 4.4(3) . .
N6 Co3 Gd3 O15 -54.7(6) . .
N7 Co3 Gd3 O15 124.6(4) . .
O16 Co3 Gd3 O10 48.7(5) . .
O7 Co3 Gd3 O10 172.2(4) . .
O17 Co3 Gd3 O10 -114.2(5) . .
O6 Co3 Gd3 O10 -24.3(5) . .
N6 Co3 Gd3 O10 -83.4(7) . .
N7 Co3 Gd3 O10 95.9(5) . .
O16 Co3 Gd3 O18 -118.8(4) . .
O7 Co3 Gd3 O18 4.7(3) . .
O17 Co3 Gd3 O18 78.3(3) . .
O6 Co3 Gd3 O18 168.1(3) . .
N6 Co3 Gd3 O18 109.1(6) . .
N7 Co3 Gd3 O18 -71.7(3) . .
O7 Co3 Gd3 O16 123.4(4) . .
O17 Co3 Gd3 O16 -162.9(4) . .
O6 Co3 Gd3 O16 -73.1(4) . .
N6 Co3 Gd3 O16 -132.2(6) . .
N7 Co3 Gd3 O16 47.1(4) . .
O16 Co3 Gd3 O27' 146.6(6) . .
O7 Co3 Gd3 O27' -90.0(5) . .
O17 Co3 Gd3 O27' -16.3(5) . .
O6 Co3 Gd3 O27' 73.5(5) . .
N6 Co3 Gd3 O27' 14.4(7) . .
N7 Co3 Gd3 O27' -166.3(5) . .
O16 Co3 Gd3 O17 162.9(4) . .
O7 Co3 Gd3 O17 -73.7(3) . .
O6 Co3 Gd3 O17 89.8(4) . .
N6 Co3 Gd3 O17 30.7(6) . .
N7 Co3 Gd3 O17 -150.0(4) . .
O16 Co3 Gd3 O11 -113.3(4) . .
O7 Co3 Gd3 O11 10.1(3) . .
O17 Co3 Gd3 O11 83.8(4) . .
O6 Co3 Gd3 O11 173.6(3) . .
N6 Co3 Gd3 O11 114.5(6) . .
N7 Co3 Gd3 O11 -66.2(4) . .
O16 Co3 Gd3 Co1 -68.9(3) . .
O7 Co3 Gd3 Co1 54.6(2) . .
O17 Co3 Gd3 Co1 128.2(3) . .
O6 Co3 Gd3 Co1 -141.9(2) . .
N6 Co3 Gd3 Co1 159.0(6) . .
N7 Co3 Gd3 Co1 -21.8(3) . .
O16 Co3 Gd3 Gd1 4.2(3) . .
O7 Co3 Gd3 Gd1 127.7(2) . .
O17 Co3 Gd3 Gd1 -158.7(3) . .
O6 Co3 Gd3 Gd1 -68.8(2) . .
N6 Co3 Gd3 Gd1 -127.9(6) . .
N7 Co3 Gd3 Gd1 51.4(3) . .
O9 Co1 Gd3 O1W -152.0(5) . .
O11 Co1 Gd3 O1W 12.1(5) . .
N2 Co1 Gd3 O1W 163.1(5) . .
O2 Co1 Gd3 O1W 87.7(4) . .
O1 Co1 Gd3 O1W -81.1(4) . .
N1 Co1 Gd3 O1W -15.9(7) . .
Gd4 Co1 Gd3 O1W 53.2(4) . .
O11 Co1 Gd3 O9 164.1(4) . .
N2 Co1 Gd3 O9 -44.9(5) . .
O2 Co1 Gd3 O9 -120.4(3) . .
O1 Co1 Gd3 O9 70.8(3) . .
N1 Co1 Gd3 O9 136.1(6) . .
Gd4 Co1 Gd3 O9 -154.9(3) . .
O9 Co1 Gd3 O15 -49.4(4) . .
O11 Co1 Gd3 O15 114.7(4) . .
N2 Co1 Gd3 O15 -94.4(5) . .
O2 Co1 Gd3 O15 -169.8(3) . .
O1 Co1 Gd3 O15 21.4(4) . .
N1 Co1 Gd3 O15 86.7(6) . .
Gd4 Co1 Gd3 O15 155.7(3) . .
O9 Co1 Gd3 O10 -76.9(4) . .
O11 Co1 Gd3 O10 87.1(3) . .
N2 Co1 Gd3 O10 -121.9(4) . .
O2 Co1 Gd3 O10 162.7(3) . .
O1 Co1 Gd3 O10 -6.1(3) . .
N1 Co1 Gd3 O10 59.1(5) . .
Gd4 Co1 Gd3 O10 128.2(2) . .
O9 Co1 Gd3 O18 118.8(3) . .
O11 Co1 Gd3 O18 -77.1(3) . .
N2 Co1 Gd3 O18 73.9(4) . .
O2 Co1 Gd3 O18 -1.6(2) . .
O1 Co1 Gd3 O18 -170.4(2) . .
N1 Co1 Gd3 O18 -105.1(5) . .
Gd4 Co1 Gd3 O18 -36.06(15) . .
O9 Co1 Gd3 O16 35.3(3) . .
O11 Co1 Gd3 O16 -160.7(3) . .
N2 Co1 Gd3 O16 -9.7(4) . .
O2 Co1 Gd3 O16 -85.1(2) . .
O1 Co1 Gd3 O16 106.1(3) . .
N1 Co1 Gd3 O16 171.4(5) . .
Gd4 Co1 Gd3 O16 -119.58(18) . .
O9 Co1 Gd3 O27' -146.4(6) . .
O11 Co1 Gd3 O27' 17.7(6) . .
N2 Co1 Gd3 O27' 168.7(6) . .
O2 Co1 Gd3 O27' 93.3(5) . .
O1 Co1 Gd3 O27' -75.5(5) . .
N1 Co1 Gd3 O27' -10.3(7) . .
Gd4 Co1 Gd3 O27' 58.8(5) . .
O9 Co1 Gd3 O17 114.3(4) . .
O11 Co1 Gd3 O17 -81.6(3) . .
N2 Co1 Gd3 O17 69.4(4) . .
O2 Co1 Gd3 O17 -6.1(3) . .
O1 Co1 Gd3 O17 -174.9(3) . .
N1 Co1 Gd3 O17 -109.6(5) . .
Gd4 Co1 Gd3 O17 -40.6(2) . .
O9 Co1 Gd3 O11 -164.1(4) . .
N2 Co1 Gd3 O11 151.0(5) . .
O2 Co1 Gd3 O11 75.6(3) . .
O1 Co1 Gd3 O11 -93.3(3) . .
N1 Co1 Gd3 O11 -28.0(6) . .
Gd4 Co1 Gd3 O11 41.1(3) . .
O9 Co1 Gd3 Co3 69.2(3) . .
O11 Co1 Gd3 Co3 -126.7(3) . .
N2 Co1 Gd3 Co3 24.3(4) . .
O2 Co1 Gd3 Co3 -51.13(17) . .
O1 Co1 Gd3 Co3 140.03(18) . .
N1 Co1 Gd3 Co3 -154.7(5) . .
Gd4 Co1 Gd3 Co3 -85.64(4) . .
O9 Co1 Gd3 Gd1 -42.4(3) . .
O11 Co1 Gd3 Gd1 121.7(3) . .
N2 Co1 Gd3 Gd1 -87.3(4) . .
O2 Co1 Gd3 Gd1 -162.76(17) . .
O1 Co1 Gd3 Gd1 28.41(18) . .
N1 Co1 Gd3 Gd1 93.7(5) . .
Gd4 Co1 Gd3 Gd1 162.74(3) . .
O14 Gd1 Gd3 O1W -121.2(5) . .
O10 Gd1 Gd3 O1W -14.3(5) . .
O10W Gd1 Gd3 O1W -140.2(4) 6_575 .
O10W Gd1 Gd3 O1W -158.7(4) . .
O9 Gd1 Gd3 O1W 136.4(5) . .
O9 Gd1 Gd3 O1W -57.4(4) 6_575 .
O1 Gd1 Gd3 O1W 73.4(4) . .
O1 Gd1 Gd3 O1W 13.1(5) 6_575 .
O9W Gd1 Gd3 O1W 115.4(4) 6_575 .
O9W Gd1 Gd3 O1W 120.8(4) . .
Gd3 Gd1 Gd3 O1W -52.1(4) 6_575 .
O14 Gd1 Gd3 O9 102.5(3) . .
O10 Gd1 Gd3 O9 -150.7(4) . .
O10W Gd1 Gd3 O9 83.5(3) 6_575 .
O10W Gd1 Gd3 O9 64.9(3) . .
O9 Gd1 Gd3 O9 166.2(4) 6_575 .
O1 Gd1 Gd3 O9 -62.9(3) . .
O1 Gd1 Gd3 O9 -123.3(3) 6_575 .
O9W Gd1 Gd3 O9 -20.9(3) 6_575 .
O9W Gd1 Gd3 O9 -15.6(3) . .
Gd3 Gd1 Gd3 O9 171.5(2) 6_575 .
O14 Gd1 Gd3 O15 -43.6(3) . .
O10 Gd1 Gd3 O15 63.2(4) . .
O10W Gd1 Gd3 O15 -62.6(2) 6_575 .
O10W Gd1 Gd3 O15 -81.2(2) . .
O9 Gd1 Gd3 O15 -146.1(3) . .
O9 Gd1 Gd3 O15 20.1(2) 6_575 .
O1 Gd1 Gd3 O15 151.0(2) . .
O1 Gd1 Gd3 O15 90.6(3) 6_575 .
O9W Gd1 Gd3 O15 -167.0(2) 6_575 .
O9W Gd1 Gd3 O15 -161.71(19) . .
Gd3 Gd1 Gd3 O15 25.43(19) 6_575 .
O14 Gd1 Gd3 O10 -106.9(4) . .
O10W Gd1 Gd3 O10 -125.9(4) 6_575 .
O10W Gd1 Gd3 O10 -144.4(3) . .
O9 Gd1 Gd3 O10 150.7(4) . .
O9 Gd1 Gd3 O10 -43.2(3) 6_575 .
O1 Gd1 Gd3 O10 87.7(4) . .
O1 Gd1 Gd3 O10 27.3(4) 6_575 .
O9W Gd1 Gd3 O10 129.7(3) 6_575 .
O9W Gd1 Gd3 O10 135.0(3) . .
Gd3 Gd1 Gd3 O10 -37.8(3) 6_575 .
O14 Gd1 Gd3 O18 118.0(3) . .
O10 Gd1 Gd3 O18 -135.1(4) . .
O10W Gd1 Gd3 O18 99.0(2) 6_575 .
O10W Gd1 Gd3 O18 80.4(2) . .
O9 Gd1 Gd3 O18 15.5(3) . .
O9 Gd1 Gd3 O18 -178.3(2) 6_575 .
O1 Gd1 Gd3 O18 -47.4(2) . .
O1 Gd1 Gd3 O18 -107.8(3) 6_575 .
O9W Gd1 Gd3 O18 -5.4(2) 6_575 .
O9W Gd1 Gd3 O18 -0.06(18) . .
Gd3 Gd1 Gd3 O18 -172.92(17) 6_575 .
O14 Gd1 Gd3 O16 29.6(3) . .
O10 Gd1 Gd3 O16 136.5(4) . .
O10W Gd1 Gd3 O16 10.6(2) 6_575 .
O10W Gd1 Gd3 O16 -7.9(2) . .
O9 Gd1 Gd3 O16 -72.8(3) . .
O9 Gd1 Gd3 O16 93.3(2) 6_575 .
O1 Gd1 Gd3 O16 -135.8(2) . .
O1 Gd1 Gd3 O16 163.8(3) 6_575 .
O9W Gd1 Gd3 O16 -93.8(2) 6_575 .
O9W Gd1 Gd3 O16 -88.46(19) . .
Gd3 Gd1 Gd3 O16 98.69(18) 6_575 .
O14 Gd1 Gd3 O27' -115.1(5) . .
O10 Gd1 Gd3 O27' -8.2(6) . .
O10W Gd1 Gd3 O27' -134.1(5) 6_575 .
O10W Gd1 Gd3 O27' -152.7(5) . .
O9 Gd1 Gd3 O27' 142.4(6) . .
O9 Gd1 Gd3 O27' -51.4(5) 6_575 .
O1 Gd1 Gd3 O27' 79.5(5) . .
O1 Gd1 Gd3 O27' 19.1(5) 6_575 .
O9W Gd1 Gd3 O27' 121.5(5) 6_575 .
O9W Gd1 Gd3 O27' 126.8(5) . .
Gd3 Gd1 Gd3 O27' -46.0(5) 6_575 .
O14 Gd1 Gd3 O17 -2.5(4) . .
O10 Gd1 Gd3 O17 104.3(5) . .
O10W Gd1 Gd3 O17 -21.5(4) 6_575 .
O10W Gd1 Gd3 O17 -40.1(4) . .
O9 Gd1 Gd3 O17 -105.0(4) . .
O9 Gd1 Gd3 O17 61.2(4) 6_575 .
O1 Gd1 Gd3 O17 -167.9(4) . .
O1 Gd1 Gd3 O17 131.7(4) 6_575 .
O9W Gd1 Gd3 O17 -125.9(4) 6_575 .
O9W Gd1 Gd3 O17 -120.6(4) . .
Gd3 Gd1 Gd3 O17 66.5(4) 6_575 .
O14 Gd1 Gd3 O11 170.7(2) . .
O10 Gd1 Gd3 O11 -82.4(3) . .
O10W Gd1 Gd3 O11 151.7(2) 6_575 .
O10W Gd1 Gd3 O11 133.1(2) . .
O9 Gd1 Gd3 O11 68.2(3) . .
O9 Gd1 Gd3 O11 -125.6(2) 6_575 .
O1 Gd1 Gd3 O11 5.3(2) . .
O1 Gd1 Gd3 O11 -55.1(2) 6_575 .
O9W Gd1 Gd3 O11 47.29(19) 6_575 .
O9W Gd1 Gd3 O11 52.61(16) . .
Gd3 Gd1 Gd3 O11 -120.25(15) 6_575 .
O14 Gd1 Gd3 Co3 27.2(2) . .
O10 Gd1 Gd3 Co3 134.1(3) . .
O10W Gd1 Gd3 Co3 8.20(17) 6_575 .
O10W Gd1 Gd3 Co3 -10.37(16) . .
O9 Gd1 Gd3 Co3 -75.3(2) . .
O9 Gd1 Gd3 Co3 90.92(16) 6_575 .
O1 Gd1 Gd3 Co3 -138.20(17) . .
O1 Gd1 Gd3 Co3 161.4(2) 6_575 .
O9W Gd1 Gd3 Co3 -96.20(11) 6_575 .
O9W Gd1 Gd3 Co3 -90.88(6) . .
Gd3 Gd1 Gd3 Co3 96.26(4) 6_575 .
O14 Gd1 Gd3 Co1 140.7(2) . .
O10 Gd1 Gd3 Co1 -112.4(3) . .
O10W Gd1 Gd3 Co1 121.74(17) 6_575 .
O10W Gd1 Gd3 Co1 103.16(15) . .
O9 Gd1 Gd3 Co1 38.3(2) . .
O9 Gd1 Gd3 Co1 -155.54(16) 6_575 .
O1 Gd1 Gd3 Co1 -24.67(17) . .
O1 Gd1 Gd3 Co1 -85.0(2) 6_575 .
O9W Gd1 Gd3 Co1 17.34(11) 6_575 .
O9W Gd1 Gd3 Co1 22.66(5) . .
Gd3 Gd1 Gd3 Co1 -150.20(3) 6_575 .
O9 Co1 Gd4 O11 -62.1(3) . .
N2 Co1 Gd4 O11 -162.4(4) . .
O2 Co1 Gd4 O11 -168.7(4) . .
O1 Co1 Gd4 O11 28.5(4) . .
N1 Co1 Gd4 O11 107.5(3) . .
Gd3 Co1 Gd4 O11 -45.1(3) . .
O9 Co1 Gd4 O12 -166.6(4) . .
O11 Co1 Gd4 O12 -104.4(4) . .
N2 Co1 Gd4 O12 93.2(4) . .
O2 Co1 Gd4 O12 86.9(4) . .
O1 Co1 Gd4 O12 -75.9(4) . .
N1 Co1 Gd4 O12 3.1(4) . .
Gd3 Co1 Gd4 O12 -149.5(3) . .
O9 Co1 Gd4 O18 19.6(3) . .
O11 Co1 Gd4 O18 81.7(3) . .
N2 Co1 Gd4 O18 -80.7(4) . .
O2 Co1 Gd4 O18 -87.0(3) . .
O1 Co1 Gd4 O18 110.2(3) . .
N1 Co1 Gd4 O18 -170.8(3) . .
Gd3 Co1 Gd4 O18 36.62(17) . .
O9 Co1 Gd4 O19 51.9(3) . .
O11 Co1 Gd4 O19 114.0(4) . .
N2 Co1 Gd4 O19 -48.4(4) . .
O2 Co1 Gd4 O19 -54.7(4) . .
O1 Co1 Gd4 O19 142.5(4) . .
N1 Co1 Gd4 O19 -138.5(3) . .
Gd3 Co1 Gd4 O19 68.9(3) . .
O9 Co1 Gd4 O26 -34.7(3) . .
O11 Co1 Gd4 O26 27.4(3) . .
N2 Co1 Gd4 O26 -135.0(4) . .
O2 Co1 Gd4 O26 -141.3(3) . .
O1 Co1 Gd4 O26 55.9(3) . .
N1 Co1 Gd4 O26 134.9(3) . .
Gd3 Co1 Gd4 O26 -17.64(16) . .
O9 Co1 Gd4 O3 126.6(2) . .
O11 Co1 Gd4 O3 -171.3(3) . .
N2 Co1 Gd4 O3 26.3(4) . .
O2 Co1 Gd4 O3 20.0(3) . .
O1 Co1 Gd4 O3 -142.8(3) . .
N1 Co1 Gd4 O3 -63.8(3) . .
Gd3 Co1 Gd4 O3 143.62(14) . .
O9 Co1 Gd4 O2 106.6(3) . .
O11 Co1 Gd4 O2 168.7(4) . .
N2 Co1 Gd4 O2 6.3(4) . .
O1 Co1 Gd4 O2 -162.8(4) . .
N1 Co1 Gd4 O2 -83.8(3) . .
Gd3 Co1 Gd4 O2 123.7(3) . .
O9 Co1 Gd4 O23 -161.7(3) . .
O11 Co1 Gd4 O23 -99.6(3) . .
N2 Co1 Gd4 O23 98.0(4) . .
O2 Co1 Gd4 O23 91.7(3) . .
O1 Co1 Gd4 O23 -71.1(3) . .
N1 Co1 Gd4 O23 7.9(3) . .
Gd3 Co1 Gd4 O23 -144.69(19) . .
O9 Co1 Gd4 O24 -113.7(3) . .
O11 Co1 Gd4 O24 -51.6(3) . .
N2 Co1 Gd4 O24 146.1(4) . .
O2 Co1 Gd4 O24 139.7(3) . .
O1 Co1 Gd4 O24 -23.0(3) . .
N1 Co1 Gd4 O24 56.0(3) . .
Gd3 Co1 Gd4 O24 -96.62(19) . .
O9 Co1 Gd4 N9 -137.6(3) . .
O11 Co1 Gd4 N9 -75.5(4) . .
N2 Co1 Gd4 N9 122.1(4) . .
O2 Co1 Gd4 N9 115.8(4) . .
O1 Co1 Gd4 N9 -47.0(4) . .
N1 Co1 Gd4 N9 32.0(3) . .
Gd3 Co1 Gd4 N9 -120.6(3) . .
O9 Co1 Gd4 Gd5 11.0(2) . .
O11 Co1 Gd4 Gd5 73.2(3) . .
N2 Co1 Gd4 Gd5 -89.2(3) . .
O2 Co1 Gd4 Gd5 -95.5(3) . .
O1 Co1 Gd4 Gd5 101.7(3) . .
N1 Co1 Gd4 Gd5 -179.3(2) . .
Gd3 Co1 Gd4 Gd5 28.10(3) . .
O11 Gd4 Gd5 O17 2.4(2) . .
O12 Gd4 Gd5 O17 147.8(2) . .
O18 Gd4 Gd5 O17 -43.2(3) . .
O19 Gd4 Gd5 O17 -170.1(3) . .
O26 Gd4 Gd5 O17 72.7(3) . .
O3 Gd4 Gd5 O17 -141.0(2) . .
O2 Gd4 Gd5 O17 -69.3(2) . .
O23 Gd4 Gd5 O17 88.8(13) . .
O24 Gd4 Gd5 O17 74.9(3) . .
N9 Gd4 Gd5 O17 77.6(4) . .
Co1 Gd4 Gd5 O17 -30.95(17) . .
O11 Gd4 Gd5 O20 -143.9(2) . .
O12 Gd4 Gd5 O20 1.4(2) . .
O18 Gd4 Gd5 O20 170.4(3) . .
O19 Gd4 Gd5 O20 43.6(3) . .
O26 Gd4 Gd5 O20 -73.7(3) . .
O3 Gd4 Gd5 O20 72.6(2) . .
O2 Gd4 Gd5 O20 144.3(2) . .
O23 Gd4 Gd5 O20 -57.6(13) . .
O24 Gd4 Gd5 O20 -71.5(3) . .
N9 Gd4 Gd5 O20 -68.7(4) . .
Co1 Gd4 Gd5 O20 -177.31(16) . .
O11 Gd4 Gd5 O19 172.5(3) . .
O12 Gd4 Gd5 O19 -42.2(3) . .
O18 Gd4 Gd5 O19 126.9(3) . .
O26 Gd4 Gd5 O19 -117.2(3) . .
O3 Gd4 Gd5 O19 29.1(3) . .
O2 Gd4 Gd5 O19 100.8(3) . .
O23 Gd4 Gd5 O19 -101.1(13) . .
O24 Gd4 Gd5 O19 -115.0(3) . .
N9 Gd4 Gd5 O19 -112.3(5) . .
Co1 Gd4 Gd5 O19 139.1(2) . .
O11 Gd4 Gd5 O7 73.3(2) . .
O12 Gd4 Gd5 O7 -141.4(2) . .
O18 Gd4 Gd5 O7 27.6(3) . .
O19 Gd4 Gd5 O7 -99.2(3) . .
O26 Gd4 Gd5 O7 143.5(3) . .
O3 Gd4 Gd5 O7 -70.2(2) . .
O2 Gd4 Gd5 O7 1.5(2) . .
O23 Gd4 Gd5 O7 159.6(13) . .
O24 Gd4 Gd5 O7 145.8(3) . .
N9 Gd4 Gd5 O7 148.5(5) . .
Co1 Gd4 Gd5 O7 39.90(17) . .
O11 Gd4 Gd5 O18 45.7(3) . .
O12 Gd4 Gd5 O18 -169.0(3) . .
O19 Gd4 Gd5 O18 -126.9(3) . .
O26 Gd4 Gd5 O18 115.9(3) . .
O3 Gd4 Gd5 O18 -97.8(3) . .
O2 Gd4 Gd5 O18 -26.1(3) . .
O23 Gd4 Gd5 O18 132.0(13) . .
O24 Gd4 Gd5 O18 118.1(3) . .
N9 Gd4 Gd5 O18 120.8(5) . .
Co1 Gd4 Gd5 O18 12.3(2) . .
O11 Gd4 Gd5 O26 -70.2(3) . .
O12 Gd4 Gd5 O26 75.1(3) . .
O18 Gd4 Gd5 O26 -115.9(3) . .
O19 Gd4 Gd5 O26 117.2(3) . .
O3 Gd4 Gd5 O26 146.3(3) . .
O2 Gd4 Gd5 O26 -142.0(3) . .
O23 Gd4 Gd5 O26 16.1(13) . .
O24 Gd4 Gd5 O26 2.2(3) . .
N9 Gd4 Gd5 O26 4.9(5) . .
Co1 Gd4 Gd5 O26 -103.6(2) . .
O11 Gd4 Gd5 O8 145.3(2) . .
O12 Gd4 Gd5 O8 -69.4(2) . .
O18 Gd4 Gd5 O8 99.6(3) . .
O19 Gd4 Gd5 O8 -27.3(3) . .
O26 Gd4 Gd5 O8 -144.5(3) . .
O3 Gd4 Gd5 O8 1.8(2) . .
O2 Gd4 Gd5 O8 73.5(2) . .
O23 Gd4 Gd5 O8 -128.4(13) . .
O24 Gd4 Gd5 O8 -142.3(3) . .
N9 Gd4 Gd5 O8 -139.6(4) . .
Co1 Gd4 Gd5 O8 111.86(17) . .
O11 Gd4 Gd5 O30 -64.0(16) . .
O12 Gd4 Gd5 O30 81.3(16) . .
O18 Gd4 Gd5 O30 -109.7(17) . .
O19 Gd4 Gd5 O30 123.5(17) . .
O26 Gd4 Gd5 O30 6.2(17) . .
O3 Gd4 Gd5 O30 152.5(16) . .
O2 Gd4 Gd5 O30 -135.8(16) . .
O23 Gd4 Gd5 O30 22(2) . .
O24 Gd4 Gd5 O30 8.5(17) . .
N9 Gd4 Gd5 O30 11.2(17) . .
Co1 Gd4 Gd5 O30 -97.4(16) . .
O11 Gd4 Gd5 O29 -71.4(3) . .
O12 Gd4 Gd5 O29 73.9(3) . .
O18 Gd4 Gd5 O29 -117.0(3) . .
O19 Gd4 Gd5 O29 116.1(3) . .
O26 Gd4 Gd5 O29 -1.1(3) . .
O3 Gd4 Gd5 O29 145.2(3) . .
O2 Gd4 Gd5 O29 -143.1(3) . .
O23 Gd4 Gd5 O29 15.0(13) . .
O24 Gd4 Gd5 O29 1.1(3) . .
N9 Gd4 Gd5 O29 3.8(5) . .
Co1 Gd4 Gd5 O29 -104.8(2) . .
O11 Gd4 Gd5 N11 -72.1(4) . .
O12 Gd4 Gd5 N11 73.2(5) . .
O18 Gd4 Gd5 N11 -117.8(5) . .
O19 Gd4 Gd5 N11 115.3(5) . .
O26 Gd4 Gd5 N11 -1.9(5) . .
O3 Gd4 Gd5 N11 144.4(4) . .
O2 Gd4 Gd5 N11 -143.9(5) . .
O23 Gd4 Gd5 N11 14.2(14) . .
O24 Gd4 Gd5 N11 0.3(5) . .
N9 Gd4 Gd5 N11 3.0(6) . .
Co1 Gd4 Gd5 N11 -105.5(4) . .
O11 Gd4 Gd5 Gd3 7.14(16) . .
O12 Gd4 Gd5 Gd3 152.45(16) . .
O18 Gd4 Gd5 Gd3 -38.5(2) . .
O19 Gd4 Gd5 Gd3 -165.4(2) . .
O26 Gd4 Gd5 Gd3 77.4(2) . .
O3 Gd4 Gd5 Gd3 -136.34(16) . .
O2 Gd4 Gd5 Gd3 -64.62(17) . .
O23 Gd4 Gd5 Gd3 93.5(13) . .
O24 Gd4 Gd5 Gd3 79.6(2) . .
N9 Gd4 Gd5 Gd3 82.3(4) . .
Co1 Gd4 Gd5 Gd3 -26.25(3) . .
O1W Gd3 Gd5 O17 91.5(5) . .
O9 Gd3 Gd5 O17 -129.7(3) . .
O15 Gd3 Gd5 O17 17.2(3) . .
O10 Gd3 Gd5 O17 102.6(5) . .
O18 Gd3 Gd5 O17 -144.3(3) . .
O16 Gd3 Gd5 O17 -54.4(3) . .
O27' Gd3 Gd5 O17 86.7(6) . .
O11 Gd3 Gd5 O17 165.7(3) . .
Co3 Gd3 Gd5 O17 -41.2(3) . .
Co1 Gd3 Gd5 O17 -162.3(3) . .
Gd1 Gd3 Gd5 O17 -138.1(3) . .
O1W Gd3 Gd5 O20 -19.3(5) . .
O9 Gd3 Gd5 O20 119.5(4) . .
O15 Gd3 Gd5 O20 -93.5(4) . .
O10 Gd3 Gd5 O20 -8.1(6) . .
O18 Gd3 Gd5 O20 104.9(4) . .
O16 Gd3 Gd5 O20 -165.2(4) . .
O27' Gd3 Gd5 O20 -24.1(6) . .
O17 Gd3 Gd5 O20 -110.8(4) . .
O11 Gd3 Gd5 O20 54.9(3) . .
Co3 Gd3 Gd5 O20 -152.0(3) . .
Co1 Gd3 Gd5 O20 86.9(3) . .
Gd1 Gd3 Gd5 O20 111.1(3) . .
O1W Gd3 Gd5 O19 -90.8(4) . .
O9 Gd3 Gd5 O19 48.0(2) . .
O15 Gd3 Gd5 O19 -165.0(3) . .
O10 Gd3 Gd5 O19 -79.7(5) . .
O18 Gd3 Gd5 O19 33.4(3) . .
O16 Gd3 Gd5 O19 123.3(2) . .
O27' Gd3 Gd5 O19 -95.6(5) . .
O17 Gd3 Gd5 O19 177.7(3) . .
O11 Gd3 Gd5 O19 -16.6(2) . .
Co3 Gd3 Gd5 O19 136.47(16) . .
Co1 Gd3 Gd5 O19 15.37(16) . .
Gd1 Gd3 Gd5 O19 39.64(17) . .
O1W Gd3 Gd5 O7 161.1(4) . .
O9 Gd3 Gd5 O7 -60.1(3) . .
O15 Gd3 Gd5 O7 86.9(3) . .
O10 Gd3 Gd5 O7 172.3(5) . .
O18 Gd3 Gd5 O7 -74.6(3) . .
O16 Gd3 Gd5 O7 15.2(3) . .
O27' Gd3 Gd5 O7 156.3(5) . .
O17 Gd3 Gd5 O7 69.7(3) . .
O11 Gd3 Gd5 O7 -124.6(2) . .
Co3 Gd3 Gd5 O7 28.42(19) . .
Co1 Gd3 Gd5 O7 -92.69(19) . .
Gd1 Gd3 Gd5 O7 -68.4(2) . .
O1W Gd3 Gd5 O18 -124.2(5) . .
O9 Gd3 Gd5 O18 14.5(3) . .
O15 Gd3 Gd5 O18 161.5(3) . .
O10 Gd3 Gd5 O18 -113.1(5) . .
O16 Gd3 Gd5 O18 89.9(3) . .
O27' Gd3 Gd5 O18 -129.1(5) . .
O17 Gd3 Gd5 O18 144.3(3) . .
O11 Gd3 Gd5 O18 -50.0(3) . .
Co3 Gd3 Gd5 O18 103.0(2) . .
Co1 Gd3 Gd5 O18 -18.1(2) . .
Gd1 Gd3 Gd5 O18 6.2(2) . .
O1W Gd3 Gd5 O26 -33.4(4) . .
O9 Gd3 Gd5 O26 105.4(3) . .
O15 Gd3 Gd5 O26 -107.6(3) . .
O10 Gd3 Gd5 O26 -22.2(5) . .
O18 Gd3 Gd5 O26 90.9(3) . .
O16 Gd3 Gd5 O26 -179.3(3) . .
O27' Gd3 Gd5 O26 -38.2(5) . .
O17 Gd3 Gd5 O26 -124.9(3) . .
O11 Gd3 Gd5 O26 40.8(3) . .
Co3 Gd3 Gd5 O26 -166.1(2) . .
Co1 Gd3 Gd5 O26 72.8(2) . .
Gd1 Gd3 Gd5 O26 97.1(2) . .
O1W Gd3 Gd5 O8 -170.5(5) . .
O9 Gd3 Gd5 O8 -31.7(3) . .
O15 Gd3 Gd5 O8 115.2(3) . .
O10 Gd3 Gd5 O8 -159.4(5) . .
O18 Gd3 Gd5 O8 -46.3(3) . .
O16 Gd3 Gd5 O8 43.6(3) . .
O27' Gd3 Gd5 O8 -175.3(6) . .
O17 Gd3 Gd5 O8 98.0(4) . .
O11 Gd3 Gd5 O8 -96.3(3) . .
Co3 Gd3 Gd5 O8 56.8(3) . .
Co1 Gd3 Gd5 O8 -64.3(3) . .
Gd1 Gd3 Gd5 O8 -40.1(3) . .
O1W Gd3 Gd5 O30 92.5(4) . .
O9 Gd3 Gd5 O30 -128.8(3) . .
O15 Gd3 Gd5 O30 18.2(3) . .
O10 Gd3 Gd5 O30 103.6(5) . .
O18 Gd3 Gd5 O30 -143.3(3) . .
O16 Gd3 Gd5 O30 -53.4(3) . .
O27' Gd3 Gd5 O30 87.6(5) . .
O17 Gd3 Gd5 O30 1.0(3) . .
O11 Gd3 Gd5 O30 166.7(2) . .
Co3 Gd3 Gd5 O30 -40.26(19) . .
Co1 Gd3 Gd5 O30 -161.37(19) . .
Gd1 Gd3 Gd5 O30 -137.1(2) . .
O1W Gd3 Gd5 O29 43.2(4) . .
O9 Gd3 Gd5 O29 -178.0(2) . .
O15 Gd3 Gd5 O29 -31.0(3) . .
O10 Gd3 Gd5 O29 54.4(5) . .
O18 Gd3 Gd5 O29 167.5(3) . .
O16 Gd3 Gd5 O29 -102.7(2) . .
O27' Gd3 Gd5 O29 38.4(5) . .
O17 Gd3 Gd5 O29 -48.2(3) . .
O11 Gd3 Gd5 O29 117.5(2) . .
Co3 Gd3 Gd5 O29 -89.48(16) . .
Co1 Gd3 Gd5 O29 149.41(16) . .
Gd1 Gd3 Gd5 O29 173.68(17) . .
O1W Gd3 Gd5 N11 67.1(4) . .
O9 Gd3 Gd5 N11 -154.1(3) . .
O15 Gd3 Gd5 N11 -7.1(3) . .
O10 Gd3 Gd5 N11 78.3(5) . .
O18 Gd3 Gd5 N11 -168.6(3) . .
O16 Gd3 Gd5 N11 -78.8(3) . .
O27' Gd3 Gd5 N11 62.3(5) . .
O17 Gd3 Gd5 N11 -24.3(3) . .
O11 Gd3 Gd5 N11 141.4(3) . .
Co3 Gd3 Gd5 N11 -65.6(2) . .
Co1 Gd3 Gd5 N11 173.3(2) . .
Gd1 Gd3 Gd5 N11 -162.4(2) . .
O1W Gd3 Gd5 Gd4 -80.9(4) . .
O9 Gd3 Gd5 Gd4 57.87(19) . .
O15 Gd3 Gd5 Gd4 -155.1(2) . .
O10 Gd3 Gd5 Gd4 -69.8(5) . .
O18 Gd3 Gd5 Gd4 43.3(2) . .
O16 Gd3 Gd5 Gd4 133.19(19) . .
O27' Gd3 Gd5 Gd4 -85.7(5) . .
O17 Gd3 Gd5 Gd4 -172.4(3) . .
O11 Gd3 Gd5 Gd4 -6.68(15) . .
Co3 Gd3 Gd5 Gd4 146.37(4) . .
Co1 Gd3 Gd5 Gd4 25.27(3) . .
Gd1 Gd3 Gd5 Gd4 49.54(7) . .
O21 Co4 Gd6 O19 120.6(3) . .
O20 Co4 Gd6 O19 -78.2(3) . .
O8 Co4 Gd6 O19 -3.7(3) . .
O5 Co4 Gd6 O19 -166.8(3) 2_656 .
N8 Co4 Gd6 O19 71.3(3) . .
N5 Co4 Gd6 O19 -106.7(5) 2_656 .
O21 Co4 Gd6 O27 -147.0(6) . .
O20 Co4 Gd6 O27 14.2(6) . .
O8 Co4 Gd6 O27 88.7(5) . .
O5 Co4 Gd6 O27 -74.4(5) 2_656 .
N8 Co4 Gd6 O27 163.7(5) . .
N5 Co4 Gd6 O27 -14.3(7) 2_656 .
O21 Co4 Gd6 O1W' -153.2(5) . .
O20 Co4 Gd6 O1W' 8.1(5) . .
O8 Co4 Gd6 O1W' 82.6(5) . .
O5 Co4 Gd6 O1W' -80.5(5) 2_656 .
N8 Co4 Gd6 O1W' 157.6(5) . .
N5 Co4 Gd6 O1W' -20.5(6) 2_656 .
O21 Co4 Gd6 O22 -76.7(3) . .
O20 Co4 Gd6 O22 84.6(3) . .
O8 Co4 Gd6 O22 159.1(3) . .
O5 Co4 Gd6 O22 -4.0(2) 2_656 .
N8 Co4 Gd6 O22 -125.9(3) . .
N5 Co4 Gd6 O22 56.1(5) 2_656 .
O21 Co4 Gd6 O22 -50.2(4) . 2_656
O20 Co4 Gd6 O22 111.0(4) . 2_656
O8 Co4 Gd6 O22 -174.5(3) . 2_656
O5 Co4 Gd6 O22 22.5(3) 2_656 2_656
N8 Co4 Gd6 O22 -99.5(4) . 2_656
N5 Co4 Gd6 O22 82.5(5) 2_656 2_656
O20 Co4 Gd6 O21 161.2(4) . .
O8 Co4 Gd6 O21 -124.3(3) . .
O5 Co4 Gd6 O21 72.7(3) 2_656 .
N8 Co4 Gd6 O21 -49.3(4) . .
N5 Co4 Gd6 O21 132.7(5) 2_656 .
O21 Co4 Gd6 O13 35.3(3) . .
O20 Co4 Gd6 O13 -163.4(3) . .
O8 Co4 Gd6 O13 -88.9(3) . .
O5 Co4 Gd6 O13 108.0(2) 2_656 .
N8 Co4 Gd6 O13 -13.9(3) . .
N5 Co4 Gd6 O13 168.0(5) 2_656 .
O21 Co4 Gd6 O12 113.2(4) . .
O20 Co4 Gd6 O12 -85.6(4) . .
O8 Co4 Gd6 O12 -11.0(3) . .
O5 Co4 Gd6 O12 -174.1(3) 2_656 .
N8 Co4 Gd6 O12 64.0(4) . .
N5 Co4 Gd6 O12 -114.1(5) 2_656 .
O21 Co4 Gd6 O20 -161.2(4) . .
O8 Co4 Gd6 O20 74.5(3) . .
O5 Co4 Gd6 O20 -88.6(3) 2_656 .
N8 Co4 Gd6 O20 149.5(4) . .
N5 Co4 Gd6 O20 -28.5(5) 2_656 .
O21 Co4 Gd6 Co2 69.5(3) . .
O20 Co4 Gd6 Co2 -129.3(3) . .
O8 Co4 Gd6 Co2 -54.8(2) . .
O5 Co4 Gd6 Co2 142.15(19) 2_656 .
N8 Co4 Gd6 Co2 20.2(3) . .
N5 Co4 Gd6 Co2 -157.8(4) 2_656 .
O21 Co4 Gd6 Gd7 -43.1(3) . .
O20 Co4 Gd6 Gd7 118.2(3) . .
O8 Co4 Gd6 Gd7 -167.3(2) . .
O5 Co4 Gd6 Gd7 29.59(19) 2_656 .
N8 Co4 Gd6 Gd7 -92.3(3) . .
N5 Co4 Gd6 Gd7 89.6(5) 2_656 .
O13 Co2 Gd6 O19 -123.7(3) . .
O3 Co2 Gd6 O19 5.5(2) . .
O12 Co2 Gd6 O19 79.0(3) . .
O4 Co2 Gd6 O19 162.4(3) . .
N4 Co2 Gd6 O19 105.5(5) . .
N3 Co2 Gd6 O19 -69.8(3) . .
O13 Co2 Gd6 O27 144.8(4) . .
O3 Co2 Gd6 O27 -86.0(4) . .
O12 Co2 Gd6 O27 -12.5(4) . .
O4 Co2 Gd6 O27 71.0(4) . .
N4 Co2 Gd6 O27 14.0(6) . .
N3 Co2 Gd6 O27 -161.3(4) . .
O13 Co2 Gd6 O1W' 150.6(4) . .
O3 Co2 Gd6 O1W' -80.2(4) . .
O12 Co2 Gd6 O1W' -6.7(4) . .
O4 Co2 Gd6 O1W' 76.7(4) . .
N4 Co2 Gd6 O1W' 19.8(6) . .
N3 Co2 Gd6 O1W' -155.5(4) . .
O13 Co2 Gd6 O22 44.3(3) . .
O3 Co2 Gd6 O22 173.5(3) . .
O12 Co2 Gd6 O22 -113.0(3) . .
O4 Co2 Gd6 O22 -29.6(3) . .
N4 Co2 Gd6 O22 -86.5(5) . .
N3 Co2 Gd6 O22 98.2(3) . .
O13 Co2 Gd6 O22 75.6(3) . 2_656
O3 Co2 Gd6 O22 -155.3(2) . 2_656
O12 Co2 Gd6 O22 -81.7(3) . 2_656
O4 Co2 Gd6 O22 1.7(2) . 2_656
N4 Co2 Gd6 O22 -55.2(4) . 2_656
N3 Co2 Gd6 O22 129.5(3) . 2_656
O13 Co2 Gd6 O21 -38.2(3) . .
O3 Co2 Gd6 O21 91.0(2) . .
O12 Co2 Gd6 O21 164.5(3) . .
O4 Co2 Gd6 O21 -112.1(2) . .
N4 Co2 Gd6 O21 -169.0(4) . .
N3 Co2 Gd6 O21 15.7(3) . .
O3 Co2 Gd6 O13 129.1(3) . .
O12 Co2 Gd6 O13 -157.3(3) . .
O4 Co2 Gd6 O13 -73.9(3) . .
N4 Co2 Gd6 O13 -130.8(5) . .
N3 Co2 Gd6 O13 53.9(3) . .
O13 Co2 Gd6 O12 157.3(3) . .
O3 Co2 Gd6 O12 -73.6(3) . .
O4 Co2 Gd6 O12 83.4(3) . .
N4 Co2 Gd6 O12 26.5(5) . .
N3 Co2 Gd6 O12 -148.8(3) . .
O13 Co2 Gd6 O20 -115.2(3) . .
O3 Co2 Gd6 O20 14.0(3) . .
O12 Co2 Gd6 O20 87.5(3) . .
O4 Co2 Gd6 O20 171.0(3) . .
N4 Co2 Gd6 O20 114.0(5) . .
N3 Co2 Gd6 O20 -61.3(3) . .
O13 Co2 Gd6 Co4 -72.2(2) . .
O3 Co2 Gd6 Co4 56.93(19) . .
O12 Co2 Gd6 Co4 130.5(2) . .
O4 Co2 Gd6 Co4 -146.09(19) . .
N4 Co2 Gd6 Co4 157.0(4) . .
N3 Co2 Gd6 Co4 -18.3(3) . .
O13 Co2 Gd6 Gd7 1.1(2) . .
O3 Co2 Gd6 Gd7 130.24(18) . .
O12 Co2 Gd6 Gd7 -156.2(2) . .
O4 Co2 Gd6 Gd7 -72.79(19) . .
N4 Co2 Gd6 Gd7 -129.7(4) . .
N3 Co2 Gd6 Gd7 55.0(3) . .
O9 Co1 N1 C1 -147.3(9) . .
O11 Co1 N1 C1 95.4(10) . .
N2 Co1 N1 C1 -63.5(10) . .
O2 Co1 N1 C1 12.0(10) . .
O1 Co1 N1 C1 -174.6(11) . .
Gd3 Co1 N1 C1 115.7(9) . .
Gd4 Co1 N1 C1 54.6(10) . .
O9 Co1 N1 C5 27.5(12) . .
O11 Co1 N1 C5 -89.8(8) . .
N2 Co1 N1 C5 111.3(9) . .
O2 Co1 N1 C5 -173.2(8) . .
O1 Co1 N1 C5 0.2(8) . .
Gd3 Co1 N1 C5 -69.6(10) . .
Gd4 Co1 N1 C5 -130.7(8) . .
O9 Co1 N2 C12 -119.4(9) . .
O11 Co1 N2 C12 -38.5(14) . .
O2 Co1 N2 C12 -6.5(8) . .
O1 Co1 N2 C12 160.5(8) . .
N1 Co1 N2 C12 88.1(9) . .
Gd3 Co1 N2 C12 -91.4(9) . .
Gd4 Co1 N2 C12 -11.0(10) . .
O9 Co1 N2 C8 59.4(11) . .
O11 Co1 N2 C8 140.4(10) . .
O2 Co1 N2 C8 172.3(11) . .
O1 Co1 N2 C8 -20.7(12) . .
N1 Co1 N2 C8 -93.0(11) . .
Gd3 Co1 N2 C8 87.5(11) . .
Gd4 Co1 N2 C8 167.9(10) . .
O13 Co2 N3 C16 127.1(8) . .
O3 Co2 N3 C16 7.9(8) . .
O12 Co2 N3 C16 46.9(12) . .
O4 Co2 N3 C16 -155.2(7) . .
N4 Co2 N3 C16 -83.7(8) . .
Gd6 Co2 N3 C16 94.0(8) . .
O13 Co2 N3 C20 -51.4(9) . .
O3 Co2 N3 C20 -170.6(9) . .
O12 Co2 N3 C20 -131.6(8) . .
O4 Co2 N3 C20 26.4(10) . .
N4 Co2 N3 C20 97.8(9) . .
Gd6 Co2 N3 C20 -84.5(8) . .
O13 Co2 N4 C21 137.1(8) . .
O3 Co2 N4 C21 -28.7(9) . .
O12 Co2 N4 C21 -110.2(8) . .
O4 Co2 N4 C21 170.4(9) . .
N3 Co2 N4 C21 46.5(9) . .
Gd6 Co2 N4 C21 -129.4(8) . .
O13 Co2 N4 C25 -44.2(10) . .
O3 Co2 N4 C25 150.1(7) . .
O12 Co2 N4 C25 68.5(7) . .
O4 Co2 N4 C25 -10.9(7) . .
N3 Co2 N4 C25 -134.7(7) . .
Gd6 Co2 N4 C25 49.4(9) . .
O16 Co3 N6 C38 -39.5(14) . .
O7 Co3 N6 C38 162.2(11) . .
O17 Co3 N6 C38 80.4(11) . .
O6 Co3 N6 C38 -5.0(10) . .
N7 Co3 N6 C38 -121.5(11) . .
Gd3 Co3 N6 C38 57.9(13) . .
O16 Co3 N6 C34 138.0(9) . .
O7 Co3 N6 C34 -20.3(9) . .
O17 Co3 N6 C34 -102.1(9) . .
O6 Co3 N6 C34 172.5(10) . .
N7 Co3 N6 C34 56.0(9) . .
Gd3 Co3 N6 C34 -124.6(9) . .
O16 Co3 N7 C45 119.5(9) . .
O7 Co3 N7 C45 3.9(9) . .
O17 Co3 N7 C45 41.7(14) . .
O6 Co3 N7 C45 -161.9(8) . .
N6 Co3 N7 C45 -90.5(9) . .
Gd3 Co3 N7 C45 89.8(9) . .
O16 Co3 N7 C41 -53.1(11) . .
O7 Co3 N7 C41 -168.7(12) . .
O17 Co3 N7 C41 -130.9(11) . .
O6 Co3 N7 C41 25.5(13) . .
N6 Co3 N7 C41 96.9(12) . .
Gd3 Co3 N7 C41 -82.8(11) . .
O21 Co4 N8 C49 -123.1(7) . .
O20 Co4 N8 C49 -44.0(10) . .
O8 Co4 N8 C49 -6.0(7) . .
O5 Co4 N8 C49 159.1(7) 2_656 .
N5 Co4 N8 C49 86.8(7) 2_656 .
Gd6 Co4 N8 C49 -92.2(7) . .
O21 Co4 N8 C53 55.3(9) . .
O20 Co4 N8 C53 134.4(8) . .
O8 Co4 N8 C53 172.4(9) . .
O5 Co4 N8 C53 -22.5(9) 2_656 .
N5 Co4 N8 C53 -94.8(9) 2_656 .
Gd6 Co4 N8 C53 86.2(9) . .
O11 Gd4 N9 O23 -101.0(7) . .
O12 Gd4 N9 O23 98.0(7) . .
O18 Gd4 N9 O23 -105.5(7) . .
O19 Gd4 N9 O23 104.1(7) . .
O26 Gd4 N9 O23 179.8(6) . .
O3 Gd4 N9 O23 33.0(7) . .
O2 Gd4 N9 O23 -34.4(7) . .
O24 Gd4 N9 O23 -178.3(11) . .
Co1 Gd4 N9 O23 -66.2(6) . .
Gd5 Gd4 N9 O23 176.4(4) . .
O11 Gd4 N9 O25 -135(49) . .
O12 Gd4 N9 O25 64(49) . .
O18 Gd4 N9 O25 -139(49) . .
O19 Gd4 N9 O25 70(49) . .
O26 Gd4 N9 O25 146(49) . .
O3 Gd4 N9 O25 -1(49) . .
O2 Gd4 N9 O25 -68(49) . .
O23 Gd4 N9 O25 -34(49) . .
O24 Gd4 N9 O25 148(49) . .
Co1 Gd4 N9 O25 -100(49) . .
Gd5 Gd4 N9 O25 143(49) . .
O11 Gd4 N9 O24 77.3(6) . .
O12 Gd4 N9 O24 -83.7(6) . .
O18 Gd4 N9 O24 72.8(8) . .
O19 Gd4 N9 O24 -77.6(8) . .
O26 Gd4 N9 O24 -1.9(7) . .
O3 Gd4 N9 O24 -148.7(6) . .
O2 Gd4 N9 O24 143.9(6) . .
O23 Gd4 N9 O24 178.3(11) . .
Co1 Gd4 N9 O24 112.2(6) . .
Gd5 Gd4 N9 O24 -5.3(9) . .
O26 N10 O27 Gd6 5(3) . .
O28 N10 O27 Gd6 171.5(14) . .
O19 Gd6 O27 N10 -1.9(14) . .
O1W' Gd6 O27 N10 4(7) . .
O22 Gd6 O27 N10 -147.1(14) . .
O22 Gd6 O27 N10 142.4(14) 2_656 .
O21 Gd6 O27 N10 -104.6(14) . .
O13 Gd6 O27 N10 100.9(12) . .
O12 Gd6 O27 N10 63.5(13) . .
O20 Gd6 O27 N10 -67.3(13) . .
Co4 Gd6 O27 N10 -75.7(14) . .
Co2 Gd6 O27 N10 71.0(13) . .
Gd7 Gd6 O27 N10 -141.4(12) . .
O26 N10' O27' Gd3 -2(3) . .
O28' N10' O27' Gd3 172.0(17) . .
O1W Gd3 O27' N10' -17(7) . .
O9 Gd3 O27' N10' -101.9(15) . .
O15 Gd3 O27' N10' 146.5(15) . .
O10 Gd3 O27' N10' -142.7(15) . .
O18 Gd3 O27' N10' 2.1(15) . .
O16 Gd3 O27' N10' 104.9(13) . .
O17 Gd3 O27' N10' 66.3(14) . .
O11 Gd3 O27' N10' -62.4(13) . .
Co3 Gd3 O27' N10' 76.0(14) . .
Co1 Gd3 O27' N10' -72.7(15) . .
Gd1 Gd3 O27' N10' -137.7(13) . .
O17 Gd5 N11 O30 96.2(7) . .
O20 Gd5 N11 O30 -103.2(7) . .
O19 Gd5 N11 O30 -105.1(7) . .
O7 Gd5 N11 O30 30.7(7) . .
O18 Gd5 N11 O30 99.9(7) . .
O26 Gd5 N11 O30 176.5(6) . .
O8 Gd5 N11 O30 -36.8(7) . .
O29 Gd5 N11 O30 176.4(11) . .
Gd4 Gd5 N11 O30 177.8(5) . .
Gd3 Gd5 N11 O30 111.3(6) . .
O17 Gd5 N11 O31 176(7) . .
O20 Gd5 N11 O31 -24(7) . .
O19 Gd5 N11 O31 -25(7) . .
O7 Gd5 N11 O31 110(7) . .
O18 Gd5 N11 O31 180(100) . .
O26 Gd5 N11 O31 -104(7) . .
O8 Gd5 N11 O31 43(7) . .
O30 Gd5 N11 O31 80(7) . .
O29 Gd5 N11 O31 -104(7) . .
Gd4 Gd5 N11 O31 -103(7) . .
Gd3 Gd5 N11 O31 -169(7) . .
O17 Gd5 N11 O29 -80.2(6) . .
O20 Gd5 N11 O29 80.4(6) . .
O19 Gd5 N11 O29 78.5(7) . .
O7 Gd5 N11 O29 -145.7(6) . .
O18 Gd5 N11 O29 -76.5(7) . .
O26 Gd5 N11 O29 0.1(7) . .
O8 Gd5 N11 O29 146.8(6) . .
O30 Gd5 N11 O29 -176.4(11) . .
Gd4 Gd5 N11 O29 1.5(9) . .
Gd3 Gd5 N11 O29 -65.0(6) . .
O22 Gd7 N12 O32 -0.01(15) . .
O33 Gd7 N12 O32 -180.0(4) . .
O4 Gd7 N12 O32 -87.2(5) 2_656 .
O5 Gd7 N12 O32 86.0(5) 2_656 .
O21 Gd7 N12 O32 72.39(15) . .
O13 Gd7 N12 O32 -72.53(17) 2_656 .
O34 Gd7 N12 O32 158.6(2) . .
O34' Gd7 N12 O32 163.9(3) . .
O35' Gd7 N12 O32 -152.5(3) . .
O35 Gd7 N12 O32 -152.8(2) . .
O22 Gd7 N12 O33 0(5) . 2_656
O32 Gd7 N12 O33 0(5) . 2_656
O33 Gd7 N12 O33 180(100) . 2_656
O4 Gd7 N12 O33 -87(5) 2_656 2_656
O5 Gd7 N12 O33 86(5) 2_656 2_656
O21 Gd7 N12 O33 72(5) . 2_656
O13 Gd7 N12 O33 -73(5) 2_656 2_656
O34 Gd7 N12 O33 159(5) . 2_656
O34' Gd7 N12 O33 164(5) . 2_656
O35' Gd7 N12 O33 -153(5) . 2_656
O35 Gd7 N12 O33 -153(5) . 2_656
O22 Gd7 N12 O33 180.0(5) . .
O32 Gd7 N12 O33 180.0(4) . .
O4 Gd7 N12 O33 92.7(6) 2_656 .
O5 Gd7 N12 O33 -94.0(7) 2_656 .
O21 Gd7 N12 O33 -107.6(5) . .
O13 Gd7 N12 O33 107.5(5) 2_656 .
O34 Gd7 N12 O33 -21.4(5) . .
O34' Gd7 N12 O33 -16.1(5) . .
O35' Gd7 N12 O33 27.5(5) . .
O35 Gd7 N12 O33 27.2(5) . .
O22 Gd7 N12 Gd7 -0.01(15) . 2_656
O32 Gd7 N12 Gd7 0.0 . 2_656
O33 Gd7 N12 Gd7 -180.0(4) . 2_656
O4 Gd7 N12 Gd7 -87.2(5) 2_656 2_656
O5 Gd7 N12 Gd7 86.0(5) 2_656 2_656
O21 Gd7 N12 Gd7 72.39(15) . 2_656
O13 Gd7 N12 Gd7 -72.53(17) 2_656 2_656
O34 Gd7 N12 Gd7 158.6(2) . 2_656
O34' Gd7 N12 Gd7 163.9(3) . 2_656
O35' Gd7 N12 Gd7 -152.5(3) . 2_656
O35 Gd7 N12 Gd7 -152.8(2) . 2_656
O43 N16 O45 O44 178.1(12) . .
O44 N16' O45' O43 178.0(13) . .
O9 Co1 O1 C6 -175.0(9) . .
O11 Co1 O1 C6 101.1(9) . .
N2 Co1 O1 C6 -86.9(9) . .
O2 Co1 O1 C6 22.3(18) . .
N1 Co1 O1 C6 -7.4(8) . .
Gd3 Co1 O1 C6 145.4(8) . .
Gd4 Co1 O1 C6 83.0(9) . .
O9 Co1 O1 Gd1 -1.7(3) . .
O11 Co1 O1 Gd1 -85.7(3) . .
N2 Co1 O1 Gd1 86.3(4) . .
O2 Co1 O1 Gd1 -164.5(12) . .
N1 Co1 O1 Gd1 165.8(4) . .
Gd3 Co1 O1 Gd1 -41.4(3) . .
Gd4 Co1 O1 Gd1 -103.8(2) . .
O14 Gd1 O1 C6 -169.7(10) . .
O10 Gd1 O1 C6 -111.4(10) . .
O10W Gd1 O1 C6 99.9(10) 6_575 .
O10W Gd1 O1 C6 118.4(10) . .
O9 Gd1 O1 C6 173.5(11) . .
O9 Gd1 O1 C6 -51.1(11) 6_575 .
O1 Gd1 O1 C6 -26.4(11) 6_575 .
O9W Gd1 O1 C6 45.2(10) 6_575 .
O9W Gd1 O1 C6 61.6(10) . .
Gd3 Gd1 O1 C6 -149.9(10) . .
Gd3 Gd1 O1 C6 -94.8(10) 6_575 .
O14 Gd1 O1 Co1 18.4(6) . .
O10 Gd1 O1 Co1 76.7(3) . .
O10W Gd1 O1 Co1 -72.0(5) 6_575 .
O10W Gd1 O1 Co1 -53.5(4) . .
O9 Gd1 O1 Co1 1.6(3) . .
O9 Gd1 O1 Co1 137.0(3) 6_575 .
O1 Gd1 O1 Co1 161.73(16) 6_575 .
O9W Gd1 O1 Co1 -126.7(3) 6_575 .
O9W Gd1 O1 Co1 -110.3(3) . .
Gd3 Gd1 O1 Co1 38.2(3) . .
Gd3 Gd1 O1 Co1 93.3(3) 6_575 .
O9 Co1 O2 C13 95.1(7) . .
O11 Co1 O2 C13 176.5(7) . .
N2 Co1 O2 C13 9.6(7) . .
O1 Co1 O2 C13 -103.3(14) . .
N1 Co1 O2 C13 -74.7(7) . .
Gd3 Co1 O2 C13 133.5(7) . .
Gd4 Co1 O2 C13 -176.2(8) . .
O9 Co1 O2 Gd4 -88.7(3) . .
O11 Co1 O2 Gd4 -7.4(2) . .
N2 Co1 O2 Gd4 -174.3(4) . .
O1 Co1 O2 Gd4 72.8(14) . .
N1 Co1 O2 Gd4 101.5(3) . .
Gd3 Co1 O2 Gd4 -50.30(19) . .
O11 Gd4 O2 C13 -178.6(10) . .
O12 Gd4 O2 C13 40.6(11) . .
O18 Gd4 O2 C13 -103.9(10) . .
O19 Gd4 O2 C13 -41.3(10) . .
O26 Gd4 O2 C13 -125.2(10) . .
O3 Gd4 O2 C13 16.0(10) . .
O23 Gd4 O2 C13 96.9(10) . .
O24 Gd4 O2 C13 128.0(10) . .
N9 Gd4 O2 C13 111.1(10) . .
Co1 Gd4 O2 C13 174.6(11) . .
Gd5 Gd4 O2 C13 -86.2(10) . .
O11 Gd4 O2 Co1 6.8(2) . .
O12 Gd4 O2 Co1 -134.0(3) . .
O18 Gd4 O2 Co1 81.6(3) . .
O19 Gd4 O2 Co1 144.1(2) . .
O26 Gd4 O2 Co1 60.2(4) . .
O3 Gd4 O2 Co1 -158.5(3) . .
O23 Gd4 O2 Co1 -77.7(3) . .
O24 Gd4 O2 Co1 -46.6(3) . .
N9 Gd4 O2 Co1 -63.4(3) . .
Gd5 Gd4 O2 Co1 99.3(2) . .
O13 Co2 O3 C15 -98.9(8) . .
O12 Co2 O3 C15 -177.7(8) . .
O4 Co2 O3 C15 125.6(9) . .
N4 Co2 O3 C15 72.9(8) . .
N3 Co2 O3 C15 -15.9(8) . .
Gd6 Co2 O3 C15 -135.4(7) . .
O13 Co2 O3 Gd4 84.4(3) . .
O12 Co2 O3 Gd4 5.6(3) . .
O4 Co2 O3 Gd4 -51.1(8) . .
N4 Co2 O3 Gd4 -103.8(3) . .
N3 Co2 O3 Gd4 167.4(4) . .
Gd6 Co2 O3 Gd4 47.9(2) . .
O11 Gd4 O3 C15 -39.5(11) . .
O12 Gd4 O3 C15 179.1(10) . .
O18 Gd4 O3 C15 41.6(10) . .
O19 Gd4 O3 C15 105.3(10) . .
O26 Gd4 O3 C15 120.6(10) . .
O2 Gd4 O3 C15 -20.2(10) . .
O23 Gd4 O3 C15 -100.6(10) . .
O24 Gd4 O3 C15 -129.4(10) . .
N9 Gd4 O3 C15 -114.3(10) . .
Co1 Gd4 O3 C15 -32.6(10) . .
Gd5 Gd4 O3 C15 85.6(10) . .
O11 Gd4 O3 Co2 136.2(3) . .
O12 Gd4 O3 Co2 -5.3(2) . .
O18 Gd4 O3 Co2 -142.8(3) . .
O19 Gd4 O3 Co2 -79.0(3) . .
O26 Gd4 O3 Co2 -63.7(4) . .
O2 Gd4 O3 Co2 155.5(3) . .
O23 Gd4 O3 Co2 75.1(3) . .
O24 Gd4 O3 Co2 46.3(4) . .
N9 Gd4 O3 Co2 61.4(3) . .
Co1 Gd4 O3 Co2 143.1(2) . .
Gd5 Gd4 O3 Co2 -98.7(2) . .
O13 Co2 O4 C26 177.0(8) . .
O3 Co2 O4 C26 -41.9(12) . .
O12 Co2 O4 C26 -97.9(8) . .
N4 Co2 O4 C26 13.6(8) . .
N3 Co2 O4 C26 92.7(8) . .
Gd6 Co2 O4 C26 -141.7(8) . .
O13 Co2 O4 Gd7 5.0(3) . 2_656
O3 Co2 O4 Gd7 146.1(6) . 2_656
O12 Co2 O4 Gd7 90.1(3) . 2_656
N4 Co2 O4 Gd7 -158.3(4) . 2_656
N3 Co2 O4 Gd7 -79.2(4) . 2_656
Gd6 Co2 O4 Gd7 46.4(2) . 2_656
O16 Co3 O6 C39 171.4(8) . .
O7 Co3 O6 C39 -39.4(13) . .
O17 Co3 O6 C39 -103.3(8) . .
N6 Co3 O6 C39 8.3(8) . .
N7 Co3 O6 C39 87.5(8) . .
Gd3 Co3 O6 C39 -147.6(7) . .
O16 Co3 O6 Gd2 3.2(3) . .
O7 Co3 O6 Gd2 152.4(7) . .
O17 Co3 O6 Gd2 88.5(3) . .
N6 Co3 O6 Gd2 -159.9(4) . .
N7 Co3 O6 Gd2 -80.6(4) . .
Gd3 Co3 O6 Gd2 44.2(2) . .
O14 Gd2 O6 C39 172.2(9) . .
O15 Gd2 O6 C39 115.4(10) . .
O11W Gd2 O6 C39 -104.9(10) 6_575 .
O11W Gd2 O6 C39 -84.9(11) . .
O6 Gd2 O6 C39 31.5(10) 6_575 .
O16 Gd2 O6 C39 -168.3(10) . .
O16 Gd2 O6 C39 56.1(10) 6_575 .
O12W Gd2 O6 C39 -42.3(10) 6_575 .
O12W Gd2 O6 C39 -59.0(10) . .
Gd3 Gd2 O6 C39 153.9(10) . .
Gd3 Gd2 O6 C39 99.2(9) 6_575 .
O14 Gd2 O6 Co3 -22.5(5) . .
O15 Gd2 O6 Co3 -79.2(3) . .
O11W Gd2 O6 Co3 60.4(3) 6_575 .
O11W Gd2 O6 Co3 80.5(4) . .
O6 Gd2 O6 Co3 -163.16(15) 6_575 .
O16 Gd2 O6 Co3 -2.9(2) . .
O16 Gd2 O6 Co3 -138.5(3) 6_575 .
O12W Gd2 O6 Co3 123.1(3) 6_575 .
O12W Gd2 O6 Co3 106.4(3) . .
Gd3 Gd2 O6 Co3 -40.7(2) . .
Gd3 Gd2 O6 Co3 -95.5(3) 6_575 .
O16 Co3 O7 C46 -93.2(9) . .
O17 Co3 O7 C46 -174.2(9) . .
O6 Co3 O7 C46 120.5(11) . .
N6 Co3 O7 C46 74.9(9) . .
N7 Co3 O7 C46 -11.2(9) . .
Gd3 Co3 O7 C46 -131.5(9) . .
O16 Co3 O7 Gd5 87.6(4) . .
O17 Co3 O7 Gd5 6.6(3) . .
O6 Co3 O7 Gd5 -58.7(10) . .
N6 Co3 O7 Gd5 -104.3(4) . .
N7 Co3 O7 Gd5 169.6(4) . .
Gd3 Co3 O7 Gd5 49.3(3) . .
O17 Gd5 O7 C46 174.9(13) . .
O20 Gd5 O7 C46 -42.5(13) . .
O19 Gd5 O7 C46 37.2(13) . .
O18 Gd5 O7 C46 100.1(12) . .
O26 Gd5 O7 C46 117.8(12) . .
O8 Gd5 O7 C46 -24.1(12) . .
O30 Gd5 O7 C46 -102.9(12) . .
O29 Gd5 O7 C46 -132.1(12) . .
N11 Gd5 O7 C46 -115.5(12) . .
Gd4 Gd5 O7 C46 81.5(12) . .
Gd3 Gd5 O7 C46 137.2(12) . .
O17 Gd5 O7 Co3 -6.1(3) . .
O20 Gd5 O7 Co3 136.5(3) . .
O19 Gd5 O7 Co3 -143.8(3) . .
O18 Gd5 O7 Co3 -80.9(3) . .
O26 Gd5 O7 Co3 -63.2(5) . .
O8 Gd5 O7 Co3 154.9(4) . .
O30 Gd5 O7 Co3 76.0(3) . .
O29 Gd5 O7 Co3 46.9(4) . .
N11 Gd5 O7 Co3 63.4(4) . .
Gd4 Gd5 O7 Co3 -99.6(3) . .
Gd3 Gd5 O7 Co3 -43.9(3) . .
O21 Co4 O8 C48 90.9(7) . .
O20 Co4 O8 C48 171.9(7) . .
O5 Co4 O8 C48 -122.3(9) 2_656 .
N8 Co4 O8 C48 9.0(7) . .
N5 Co4 O8 C48 -81.0(7) 2_656 .
Gd6 Co4 O8 C48 129.4(7) . .
O21 Co4 O8 Gd5 -86.7(3) . .
O20 Co4 O8 Gd5 -5.6(3) . .
O5 Co4 O8 Gd5 60.1(9) 2_656 .
N8 Co4 O8 Gd5 -168.6(4) . .
N5 Co4 O8 Gd5 101.4(3) 2_656 .
Gd6 Co4 O8 Gd5 -48.2(2) . .
O17 Gd5 O8 C48 46.8(11) . .
O20 Gd5 O8 C48 -171.6(10) . .
O19 Gd5 O8 C48 -98.1(10) . .
O7 Gd5 O8 C48 22.5(9) . .
O18 Gd5 O8 C48 -35.4(10) . .
O26 Gd5 O8 C48 -117.0(9) . .
O30 Gd5 O8 C48 103.7(10) . .
O29 Gd5 O8 C48 134.3(9) . .
N11 Gd5 O8 C48 118.6(10) . .
Gd4 Gd5 O8 C48 -79.5(9) . .
Gd3 Gd5 O8 C48 -7.8(11) . .
O17 Gd5 O8 Co4 -136.5(3) . .
O20 Gd5 O8 Co4 5.2(2) . .
O19 Gd5 O8 Co4 78.7(3) . .
O7 Gd5 O8 Co4 -160.7(4) . .
O18 Gd5 O8 Co4 141.3(3) . .
O26 Gd5 O8 Co4 59.7(5) . .
O30 Gd5 O8 Co4 -79.6(3) . .
O29 Gd5 O8 Co4 -49.0(3) . .
N11 Gd5 O8 Co4 -64.6(3) . .
Gd4 Gd5 O8 Co4 97.2(3) . .
Gd3 Gd5 O8 Co4 168.89(8) . .
O11 Co1 O9 Gd3 -11.1(3) . .
N2 Co1 O9 Gd3 144.0(4) . .
O2 Co1 O9 Gd3 68.8(3) . .
O1 Co1 O9 Gd3 -107.0(3) . .
N1 Co1 O9 Gd3 -133.6(6) . .
Gd4 Co1 O9 Gd3 24.0(3) . .
O11 Co1 O9 Gd1 97.6(3) . .
N2 Co1 O9 Gd1 -107.2(4) . .
O2 Co1 O9 Gd1 177.5(3) . .
O1 Co1 O9 Gd1 1.8(3) . .
N1 Co1 O9 Gd1 -24.9(8) . .
Gd3 Co1 O9 Gd1 108.7(4) . .
Gd4 Co1 O9 Gd1 132.7(2) . .
O1W Gd3 O9 Co1 42.1(7) . .
O15 Gd3 O9 Co1 148.9(3) . .
O10 Gd3 O9 Co1 93.5(3) . .
O18 Gd3 O9 Co1 -56.3(3) . .
O16 Gd3 O9 Co1 -145.7(3) . .
O27' Gd3 O9 Co1 51.7(8) . .
O17 Gd3 O9 Co1 -109.8(3) . .
O11 Gd3 O9 Co1 9.8(2) . .
Co3 Gd3 O9 Co1 -126.3(2) . .
Gd1 Gd3 O9 Co1 111.4(4) . .
O1W Gd3 O9 Gd1 -69.4(6) . .
O15 Gd3 O9 Gd1 37.5(3) . .
O10 Gd3 O9 Gd1 -17.9(2) . .
O18 Gd3 O9 Gd1 -167.7(2) . .
O16 Gd3 O9 Gd1 102.8(3) . .
O27' Gd3 O9 Gd1 -59.8(7) . .
O17 Gd3 O9 Gd1 138.7(3) . .
O11 Gd3 O9 Gd1 -101.7(3) . .
Co3 Gd3 O9 Gd1 122.28(17) . .
Co1 Gd3 O9 Gd1 -111.4(4) . .
O14 Gd1 O9 Co1 -170.5(4) . .
O10 Gd1 O9 Co1 -90.4(4) . .
O10W Gd1 O9 Co1 145.2(3) 6_575 .
O10W Gd1 O9 Co1 137.4(3) . .
O9 Gd1 O9 Co1 -129.4(3) 6_575 .
O1 Gd1 O9 Co1 -1.6(3) . .
O1 Gd1 O9 Co1 -26.5(5) 6_575 .
O9W Gd1 O9 Co1 62.1(3) 6_575 .
O9W Gd1 O9 Co1 60.7(3) . .
Gd3 Gd1 O9 Co1 -108.8(4) . .
Gd3 Gd1 O9 Co1 -116.6(3) 6_575 .
O14 Gd1 O9 Gd3 -61.7(3) . .
O10 Gd1 O9 Gd3 18.4(3) . .
O10W Gd1 O9 Gd3 -106.0(2) 6_575 .
O10W Gd1 O9 Gd3 -113.8(2) . .
O9 Gd1 O9 Gd3 -20.6(6) 6_575 .
O1 Gd1 O9 Gd3 107.2(3) . .
O1 Gd1 O9 Gd3 82.3(4) 6_575 .
O9W Gd1 O9 Gd3 170.87(11) 6_575 .
O9W Gd1 O9 Gd3 169.48(17) . .
Gd3 Gd1 O9 Gd3 -7.7(2) 6_575 .
O14 Gd1 O10 Gd3 -58.6(2) . 6_575
O10W Gd1 O10 Gd3 -45.3(4) 6_575 6_575
O10W Gd1 O10 Gd3 -71.9(3) . 6_575
O9 Gd1 O10 Gd3 -135.7(4) . 6_575
O9 Gd1 O10 Gd3 18.4(2) 6_575 6_575
O1 Gd1 O10 Gd3 155.7(3) . 6_575
O1 Gd1 O10 Gd3 87.1(3) 6_575 6_575
O9W Gd1 O10 Gd3 100.8(5) 6_575 6_575
O9W Gd1 O10 Gd3 142.0(3) . 6_575
Gd3 Gd1 O10 Gd3 -117.2(5) . 6_575
O14 Gd1 O10 Gd3 58.6(2) . .
O10W Gd1 O10 Gd3 71.9(3) 6_575 .
O10W Gd1 O10 Gd3 45.3(4) . .
O9 Gd1 O10 Gd3 -18.4(2) . .
O9 Gd1 O10 Gd3 135.7(4) 6_575 .
O1 Gd1 O10 Gd3 -87.1(3) . .
O1 Gd1 O10 Gd3 -155.7(3) 6_575 .
O9W Gd1 O10 Gd3 -142.0(3) 6_575 .
O9W Gd1 O10 Gd3 -100.8(5) . .
Gd3 Gd1 O10 Gd3 117.2(5) 6_575 .
O1W Gd3 O10 Gd1 167.0(5) . .
O9 Gd3 O10 Gd1 18.6(3) . .
O15 Gd3 O10 Gd1 -107.8(4) . .
O18 Gd3 O10 Gd1 81.5(5) . .
O16 Gd3 O10 Gd1 -49.2(4) . .
O27' Gd3 O10 Gd1 172.2(6) . .
O17 Gd3 O10 Gd1 -137.5(3) . .
O11 Gd3 O10 Gd1 90.6(3) . .
Co3 Gd3 O10 Gd1 -77.4(4) . .
Co1 Gd3 O10 Gd1 54.3(2) . .
O1W Gd3 O10 Gd3 -79.9(5) . 6_575
O9 Gd3 O10 Gd3 131.7(4) . 6_575
O15 Gd3 O10 Gd3 5.3(3) . 6_575
O18 Gd3 O10 Gd3 -165.5(3) . 6_575
O16 Gd3 O10 Gd3 63.8(4) . 6_575
O27' Gd3 O10 Gd3 -74.7(6) . 6_575
O17 Gd3 O10 Gd3 -24.5(6) . 6_575
O11 Gd3 O10 Gd3 -156.4(4) . 6_575
Co3 Gd3 O10 Gd3 35.6(6) . 6_575
Co1 Gd3 O10 Gd3 167.4(4) . 6_575
Gd1 Gd3 O10 Gd3 113.1(4) . 6_575
O9 Co1 O11 Gd4 121.2(3) . .
N2 Co1 O11 Gd4 38.9(8) . .
O2 Co1 O11 Gd4 7.7(2) . .
O1 Co1 O11 Gd4 -159.1(3) . .
N1 Co1 O11 Gd4 -83.3(3) . .
Gd3 Co1 O11 Gd4 110.7(3) . .
O9 Co1 O11 Gd3 10.6(3) . .
N2 Co1 O11 Gd3 -71.8(8) . .
O2 Co1 O11 Gd3 -103.0(3) . .
O1 Co1 O11 Gd3 90.2(3) . .
N1 Co1 O11 Gd3 166.1(3) . .
Gd4 Co1 O11 Gd3 -110.7(3) . .
O12 Gd4 O11 Co1 125.6(3) . .
O18 Gd4 O11 Co1 -86.2(3) . .
O19 Gd4 O11 Co1 -108.6(4) . .
O26 Gd4 O11 Co1 -155.3(3) . .
O3 Gd4 O11 Co1 11.9(4) . .
O2 Gd4 O11 Co1 -7.0(2) . .
O23 Gd4 O11 Co1 71.6(3) . .
O24 Gd4 O11 Co1 123.6(3) . .
N9 Gd4 O11 Co1 96.6(4) . .
Gd5 Gd4 O11 Co1 -116.3(2) . .
O12 Gd4 O11 Gd3 -128.4(3) . .
O18 Gd4 O11 Gd3 19.8(2) . .
O19 Gd4 O11 Gd3 -2.6(5) . .
O26 Gd4 O11 Gd3 -49.3(2) . .
O3 Gd4 O11 Gd3 117.9(3) . .
O2 Gd4 O11 Gd3 99.0(3) . .
O23 Gd4 O11 Gd3 177.6(3) . .
O24 Gd4 O11 Gd3 -130.4(3) . .
N9 Gd4 O11 Gd3 -157.4(4) . .
Co1 Gd4 O11 Gd3 106.0(3) . .
Gd5 Gd4 O11 Gd3 -10.4(2) . .
O1W Gd3 O11 Co1 -168.2(5) . .
O9 Gd3 O11 Co1 -9.6(2) . .
O15 Gd3 O11 Co1 -113.6(5) . .
O10 Gd3 O11 Co1 -85.0(3) . .
O18 Gd3 O11 Co1 89.4(3) . .
O16 Gd3 O11 Co1 29.4(5) . .
O27' Gd3 O11 Co1 -163.5(6) . .
O17 Gd3 O11 Co1 128.8(3) . .
Co3 Gd3 O11 Co1 83.9(3) . .
Gd1 Gd3 O11 Co1 -47.7(2) . .
O1W Gd3 O11 Gd4 82.5(5) . .
O9 Gd3 O11 Gd4 -119.0(3) . .
O15 Gd3 O11 Gd4 137.1(4) . .
O10 Gd3 O11 Gd4 165.6(3) . .
O18 Gd3 O11 Gd4 -19.9(2) . .
O16 Gd3 O11 Gd4 -79.9(4) . .
O27' Gd3 O11 Gd4 87.2(5) . .
O17 Gd3 O11 Gd4 19.5(4) . .
Co3 Gd3 O11 Gd4 -25.5(4) . .
Co1 Gd3 O11 Gd4 -109.3(3) . .
Gd1 Gd3 O11 Gd4 -157.0(2) . .
O13 Co2 O12 Gd4 -125.7(3) . .
O3 Co2 O12 Gd4 -5.8(3) . .
O4 Co2 O12 Gd4 154.8(3) . .
N4 Co2 O12 Gd4 82.7(3) . .
N3 Co2 O12 Gd4 -43.7(7) . .
Gd6 Co2 O12 Gd4 -110.5(3) . .
O13 Co2 O12 Gd6 -15.2(2) . .
O3 Co2 O12 Gd6 104.7(3) . .
O4 Co2 O12 Gd6 -94.7(3) . .
N4 Co2 O12 Gd6 -166.9(2) . .
N3 Co2 O12 Gd6 66.7(7) . .
O11 Gd4 O12 Co2 -130.1(3) . .
O18 Gd4 O12 Co2 100.6(4) . .
O19 Gd4 O12 Co2 83.5(3) . .
O26 Gd4 O12 Co2 151.9(3) . .
O3 Gd4 O12 Co2 5.2(2) . .
O2 Gd4 O12 Co2 -18.9(4) . .
O23 Gd4 O12 Co2 -75.0(3) . .
O24 Gd4 O12 Co2 -128.2(3) . .
N9 Gd4 O12 Co2 -100.6(4) . .
Co1 Gd4 O12 Co2 -70.3(4) . .
Gd5 Gd4 O12 Co2 111.9(2) . .
O11 Gd4 O12 Gd6 124.5(3) . .
O18 Gd4 O12 Gd6 -4.8(5) . .
O19 Gd4 O12 Gd6 -21.8(2) . .
O26 Gd4 O12 Gd6 46.6(3) . .
O3 Gd4 O12 Gd6 -100.1(3) . .
O2 Gd4 O12 Gd6 -124.2(3) . .
O23 Gd4 O12 Gd6 179.6(3) . .
O24 Gd4 O12 Gd6 126.5(3) . .
N9 Gd4 O12 Gd6 154.0(4) . .
Co1 Gd4 O12 Gd6 -175.72(8) . .
Gd5 Gd4 O12 Gd6 6.5(2) . .
O19 Gd6 O12 Co2 -86.9(3) . .
O27 Gd6 O12 Co2 168.5(4) . .
O1W' Gd6 O12 Co2 173.6(4) . .
O22 Gd6 O12 Co2 116.2(3) . .
O22 Gd6 O12 Co2 90.5(2) 2_656 .
O21 Gd6 O12 Co2 -23.6(4) . .
O13 Gd6 O12 Co2 13.44(19) . .
O20 Gd6 O12 Co2 -125.2(2) . .
Co4 Gd6 O12 Co2 -79.3(3) . .
Gd7 Gd6 O12 Co2 49.2(4) . .
O19 Gd6 O12 Gd4 22.3(2) . .
O27 Gd6 O12 Gd4 -82.3(4) . .
O1W' Gd6 O12 Gd4 -77.2(4) . .
O22 Gd6 O12 Gd4 -134.6(3) . .
O22 Gd6 O12 Gd4 -160.3(3) 2_656 .
O21 Gd6 O12 Gd4 85.6(4) . .
O13 Gd6 O12 Gd4 122.7(3) . .
O20 Gd6 O12 Gd4 -16.0(4) . .
Co4 Gd6 O12 Gd4 29.9(4) . .
Co2 Gd6 O12 Gd4 109.2(3) . .
Gd7 Gd6 O12 Gd4 158.38(12) . .
O3 Co2 O13 Gd6 -61.6(3) . .
O12 Co2 O13 Gd6 15.6(2) . .
O4 Co2 O13 Gd6 102.0(3) . .
N4 Co2 O13 Gd6 134.7(5) . .
N3 Co2 O13 Gd6 -135.3(3) . .
O3 Co2 O13 Gd7 -168.5(2) . 2_656
O12 Co2 O13 Gd7 -91.3(3) . 2_656
O4 Co2 O13 Gd7 -4.9(3) . 2_656
N4 Co2 O13 Gd7 27.8(7) . 2_656
N3 Co2 O13 Gd7 117.8(3) . 2_656
Gd6 Co2 O13 Gd7 -106.9(3) . 2_656
O19 Gd6 O13 Co2 51.7(3) . .
O27 Gd6 O13 Co2 -53.9(7) . .
O1W' Gd6 O13 Co2 -44.9(7) . .
O22 Gd6 O13 Co2 -152.1(2) . .
O22 Gd6 O13 Co2 -96.1(3) 2_656 .
O21 Gd6 O13 Co2 142.7(3) . .
O12 Gd6 O13 Co2 -14.2(2) . .
O20 Gd6 O13 Co2 107.5(4) . .
Co4 Gd6 O13 Co2 122.81(18) . .
Gd7 Gd6 O13 Co2 -179.09(19) . .
O19 Gd6 O13 Gd7 163.2(2) . 2_656
O27 Gd6 O13 Gd7 57.6(7) . 2_656
O1W' Gd6 O13 Gd7 66.5(7) . 2_656
O22 Gd6 O13 Gd7 -40.7(3) . 2_656
O22 Gd6 O13 Gd7 15.3(2) 2_656 2_656
O21 Gd6 O13 Gd7 -105.9(2) . 2_656
O12 Gd6 O13 Gd7 97.2(2) . 2_656
O20 Gd6 O13 Gd7 -141.1(3) . 2_656
Co4 Gd6 O13 Gd7 -125.78(16) . 2_656
Co2 Gd6 O13 Gd7 111.4(3) . 2_656
Gd7 Gd6 O13 Gd7 -67.68(19) . 2_656
O15 Gd2 O14 Gd1 0.000(5) . .
O11W Gd2 O14 Gd1 -167.3(2) 6_575 .
O11W Gd2 O14 Gd1 167.3(2) . .
O6 Gd2 O14 Gd1 -58.4(4) . .
O6 Gd2 O14 Gd1 58.4(4) 6_575 .
O16 Gd2 O14 Gd1 -77.16(18) . .
O16 Gd2 O14 Gd1 77.16(18) 6_575 .
O12W Gd2 O14 Gd1 167.3(2) 6_575 .
O12W Gd2 O14 Gd1 -167.3(2) . .
Gd3 Gd2 O14 Gd1 -37.45(9) . .
Gd3 Gd2 O14 Gd1 37.45(9) 6_575 .
O10 Gd1 O14 Gd2 0.000(7) . .
O10W Gd1 O14 Gd2 -166.1(2) 6_575 .
O10W Gd1 O14 Gd2 166.1(2) . .
O9 Gd1 O14 Gd2 76.5(2) . .
O9 Gd1 O14 Gd2 -76.5(2) 6_575 .
O1 Gd1 O14 Gd2 60.3(4) . .
O1 Gd1 O14 Gd2 -60.3(4) 6_575 .
O9W Gd1 O14 Gd2 -167.3(2) 6_575 .
O9W Gd1 O14 Gd2 167.3(2) . .
Gd3 Gd1 O14 Gd2 37.50(10) . .
Gd3 Gd1 O14 Gd2 -37.50(10) 6_575 .
O14 Gd2 O15 Gd3 -58.8(3) . .
O11W Gd2 O15 Gd3 -42.8(5) 6_575 .
O11W Gd2 O15 Gd3 -74.9(3) . .
O6 Gd2 O15 Gd3 86.5(3) . .
O6 Gd2 O15 Gd3 155.8(4) 6_575 .
O16 Gd2 O15 Gd3 17.8(3) . .
O16 Gd2 O15 Gd3 -135.5(4) 6_575 .
O12W Gd2 O15 Gd3 143.9(4) 6_575 .
O12W Gd2 O15 Gd3 98.4(6) . .
Gd3 Gd2 O15 Gd3 -117.7(6) 6_575 .
O14 Gd2 O15 Gd3 58.8(3) . 6_575
O11W Gd2 O15 Gd3 74.9(3) 6_575 6_575
O11W Gd2 O15 Gd3 42.8(5) . 6_575
O6 Gd2 O15 Gd3 -155.8(4) . 6_575
O6 Gd2 O15 Gd3 -86.5(3) 6_575 6_575
O16 Gd2 O15 Gd3 135.5(4) . 6_575
O16 Gd2 O15 Gd3 -17.8(3) 6_575 6_575
O12W Gd2 O15 Gd3 -98.4(6) 6_575 6_575
O12W Gd2 O15 Gd3 -143.9(4) . 6_575
Gd3 Gd2 O15 Gd3 117.7(6) . 6_575
O1W Gd3 O15 Gd2 -169.2(6) . .
O9 Gd3 O15 Gd2 50.5(4) . .
O10 Gd3 O15 Gd2 107.9(4) . .
O18 Gd3 O15 Gd2 -81.2(6) . .
O16 Gd3 O15 Gd2 -17.9(3) . .
O27' Gd3 O15 Gd2 -171.1(7) . .
O17 Gd3 O15 Gd2 -90.3(3) . .
O11 Gd3 O15 Gd2 138.1(3) . .
Co3 Gd3 O15 Gd2 -53.6(3) . .
Co1 Gd3 O15 Gd2 78.9(4) . .
Gd1 Gd3 O15 Gd2 72.9(3) . .
O1W Gd3 O15 Gd3 77.5(5) . 6_575
O9 Gd3 O15 Gd3 -62.8(4) . 6_575
O10 Gd3 O15 Gd3 -5.3(3) . 6_575
O18 Gd3 O15 Gd3 165.5(3) . 6_575
O16 Gd3 O15 Gd3 -131.2(5) . 6_575
O27' Gd3 O15 Gd3 75.7(6) . 6_575
O17 Gd3 O15 Gd3 156.4(4) . 6_575
O11 Gd3 O15 Gd3 24.9(7) . 6_575
Co3 Gd3 O15 Gd3 -166.8(4) . 6_575
Co1 Gd3 O15 Gd3 -34.3(6) . 6_575
Gd1 Gd3 O15 Gd3 -40.4(3) . 6_575
O7 Co3 O16 Gd3 -66.2(3) . .
O17 Co3 O16 Gd3 11.9(3) . .
O6 Co3 O16 Gd3 104.1(3) . .
N6 Co3 O16 Gd3 137.7(6) . .
N7 Co3 O16 Gd3 -140.7(3) . .
O7 Co3 O16 Gd2 -173.5(2) . .
O17 Co3 O16 Gd2 -95.4(3) . .
O6 Co3 O16 Gd2 -3.2(3) . .
N6 Co3 O16 Gd2 30.4(7) . .
N7 Co3 O16 Gd2 112.0(3) . .
Gd3 Co3 O16 Gd2 -107.3(4) . .
O1W Gd3 O16 Co3 -42.3(7) . .
O9 Gd3 O16 Co3 146.2(3) . .
O15 Gd3 O16 Co3 -93.5(4) . .
O10 Gd3 O16 Co3 -149.5(3) . .
O18 Gd3 O16 Co3 55.9(3) . .
O27' Gd3 O16 Co3 -51.2(8) . .
O17 Gd3 O16 Co3 -10.6(3) . .
O11 Gd3 O16 Co3 109.2(4) . .
Co1 Gd3 O16 Co3 126.5(2) . .
Gd1 Gd3 O16 Co3 -176.5(3) . .
O1W Gd3 O16 Gd2 68.4(7) . .
O9 Gd3 O16 Gd2 -103.2(3) . .
O15 Gd3 O16 Gd2 17.1(3) . .
O10 Gd3 O16 Gd2 -38.9(4) . .
O18 Gd3 O16 Gd2 166.5(3) . .
O27' Gd3 O16 Gd2 59.5(8) . .
O17 Gd3 O16 Gd2 100.0(3) . .
O11 Gd3 O16 Gd2 -140.2(3) . .
Co3 Gd3 O16 Gd2 110.6(4) . .
Co1 Gd3 O16 Gd2 -122.8(2) . .
Gd1 Gd3 O16 Gd2 -65.8(2) . .
O14 Gd2 O16 Co3 169.7(4) . .
O15 Gd2 O16 Co3 90.0(4) . .
O11W Gd2 O16 Co3 -128.0(2) 6_575 .
O11W Gd2 O16 Co3 -135.9(2) . .
O6 Gd2 O16 Co3 3.0(2) . .
O6 Gd2 O16 Co3 27.9(4) 6_575 .
O16 Gd2 O16 Co3 130.8(4) 6_575 .
O12W Gd2 O16 Co3 -65.3(3) 6_575 .
O12W Gd2 O16 Co3 -63.3(3) . .
Gd3 Gd2 O16 Co3 107.5(4) . .
Gd3 Gd2 O16 Co3 116.2(2) 6_575 .
O14 Gd2 O16 Gd3 62.2(3) . .
O15 Gd2 O16 Gd3 -17.5(3) . .
O11W Gd2 O16 Gd3 124.5(3) 6_575 .
O11W Gd2 O16 Gd3 116.6(2) . .
O6 Gd2 O16 Gd3 -104.5(3) . .
O6 Gd2 O16 Gd3 -79.6(4) 6_575 .
O16 Gd2 O16 Gd3 23.3(7) 6_575 .
O12W Gd2 O16 Gd3 -172.77(14) 6_575 .
O12W Gd2 O16 Gd3 -170.8(2) . .
Gd3 Gd2 O16 Gd3 8.7(3) 6_575 .
O16 Co3 O17 Gd5 -122.4(3) . .
O7 Co3 O17 Gd5 -6.8(3) . .
O6 Co3 O17 Gd5 157.5(4) . .
N6 Co3 O17 Gd5 83.6(4) . .
N7 Co3 O17 Gd5 -43.9(9) . .
Gd3 Co3 O17 Gd5 -110.9(4) . .
O16 Co3 O17 Gd3 -11.5(3) . .
O7 Co3 O17 Gd3 104.1(3) . .
O6 Co3 O17 Gd3 -91.6(3) . .
N6 Co3 O17 Gd3 -165.4(3) . .
N7 Co3 O17 Gd3 67.0(8) . .
O20 Gd5 O17 Co3 -129.1(3) . .
O19 Gd5 O17 Co3 102.1(4) . .
O7 Gd5 O17 Co3 6.2(3) . .
O18 Gd5 O17 Co3 84.0(3) . .
O26 Gd5 O17 Co3 152.0(4) . .
O8 Gd5 O17 Co3 -17.8(5) . .
O30 Gd5 O17 Co3 -73.4(3) . .
O29 Gd5 O17 Co3 -126.0(4) . .
N11 Gd5 O17 Co3 -98.4(4) . .
Gd4 Gd5 O17 Co3 112.5(3) . .
Gd3 Gd5 O17 Co3 105.6(4) . .
O20 Gd5 O17 Gd3 125.2(3) . .
O19 Gd5 O17 Gd3 -3.5(5) . .
O7 Gd5 O17 Gd3 -99.5(3) . .
O18 Gd5 O17 Gd3 -21.7(2) . .
O26 Gd5 O17 Gd3 46.4(3) . .
O8 Gd5 O17 Gd3 -123.4(3) . .
O30 Gd5 O17 Gd3 -179.1(3) . .
O29 Gd5 O17 Gd3 128.4(3) . .
N11 Gd5 O17 Gd3 156.0(3) . .
Gd4 Gd5 O17 Gd3 6.8(2) . .
O1W Gd3 O17 Co3 171.2(4) . .
O9 Gd3 O17 Co3 -27.4(5) . .
O15 Gd3 O17 Co3 86.7(3) . .
O10 Gd3 O17 Co3 114.9(4) . .
O18 Gd3 O17 Co3 -87.7(3) . .
O16 Gd3 O17 Co3 10.3(2) . .
O27' Gd3 O17 Co3 164.7(5) . .
O11 Gd3 O17 Co3 -127.1(2) . .
Co1 Gd3 O17 Co3 -83.1(3) . .
Gd1 Gd3 O17 Co3 44.8(5) . .
O1W Gd3 O17 Gd5 -79.2(4) . .
O9 Gd3 O17 Gd5 82.2(4) . .
O15 Gd3 O17 Gd5 -163.6(3) . .
O10 Gd3 O17 Gd5 -135.5(4) . .
O18 Gd3 O17 Gd5 21.9(2) . .
O16 Gd3 O17 Gd5 120.0(3) . .
O27' Gd3 O17 Gd5 -85.7(5) . .
O11 Gd3 O17 Gd5 -17.4(4) . .
Co3 Gd3 O17 Gd5 109.7(4) . .
Co1 Gd3 O17 Gd5 26.6(4) . .
Gd1 Gd3 O17 Gd5 154.50(17) . .
O11 Gd4 O18 Gd5 -131.5(3) . .
O12 Gd4 O18 Gd5 17.0(5) . .
O19 Gd4 O18 Gd5 33.7(2) . .
O26 Gd4 O18 Gd5 -40.0(2) . .
O3 Gd4 O18 Gd5 97.2(3) . .
O2 Gd4 O18 Gd5 154.7(3) . .
O23 Gd4 O18 Gd5 -170.2(3) . .
O24 Gd4 O18 Gd5 -93.3(3) . .
N9 Gd4 O18 Gd5 -127.0(5) . .
Co1 Gd4 O18 Gd5 -168.1(2) . .
O11 Gd4 O18 Gd3 -20.6(3) . .
O12 Gd4 O18 Gd3 127.9(3) . .
O19 Gd4 O18 Gd3 144.6(4) . .
O26 Gd4 O18 Gd3 70.9(3) . .
O3 Gd4 O18 Gd3 -151.9(3) . .
O2 Gd4 O18 Gd3 -94.4(3) . .
O23 Gd4 O18 Gd3 -59.2(5) . .
O24 Gd4 O18 Gd3 17.7(5) . .
N9 Gd4 O18 Gd3 -16.0(7) . .
Co1 Gd4 O18 Gd3 -57.1(2) . .
Gd5 Gd4 O18 Gd3 110.9(4) . .
O17 Gd5 O18 Gd4 134.0(3) . .
O20 Gd5 O18 Gd4 -14.6(4) . .
O19 Gd5 O18 Gd4 -33.9(2) . .
O7 Gd5 O18 Gd4 -152.5(3) . .
O26 Gd5 O18 Gd4 40.2(2) . .
O8 Gd5 O18 Gd4 -97.3(2) . .
O30 Gd5 O18 Gd4 170.5(3) . .
O29 Gd5 O18 Gd4 95.1(3) . .
N11 Gd5 O18 Gd4 130.2(4) . .
Gd3 Gd5 O18 Gd4 111.8(3) . .
O17 Gd5 O18 Gd3 22.2(2) . .
O20 Gd5 O18 Gd3 -126.4(3) . .
O19 Gd5 O18 Gd3 -145.7(3) . .
O7 Gd5 O18 Gd3 95.8(3) . .
O26 Gd5 O18 Gd3 -71.6(3) . .
O8 Gd5 O18 Gd3 151.0(2) . .
O30 Gd5 O18 Gd3 58.7(4) . .
O29 Gd5 O18 Gd3 -16.7(4) . .
N11 Gd5 O18 Gd3 18.4(5) . .
Gd4 Gd5 O18 Gd3 -111.8(3) . .
O1W Gd3 O18 Gd4 -51.5(5) . .
O9 Gd3 O18 Gd4 87.5(3) . .
O15 Gd3 O18 Gd4 -135.3(4) . .
O10 Gd3 O18 Gd4 29.5(6) . .
O16 Gd3 O18 Gd4 165.9(3) . .
O27' Gd3 O18 Gd4 -53.5(6) . .
O17 Gd3 O18 Gd4 -125.7(3) . .
O11 Gd3 O18 Gd4 19.8(3) . .
Co3 Gd3 O18 Gd4 -164.1(3) . .
Co1 Gd3 O18 Gd4 57.4(2) . .
Gd1 Gd3 O18 Gd4 77.9(3) . .
O1W Gd3 O18 Gd5 52.8(5) . .
O9 Gd3 O18 Gd5 -168.2(2) . .
O15 Gd3 O18 Gd5 -31.0(5) . .
O10 Gd3 O18 Gd5 133.8(5) . .
O16 Gd3 O18 Gd5 -89.8(3) . .
O27' Gd3 O18 Gd5 50.8(6) . .
O17 Gd3 O18 Gd5 -21.4(2) . .
O11 Gd3 O18 Gd5 124.1(3) . .
Co3 Gd3 O18 Gd5 -59.76(18) . .
Co1 Gd3 O18 Gd5 161.7(2) . .
Gd1 Gd3 O18 Gd5 -177.83(8) . .
O27 Gd6 O19 Gd5 -51.9(5) . .
O1W' Gd6 O19 Gd5 -52.5(5) . .
O22 Gd6 O19 Gd5 28.3(5) . .
O22 Gd6 O19 Gd5 -130.4(3) 2_656 .
O21 Gd6 O19 Gd5 88.9(3) . .
O13 Gd6 O19 Gd5 167.4(3) . .
O12 Gd6 O19 Gd5 -125.9(3) . .
O20 Gd6 O19 Gd5 21.4(2) . .
Co4 Gd6 O19 Gd5 59.2(2) . .
Co2 Gd6 O19 Gd5 -164.7(3) . .
Gd7 Gd6 O19 Gd5 77.6(3) . .
O27 Gd6 O19 Gd4 52.1(5) . .
O1W' Gd6 O19 Gd4 51.5(5) . .
O22 Gd6 O19 Gd4 132.3(3) . .
O22 Gd6 O19 Gd4 -26.4(5) 2_656 .
O21 Gd6 O19 Gd4 -167.1(3) . .
O13 Gd6 O19 Gd4 -88.6(3) . .
O12 Gd6 O19 Gd4 -22.0(2) . .
O20 Gd6 O19 Gd4 125.3(3) . .
Co4 Gd6 O19 Gd4 163.2(3) . .
Co2 Gd6 O19 Gd4 -60.7(2) . .
Gd7 Gd6 O19 Gd4 -178.46(9) . .
O17 Gd5 O19 Gd6 126.8(3) . .
O20 Gd5 O19 Gd6 -21.9(2) . .
O7 Gd5 O19 Gd6 -152.6(3) . .
O18 Gd5 O19 Gd6 144.7(3) . .
O26 Gd5 O19 Gd6 72.1(3) . .
O8 Gd5 O19 Gd6 -95.1(3) . .
O30 Gd5 O19 Gd6 -60.1(4) . .
O29 Gd5 O19 Gd6 15.0(4) . .
N11 Gd5 O19 Gd6 -20.0(5) . .
Gd4 Gd5 O19 Gd6 111.4(3) . .
Gd3 Gd5 O19 Gd6 124.6(2) . .
O17 Gd5 O19 Gd4 15.4(4) . .
O20 Gd5 O19 Gd4 -133.3(3) . .
O7 Gd5 O19 Gd4 96.0(3) . .
O18 Gd5 O19 Gd4 33.4(2) . .
O26 Gd5 O19 Gd4 -39.3(2) . .
O8 Gd5 O19 Gd4 153.5(3) . .
O30 Gd5 O19 Gd4 -171.5(3) . .
O29 Gd5 O19 Gd4 -96.4(3) . .
N11 Gd5 O19 Gd4 -131.4(4) . .
Gd3 Gd5 O19 Gd4 13.3(2) . .
O11 Gd4 O19 Gd6 -123.8(3) . .
O12 Gd4 O19 Gd6 22.7(2) . .
O18 Gd4 O19 Gd6 -145.9(3) . .
O26 Gd4 O19 Gd6 -72.9(3) . .
O3 Gd4 O19 Gd6 96.7(3) . .
O2 Gd4 O19 Gd6 151.0(2) . .
O23 Gd4 O19 Gd6 55.9(5) . .
O24 Gd4 O19 Gd6 -16.8(4) . .
N9 Gd4 O19 Gd6 16.6(6) . .
Co1 Gd4 O19 Gd6 -178.07(7) . .
Gd5 Gd4 O19 Gd6 -112.2(4) . .
O11 Gd4 O19 Gd5 -11.6(4) . .
O12 Gd4 O19 Gd5 134.9(3) . .
O18 Gd4 O19 Gd5 -33.7(2) . .
O26 Gd4 O19 Gd5 39.3(2) . .
O3 Gd4 O19 Gd5 -151.2(3) . .
O2 Gd4 O19 Gd5 -96.9(3) . .
O23 Gd4 O19 Gd5 168.0(3) . .
O24 Gd4 O19 Gd5 95.4(3) . .
N9 Gd4 O19 Gd5 128.8(4) . .
Co1 Gd4 O19 Gd5 -65.9(3) . .
O21 Co4 O20 Gd5 122.8(3) . .
O8 Co4 O20 Gd5 5.9(3) . .
O5 Co4 O20 Gd5 -157.9(3) 2_656 .
N8 Co4 O20 Gd5 42.7(7) . .
N5 Co4 O20 Gd5 -84.9(3) 2_656 .
Gd6 Co4 O20 Gd5 110.1(4) . .
O21 Co4 O20 Gd6 12.6(3) . .
O8 Co4 O20 Gd6 -104.3(3) . .
O5 Co4 O20 Gd6 91.9(3) 2_656 .
N8 Co4 O20 Gd6 -67.5(6) . .
N5 Co4 O20 Gd6 165.0(3) 2_656 .
O17 Gd5 O20 Co4 127.1(3) . .
O19 Gd5 O20 Co4 -85.0(3) . .
O7 Gd5 O20 Co4 12.8(5) . .
O18 Gd5 O20 Co4 -104.8(3) . .
O26 Gd5 O20 Co4 -154.2(3) . .
O8 Gd5 O20 Co4 -5.3(3) . .
O30 Gd5 O20 Co4 72.0(3) . .
O29 Gd5 O20 Co4 123.9(3) . .
N11 Gd5 O20 Co4 96.2(3) . .
Gd4 Gd5 O20 Co4 -114.4(2) . .
Gd3 Gd5 O20 Co4 -166.55(8) . .
O17 Gd5 O20 Gd6 -127.0(3) . .
O19 Gd5 O20 Gd6 20.8(2) . .
O7 Gd5 O20 Gd6 118.7(3) . .
O18 Gd5 O20 Gd6 1.1(4) . .
O26 Gd5 O20 Gd6 -48.3(3) . .
O8 Gd5 O20 Gd6 100.5(3) . .
O30 Gd5 O20 Gd6 177.8(3) . .
O29 Gd5 O20 Gd6 -130.2(3) . .
N11 Gd5 O20 Gd6 -158.0(3) . .
Gd4 Gd5 O20 Gd6 -8.5(2) . .
Gd3 Gd5 O20 Gd6 -60.7(4) . .
O19 Gd6 O20 Co4 88.4(3) . .
O27 Gd6 O20 Co4 -166.6(5) . .
O1W' Gd6 O20 Co4 -172.3(5) . .
O22 Gd6 O20 Co4 -87.6(3) . .
O22 Gd6 O20 Co4 -117.1(3) 2_656 .
O21 Gd6 O20 Co4 -11.4(2) . .
O13 Gd6 O20 Co4 25.6(5) . .
O12 Gd6 O20 Co4 126.7(3) . .
Co2 Gd6 O20 Co4 79.7(3) . .
Gd7 Gd6 O20 Co4 -50.8(2) . .
O19 Gd6 O20 Gd5 -21.1(2) . .
O27 Gd6 O20 Gd5 83.8(5) . .
O1W' Gd6 O20 Gd5 78.1(5) . .
O22 Gd6 O20 Gd5 162.8(3) . .
O22 Gd6 O20 Gd5 133.3(3) 2_656 .
O21 Gd6 O20 Gd5 -120.9(3) . .
O13 Gd6 O20 Gd5 -83.9(4) . .
O12 Gd6 O20 Gd5 17.1(4) . .
Co4 Gd6 O20 Gd5 -109.6(3) . .
Co2 Gd6 O20 Gd5 -29.8(4) . .
Gd7 Gd6 O20 Gd5 -160.3(2) . .
O20 Co4 O21 Gd6 -13.0(3) . .
O8 Co4 O21 Gd6 66.4(3) . .
O5 Co4 O21 Gd6 -103.8(3) 2_656 .
N8 Co4 O21 Gd6 139.2(3) . .
N5 Co4 O21 Gd6 -130.1(5) 2_656 .
O20 Co4 O21 Gd7 93.6(3) . .
O8 Co4 O21 Gd7 172.9(2) . .
O5 Co4 O21 Gd7 2.7(3) 2_656 .
N8 Co4 O21 Gd7 -114.2(3) . .
N5 Co4 O21 Gd7 -23.6(7) 2_656 .
Gd6 Co4 O21 Gd7 106.6(3) . .
O19 Gd6 O21 Co4 -54.8(3) . .
O27 Gd6 O21 Co4 50.8(6) . .
O1W' Gd6 O21 Co4 41.9(7) . .
O22 Gd6 O21 Co4 94.2(3) . .
O22 Gd6 O21 Co4 149.1(2) 2_656 .
O13 Gd6 O21 Co4 -145.8(3) . .
O12 Gd6 O21 Co4 -110.7(3) . .
O20 Gd6 O21 Co4 11.5(2) . .
Co2 Gd6 O21 Co4 -125.0(2) . .
Gd7 Gd6 O21 Co4 111.3(4) . .
O19 Gd6 O21 Gd7 -166.1(2) . .
O27 Gd6 O21 Gd7 -60.6(6) . .
O1W' Gd6 O21 Gd7 -69.4(6) . .
O22 Gd6 O21 Gd7 -17.1(2) . .
O22 Gd6 O21 Gd7 37.8(3) 2_656 .
O13 Gd6 O21 Gd7 102.9(2) . .
O12 Gd6 O21 Gd7 137.9(3) . .
O20 Gd6 O21 Gd7 -99.8(3) . .
Co4 Gd6 O21 Gd7 -111.3(4) . .
Co2 Gd6 O21 Gd7 123.66(17) . .
O22 Gd7 O21 Co4 -89.3(3) . .
O32 Gd7 O21 Co4 -166.2(4) . .
O33 Gd7 O21 Co4 142.0(3) . .
O4 Gd7 O21 Co4 -27.1(4) 2_656 .
O5 Gd7 O21 Co4 -2.6(2) 2_656 .
O13 Gd7 O21 Co4 -131.6(3) 2_656 .
O34 Gd7 O21 Co4 73.1(4) . .
O34' Gd7 O21 Co4 59.9(4) . .
O35' Gd7 O21 Co4 92.8(5) . .
O35 Gd7 O21 Co4 71.1(6) . .
N12 Gd7 O21 Co4 169.3(4) . .
O22 Gd7 O21 Gd6 17.7(2) . .
O32 Gd7 O21 Gd6 -59.2(3) . .
O33 Gd7 O21 Gd6 -111.0(3) . .
O4 Gd7 O21 Gd6 79.9(3) 2_656 .
O5 Gd7 O21 Gd6 104.4(3) 2_656 .
O13 Gd7 O21 Gd6 -24.5(4) 2_656 .
O34 Gd7 O21 Gd6 -179.9(4) . .
O34' Gd7 O21 Gd6 166.9(4) . .
O35' Gd7 O21 Gd6 -160.2(4) . .
O35 Gd7 O21 Gd6 178.1(5) . .
N12 Gd7 O21 Gd6 -83.7(3) . .
O32 Gd7 O22 Gd6 59.36(17) . .
O33 Gd7 O22 Gd6 59.4(4) . .
O4 Gd7 O22 Gd6 -157.4(2) 2_656 .
O5 Gd7 O22 Gd6 -86.5(2) 2_656 .
O21 Gd7 O22 Gd6 -18.1(2) . .
O13 Gd7 O22 Gd6 134.7(3) 2_656 .
O34 Gd7 O22 Gd6 -63.0(9) . .
O34' Gd7 O22 Gd6 -91.4(7) . .
O35' Gd7 O22 Gd6 158.6(7) . .
O35 Gd7 O22 Gd6 -173.4(5) . .
N12 Gd7 O22 Gd6 59.37(19) . .
O32 Gd7 O22 Gd6 -59.1(2) . 2_656
O33 Gd7 O22 Gd6 -59.0(4) . 2_656
O4 Gd7 O22 Gd6 84.2(3) 2_656 2_656
O5 Gd7 O22 Gd6 155.0(3) 2_656 2_656
O21 Gd7 O22 Gd6 -136.5(3) . 2_656
O13 Gd7 O22 Gd6 16.3(2) 2_656 2_656
O34 Gd7 O22 Gd6 178.6(8) . 2_656
O34' Gd7 O22 Gd6 150.2(7) . 2_656
O35' Gd7 O22 Gd6 40.2(8) . 2_656
O35 Gd7 O22 Gd6 68.2(6) . 2_656
N12 Gd7 O22 Gd6 -59.0(2) . 2_656
O19 Gd6 O22 Gd7 84.1(4) . .
O27 Gd6 O22 Gd7 171.2(4) . .
O1W' Gd6 O22 Gd7 168.3(4) . .
O22 Gd6 O22 Gd7 -108.95(16) 2_656 .
O21 Gd6 O22 Gd7 18.4(2) . .
O13 Gd6 O22 Gd7 -50.1(3) . .
O12 Gd6 O22 Gd7 -136.0(3) . .
O20 Gd6 O22 Gd7 90.7(2) . .
Co4 Gd6 O22 Gd7 54.23(17) . .
Co2 Gd6 O22 Gd7 -75.6(3) . .
O19 Gd6 O22 Gd6 -161.3(3) . 2_656
O27 Gd6 O22 Gd6 -74.2(4) . 2_656
O1W' Gd6 O22 Gd6 -77.0(4) . 2_656
O22 Gd6 O22 Gd6 5.7(3) 2_656 2_656
O21 Gd6 O22 Gd6 133.1(3) . 2_656
O13 Gd6 O22 Gd6 64.5(3) . 2_656
O12 Gd6 O22 Gd6 -21.4(5) . 2_656
O20 Gd6 O22 Gd6 -154.7(3) . 2_656
Co4 Gd6 O22 Gd6 168.9(3) . 2_656
Co2 Gd6 O22 Gd6 39.0(4) . 2_656
Gd7 Gd6 O22 Gd6 114.6(4) . 2_656
O25 N9 O23 Gd4 179.2(11) . .
O24 N9 O23 Gd4 -1.7(11) . .
O11 Gd4 O23 N9 73.4(7) . .
O12 Gd4 O23 N9 -74.7(7) . .
O18 Gd4 O23 N9 110.0(7) . .
O19 Gd4 O23 N9 -106.4(7) . .
O26 Gd4 O23 N9 -0.2(8) . .
O3 Gd4 O23 N9 -146.2(7) . .
O2 Gd4 O23 N9 144.7(7) . .
O24 Gd4 O23 N9 1.0(6) . .
Co1 Gd4 O23 N9 107.9(7) . .
Gd5 Gd4 O23 N9 -14.3(17) . .
O23 N9 O24 Gd4 1.6(11) . .
O25 N9 O24 Gd4 -179.2(11) . .
O11 Gd4 O24 N9 -94.2(7) . .
O12 Gd4 O24 N9 87.1(6) . .
O18 Gd4 O24 N9 -132.6(6) . .
O19 Gd4 O24 N9 126.2(6) . .
O26 Gd4 O24 N9 178.2(7) . .
O3 Gd4 O24 N9 36.1(7) . .
O2 Gd4 O24 N9 -41.1(7) . .
O23 Gd4 O24 N9 -0.9(6) . .
Co1 Gd4 O24 N9 -66.0(6) . .
Gd5 Gd4 O24 N9 176.7(6) . .
O27' N10' O26 N10 178(3) . .
O28' N10' O26 N10 3.0(13) . .
O27' N10' O26 Gd5 -61(3) . .
O28' N10' O26 Gd5 123.7(10) . .
O27' N10' O26 Gd4 62(3) . .
O28' N10' O26 Gd4 -113.1(12) . .
O27 N10 O26 N10' 174(2) . .
O28 N10 O26 N10' 4.2(13) . .
O27 N10 O26 Gd5 55(2) . .
O28 N10 O26 Gd5 -114.4(10) . .
O27 N10 O26 Gd4 -65(2) . .
O28 N10 O26 Gd4 125.6(10) . .
O17 Gd5 O26 N10' 25.8(12) . .
O20 Gd5 O26 N10' -116.5(12) . .
O19 Gd5 O26 N10' 174.4(12) . .
O7 Gd5 O26 N10' 77.5(12) . .
O18 Gd5 O26 N10' 95.7(12) . .
O8 Gd5 O26 N10' -166.1(11) . .
O30 Gd5 O26 N10' -43.9(12) . .
O29 Gd5 O26 N10' -45.8(12) . .
N11 Gd5 O26 N10' -45.8(12) . .
Gd4 Gd5 O26 N10' 135.2(12) . .
Gd3 Gd5 O26 N10' 55.9(11) . .
O17 Gd5 O26 N10 120.6(10) . .
O20 Gd5 O26 N10 -21.7(10) . .
O19 Gd5 O26 N10 -90.8(10) . .
O7 Gd5 O26 N10 172.4(9) . .
O18 Gd5 O26 N10 -169.5(10) . .
O8 Gd5 O26 N10 -71.3(10) . .
O30 Gd5 O26 N10 50.9(10) . .
O29 Gd5 O26 N10 49.0(10) . .
N11 Gd5 O26 N10 49.0(10) . .
Gd4 Gd5 O26 N10 -130.0(10) . .
Gd3 Gd5 O26 N10 150.7(10) . .
O17 Gd5 O26 Gd4 -109.4(3) . .
O20 Gd5 O26 Gd4 108.3(2) . .
O19 Gd5 O26 Gd4 39.2(2) . .
O7 Gd5 O26 Gd4 -57.6(4) . .
O18 Gd5 O26 Gd4 -39.4(2) . .
O8 Gd5 O26 Gd4 58.7(5) . .
O30 Gd5 O26 Gd4 -179.1(2) . .
O29 Gd5 O26 Gd4 179.0(3) . .
N11 Gd5 O26 Gd4 179.0(3) . .
Gd3 Gd5 O26 Gd4 -79.3(2) . .
O11 Gd4 O26 N10' -22.4(9) . .
O12 Gd4 O26 N10' 119.0(9) . .
O18 Gd4 O26 N10' -93.6(9) . .
O19 Gd4 O26 N10' -172.5(9) . .
O3 Gd4 O26 N10' 171.9(9) . .
O2 Gd4 O26 N10' -71.5(10) . .
O23 Gd4 O26 N10' 49.4(10) . .
O24 Gd4 O26 N10' 48.5(9) . .
N9 Gd4 O26 N10' 49.3(10) . .
Co1 Gd4 O26 N10' -37.6(9) . .
Gd5 Gd4 O26 N10' -133.4(10) . .
O11 Gd4 O26 N10 -116.2(10) . .
O12 Gd4 O26 N10 25.1(10) . .
O18 Gd4 O26 N10 172.6(10) . .
O19 Gd4 O26 N10 93.6(10) . .
O3 Gd4 O26 N10 78.0(10) . .
O2 Gd4 O26 N10 -165.4(9) . .
O23 Gd4 O26 N10 -44.4(10) . .
O24 Gd4 O26 N10 -45.4(9) . .
N9 Gd4 O26 N10 -44.5(10) . .
Co1 Gd4 O26 N10 -131.4(9) . .
Gd5 Gd4 O26 N10 132.7(10) . .
O11 Gd4 O26 Gd5 111.1(2) . .
O12 Gd4 O26 Gd5 -107.6(2) . .
O18 Gd4 O26 Gd5 39.9(2) . .
O19 Gd4 O26 Gd5 -39.1(2) . .
O3 Gd4 O26 Gd5 -54.7(4) . .
O2 Gd4 O26 Gd5 61.9(4) . .
O23 Gd4 O26 Gd5 -177.1(2) . .
O24 Gd4 O26 Gd5 -178.1(3) . .
N9 Gd4 O26 Gd5 -177.2(3) . .
Co1 Gd4 O26 Gd5 95.9(2) . .
O30 N11 O29 Gd5 -3.5(10) . .
O31 N11 O29 Gd5 172.1(10) . .
O17 Gd5 O29 N11 91.4(6) . .
O20 Gd5 O29 N11 -90.7(6) . .
O19 Gd5 O29 N11 -127.3(6) . .
O7 Gd5 O29 N11 39.5(7) . .
O18 Gd5 O29 N11 129.9(6) . .
O26 Gd5 O29 N11 -179.9(6) . .
O8 Gd5 O29 N11 -37.3(7) . .
O30 Gd5 O29 N11 1.9(6) . .
Gd4 Gd5 O29 N11 -179.1(5) . .
Gd3 Gd5 O29 N11 120.1(6) . .
O31 N11 O30 Gd5 -171.9(10) . .
O29 N11 O30 Gd5 3.7(11) . .
O17 Gd5 O30 N11 -77.6(7) . .
O20 Gd5 O30 N11 70.9(7) . .
O19 Gd5 O30 N11 106.9(7) . .
O7 Gd5 O30 N11 -148.6(7) . .
O18 Gd5 O30 N11 -112.4(7) . .
O26 Gd5 O30 N11 -4.5(8) . .
O8 Gd5 O30 N11 141.7(7) . .
O29 Gd5 O30 N11 -2.1(6) . .
Gd4 Gd5 O30 N11 -10(2) . .
Gd3 Gd5 O30 N11 -78.2(7) . .
O33 N12 O32 Gd7 0.0(4) 2_656 2_656
O33 N12 O32 Gd7 180.0(4) . 2_656
Gd7 N12 O32 Gd7 180.0 . 2_656
O33 N12 O32 Gd7 180.0(4) 2_656 .
O33 N12 O32 Gd7 0.0(4) . .
Gd7 N12 O32 Gd7 180.0 2_656 .
O22 Gd7 O32 N12 179.99(15) . .
O33 Gd7 O32 N12 0.0(3) . .
O4 Gd7 O32 N12 121.5(4) 2_656 .
O5 Gd7 O32 N12 -124.7(4) 2_656 .
O21 Gd7 O32 N12 -102.06(18) . .
O13 Gd7 O32 N12 101.00(18) 2_656 .
O34 Gd7 O32 N12 -24.4(3) . .
O34' Gd7 O32 N12 -21.0(4) . .
O35' Gd7 O32 N12 29.2(3) . .
O35 Gd7 O32 N12 32.6(3) . .
O22 Gd7 O32 Gd7 -0.01(15) . 2_656
O33 Gd7 O32 Gd7 -180.0(3) . 2_656
O4 Gd7 O32 Gd7 -58.5(4) 2_656 2_656
O5 Gd7 O32 Gd7 55.3(4) 2_656 2_656
O21 Gd7 O32 Gd7 77.94(18) . 2_656
O13 Gd7 O32 Gd7 -79.00(18) 2_656 2_656
O34 Gd7 O32 Gd7 155.6(3) . 2_656
O34' Gd7 O32 Gd7 159.0(4) . 2_656
O35' Gd7 O32 Gd7 -150.8(3) . 2_656
O35 Gd7 O32 Gd7 -147.4(3) . 2_656
N12 Gd7 O32 Gd7 180.000(2) . 2_656
O32 N12 O33 Gd7 0.0(4) . .
O33 N12 O33 Gd7 -180.0(4) 2_656 .
Gd7 N12 O33 Gd7 0(5) 2_656 .
O22 Gd7 O33 N12 0.0(6) . .
O32 Gd7 O33 N12 0.0(2) . .
O4 Gd7 O33 N12 -121.5(4) 2_656 .
O5 Gd7 O33 N12 123.4(4) 2_656 .
O21 Gd7 O33 N12 70.0(4) . .
O13 Gd7 O33 N12 -69.1(4) 2_656 .
O34 Gd7 O33 N12 157.1(5) . .
O34' Gd7 O33 N12 164.8(5) . .
O35' Gd7 O33 N12 -148.5(5) . .
O35 Gd7 O33 N12 -152.7(5) . .
O22 Gd7 N13 O35 -63.7(12) . .
O32 Gd7 N13 O35 98.1(10) . .
O33 Gd7 N13 O35 103.0(10) . .
O4 Gd7 N13 O35 -42.6(9) 2_656 .
O5 Gd7 N13 O35 -112.7(10) 2_656 .
O21 Gd7 N13 O35 -176.0(9) . .
O13 Gd7 N13 O35 20.5(10) 2_656 .
O34 Gd7 N13 O35 -175.6(14) . .
O34' Gd7 N13 O35 -139.5(15) . .
O35' Gd7 N13 O35 38.1(12) . .
N12 Gd7 N13 O35 100.6(9) . .
O22 Gd7 N13 O36 158(2) . .
O32 Gd7 N13 O36 -40(3) . .
O33 Gd7 N13 O36 -35(3) . .
O4 Gd7 N13 O36 179(3) 2_656 .
O5 Gd7 N13 O36 109(3) 2_656 .
O21 Gd7 N13 O36 46(3) . .
O13 Gd7 N13 O36 -118(3) 2_656 .
O34 Gd7 N13 O36 46(3) . .
O34' Gd7 N13 O36 82(3) . .
O35' Gd7 N13 O36 -100(3) . .
O35 Gd7 N13 O36 -138(3) . .
N12 Gd7 N13 O36 -38(3) . .
O22 Gd7 N13 O34 111.9(10) . .
O32 Gd7 N13 O34 -86.3(9) . .
O33 Gd7 N13 O34 -81.4(9) . .
O4 Gd7 N13 O34 132.9(9) 2_656 .
O5 Gd7 N13 O34 62.8(9) 2_656 .
O21 Gd7 N13 O34 -0.4(9) . .
O13 Gd7 N13 O34 -164.0(9) 2_656 .
O34' Gd7 N13 O34 36.0(12) . .
O35' Gd7 N13 O34 -146.4(14) . .
O35 Gd7 N13 O34 175.6(14) . .
N12 Gd7 N13 O34 -83.9(9) . .
O35 N13 O34 Gd7 4.4(13) . .
O36 N13 O34 Gd7 -166.6(10) . .
O22 Gd7 O34 N13 -137.6(7) . .
O32 Gd7 O34 N13 109.6(8) . .
O33 Gd7 O34 N13 88.8(8) . .
O4 Gd7 O34 N13 -47.2(8) 2_656 .
O5 Gd7 O34 N13 -113.5(9) 2_656 .
O21 Gd7 O34 N13 179.6(8) . .
O13 Gd7 O34 N13 20.2(11) 2_656 .
O34' Gd7 O34 N13 -61.0(12) . .
O35' Gd7 O34 N13 18.4(7) . .
O35 Gd7 O34 N13 -2.2(7) . .
N12 Gd7 O34 N13 99.6(8) . .
O36 N13 O35 Gd7 164.2(14) . .
O34 N13 O35 Gd7 -4.3(13) . .
O22 Gd7 O35 N13 150.1(7) . .
O32 Gd7 O35 N13 -97.1(9) . .
O33 Gd7 O35 N13 -70.7(9) . .
O4 Gd7 O35 N13 132.6(10) 2_656 .
O5 Gd7 O35 N13 67.8(9) 2_656 .
O21 Gd7 O35 N13 5.3(12) . .
O13 Gd7 O35 N13 -160.0(9) 2_656 .
O34 Gd7 O35 N13 2.6(8) . .
O34' Gd7 O35 N13 22.1(8) . .
O35' Gd7 O35 N13 -84.7(15) . .
N12 Gd7 O35 N13 -83.7(9) . .
O44 N16' O43 N16 -7(7) . .
O45' N16' O43 N16 5(3) . .
O44 N16' O43 O45' -12(8) . .
O44 N16 O43 N16' 5(4) . .
O45 N16 O43 N16' -2(3) . .
O44 N16 O43 O45' 179(100) . .
O45 N16 O43 O45' 172.1(17) . .
N16' O45' O43 N16 -1.4(10) . .
O43 N16' O44 N16 7(7) . .
O45' N16' O44 N16 -4(3) . .
O43 N16' O44 O45 -176(9) . .
O45' N16' O44 O45 172.5(17) . .
O43 N16 O44 N16' -5(4) . .
O45 N16 O44 N16' 3(4) . .
O43 N16 O44 O45 -7(5) . .
N16 O45 O44 N16' -0.8(10) . .
C5 N1 C1 C2 -3.9(18) . .
Co1 N1 C1 C2 170.8(10) . .
N1 C1 C2 C3 4(2) . .
C1 C2 C3 C4 -4(2) . .
C2 C3 C4 C5 2(3) . .
C3 C4 C5 N1 -2(2) . .
C3 C4 C5 C6 -179.8(14) . .
C1 N1 C5 C4 2.4(19) . .
Co1 N1 C5 C4 -173.0(11) . .
C1 N1 C5 C6 -179.2(10) . .
Co1 N1 C5 C6 5.4(13) . .
Co1 O1 C6 C7 -171.1(15) . .
Gd1 O1 C6 C7 18(2) . .
Co1 O1 C6 C5 12.2(13) . .
Gd1 O1 C6 C5 -158.7(7) . .
C4 C5 C6 O1 167.1(13) . .
N1 C5 C6 O1 -11.3(15) . .
C4 C5 C6 C7 -10(2) . .
N1 C5 C6 C7 171.8(15) . .
O1 C6 C7 C6 8(3) . 6_575
C5 C6 C7 C6 -175.2(14) . 6_575
C12 N2 C8 C9 2(2) . .
Co1 N2 C8 C9 -177.1(13) . .
N2 C8 C9 C10 0(3) . .
C8 C9 C10 C11 -5(3) . .
C9 C10 C11 C12 7(3) . .
C8 N2 C12 C11 0.6(19) . .
Co1 N2 C12 C11 179.5(11) . .
C8 N2 C12 C13 -175.7(11) . .
Co1 N2 C12 C13 3.2(14) . .
C10 C11 C12 N2 -5(2) . .
C10 C11 C12 C13 171.3(14) . .
Co1 O2 C13 C14 165.3(9) . .
Gd4 O2 C13 C14 -8.7(17) . .
Co1 O2 C13 C12 -10.8(12) . .
Gd4 O2 C13 C12 175.2(7) . .
N2 C12 C13 O2 5.0(15) . .
C11 C12 C13 O2 -171.3(12) . .
N2 C12 C13 C14 -171.0(11) . .
C11 C12 C13 C14 12.7(19) . .
O2 C13 C14 C15 -6.0(18) . .
C12 C13 C14 C15 169.7(11) . .
Co2 O3 C15 C14 -157.2(9) . .
Gd4 O3 C15 C14 18.0(18) . .
Co2 O3 C15 C16 19.9(11) . .
Gd4 O3 C15 C16 -164.9(7) . .
C13 C14 C15 O3 1.5(19) . .
C13 C14 C15 C16 -175.3(11) . .
C20 N3 C16 C17 -1.5(17) . .
Co2 N3 C16 C17 179.9(10) . .
C20 N3 C16 C15 177.8(10) . .
Co2 N3 C16 C15 -0.8(13) . .
O3 C15 C16 N3 -12.1(14) . .
C14 C15 C16 N3 165.2(11) . .
O3 C15 C16 C17 167.3(11) . .
C14 C15 C16 C17 -15.5(17) . .
N3 C16 C17 C18 1(2) . .
C15 C16 C17 C18 -177.9(12) . .
C16 C17 C18 C19 -2(2) . .
C17 C18 C19 C20 3(2) . .
C16 N3 C20 C19 2.2(16) . .
Co2 N3 C20 C19 -179.4(8) . .
C18 C19 C20 N3 -2.8(18) . .
C25 N4 C21 C22 -3.1(16) . .
Co2 N4 C21 C22 175.7(9) . .
N4 C21 C22 C23 -1(2) . .
C21 C22 C23 C24 3(2) . .
C22 C23 C24 C25 0(2) . .
C21 N4 C25 C24 5.7(16) . .
Co2 N4 C25 C24 -173.2(10) . .
C21 N4 C25 C26 -173.3(9) . .
Co2 N4 C25 C26 7.9(12) . .
C23 C24 C25 N4 -4(2) . .
C23 C24 C25 C26 174.8(12) . .
Co2 O4 C26 C27 167.5(11) . .
Gd7 O4 C26 C27 -23.4(19) 2_656 .
Co2 O4 C26 C25 -13.4(12) . .
Gd7 O4 C26 C25 155.7(7) 2_656 .
N4 C25 C26 O4 3.5(14) . .
C24 C25 C26 O4 -175.5(11) . .
N4 C25 C26 C27 -177.4(11) . .
C24 C25 C26 C27 3.6(18) . .
O4 C26 C27 C28 1(2) . .
C25 C26 C27 C28 -178.2(11) . .
Co4 O5 C28 C27 -172.1(10) 2_656 .
Gd7 O5 C28 C27 11.1(17) 2_656 .
Co4 O5 C28 C29 11.8(12) 2_656 .
Gd7 O5 C28 C29 -165.0(7) 2_656 .
C26 C27 C28 O5 5(2) . .
C26 C27 C28 C29 -179.0(12) . .
C33 N5 C29 C30 -4.4(17) . .
Co4 N5 C29 C30 169.7(10) 2_656 .
C33 N5 C29 C28 174.4(10) . .
Co4 N5 C29 C28 -11.4(12) 2_656 .
O5 C28 C29 N5 0.1(14) . .
C27 C28 C29 N5 -176.3(11) . .
O5 C28 C29 C30 179.0(11) . .
C27 C28 C29 C30 2.5(18) . .
N5 C29 C30 C31 5(2) . .
C28 C29 C30 C31 -174.2(13) . .
C29 C30 C31 C32 -2(2) . .
C30 C31 C32 C33 -1(2) . .
C29 N5 C33 C32 1.9(17) . .
Co4 N5 C33 C32 -171.6(9) 2_656 .
C31 C32 C33 N5 1(2) . .
C38 N6 C34 C35 3(2) . .
Co3 N6 C34 C35 -174.6(12) . .
N6 C34 C35 C36 -2(2) . .
C34 C35 C36 C37 2(3) . .
C35 C36 C37 C38 -3(3) . .
C34 N6 C38 C37 -4(2) . .
Co3 N6 C38 C37 174.0(13) . .
C34 N6 C38 C39 -175.8(11) . .
Co3 N6 C38 C39 1.9(17) . .
C36 C37 C38 N6 4(3) . .
C36 C37 C38 C39 175.4(15) . .
Co3 O6 C39 C40 172.2(12) . .
Gd2 O6 C39 C40 -23.9(19) . .
Co3 O6 C39 C38 -9.9(13) . .
Gd2 O6 C39 C38 154.1(9) . .
N6 C38 C39 O6 5.2(18) . .
C37 C38 C39 O6 -166.9(15) . .
N6 C38 C39 C40 -176.7(14) . .
C37 C38 C39 C40 11(2) . .
O6 C39 C40 C39 -4(3) . 6_575
C38 C39 C40 C39 178.4(13) . 6_575
C45 N7 C41 C42 3(2) . .
Co3 N7 C41 C42 175.2(12) . .
N7 C41 C42 C43 -5(2) . .
C41 C42 C43 C44 4(3) . .
C42 C43 C44 C45 0(2) . .
C41 N7 C45 C44 0.5(19) . .
Co3 N7 C45 C44 -173.1(11) . .
C41 N7 C45 C46 176.3(11) . .
Co3 N7 C45 C46 2.7(14) . .
C43 C44 C45 N7 -2(2) . .
C43 C44 C45 C46 -177.0(14) . .
Co3 O7 C46 C47 -157.9(10) . .
Gd5 O7 C46 C47 21(2) . .
Co3 O7 C46 C45 16.0(15) . .
Gd5 O7 C46 C45 -165.2(8) . .
N7 C45 C46 O7 -12.1(17) . .
C44 C45 C46 O7 163.7(13) . .
N7 C45 C46 C47 161.9(12) . .
C44 C45 C46 C47 -22(2) . .
O7 C46 C47 C48 0(2) . .
C45 C46 C47 C48 -173.7(12) . .
Co4 O8 C48 C47 166.5(8) . .
Gd5 O8 C48 C47 -17.1(16) . .
Co4 O8 C48 C49 -10.3(11) . .
Gd5 O8 C48 C49 166.0(7) . .
C46 C47 C48 O8 -1.5(19) . .
C46 C47 C48 C49 175.1(11) . .
C53 N8 C49 C50 4.2(15) . .
Co4 N8 C49 C50 -177.3(8) . .
C53 N8 C49 C48 -175.5(9) . .
Co4 N8 C49 C48 3.0(11) . .
O8 C48 C49 N8 4.6(14) . .
C47 C48 C49 N8 -172.2(10) . .
O8 C48 C49 C50 -175.1(10) . .
C47 C48 C49 C50 8.1(17) . .
N8 C49 C50 C51 -4.7(18) . .
C48 C49 C50 C51 175.0(11) . .
C49 C50 C51 C52 1.9(19) . .
C50 C51 C52 C53 1.1(19) . .
C49 N8 C53 C52 -1.1(16) . .
Co4 N8 C53 C52 -179.4(8) . .
C51 C52 C53 N8 -1.6(18) . .
O14 Gd1 O9W O9W 98.27(16) . 6_575
O10 Gd1 O9W O9W -108.2(3) . 6_575
O10W Gd1 O9W O9W 77.75(19) 6_575 6_575
O10W Gd1 O9W O9W 99.21(15) . 6_575
O9 Gd1 O9W O9W 176.39(15) . 6_575
O9 Gd1 O9W O9W 4.11(17) 6_575 6_575
O1 Gd1 O9W O9W -122.78(18) . 6_575
O1 Gd1 O9W O9W -52.95(16) 6_575 6_575
Gd3 Gd1 O9W O9W -173.85(4) . 6_575
Gd3 Gd1 O9W O9W -10.71(10) 6_575 6_575
O14 Gd1 O10W O10W 81.12(17) . 6_575
O10 Gd1 O10W O10W 97.82(15) . 6_575
O9 Gd1 O10W O10W 158.8(2) . 6_575
O9 Gd1 O10W O10W 21.2(2) 6_575 6_575
O1 Gd1 O10W O10W -150.8(3) . 6_575
O1 Gd1 O10W O10W -42.9(4) 6_575 6_575
O9W Gd1 O10W O10W -78.66(19) 6_575 6_575
O9W Gd1 O10W O10W -97.95(13) . 6_575
Gd3 Gd1 O10W O10W 124.05(3) . 6_575
Gd3 Gd1 O10W O10W 59.80(5) 6_575 6_575
O14 Gd2 O11W O11W 83.81(12) . 6_575
O15 Gd2 O11W O11W 101.6(2) . 6_575
O6 Gd2 O11W O11W -49.1(3) . 6_575
O6 Gd2 O11W O11W -144.4(2) 6_575 6_575
O16 Gd2 O11W O11W 21.10(16) . 6_575
O16 Gd2 O11W O11W 159.28(17) 6_575 6_575
O12W Gd2 O11W O11W -96.2(3) 6_575 6_575
O12W Gd2 O11W O11W -75.23(11) . 6_575
Gd3 Gd2 O11W O11W 59.88(8) . 6_575
Gd3 Gd2 O11W O11W 127.17(4) 6_575 6_575
O14 Gd2 O12W O12W -97.93(15) . 6_575
O15 Gd2 O12W O12W 110.5(4) . 6_575
O11W Gd2 O12W O12W -98.0(3) 6_575 6_575
O11W Gd2 O12W O12W -74.41(13) . 6_575
O6 Gd2 O12W O12W 122.9(2) . 6_575
O6 Gd2 O12W O12W 53.7(2) 6_575 6_575
O16 Gd2 O12W O12W -175.0(2) . 6_575
O16 Gd2 O12W O12W -5.7(2) 6_575 6_575
Gd3 Gd2 O12W O12W 176.41(6) . 6_575
Gd3 Gd2 O12W O12W 6.42(12) 6_575 6_575
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
_platon_squeeze_void_content
1 0.000 0.000 0.010 3038 712 ' '
2 0.500 0.500 0.585 3038 712 ' '
